REVIEWS OF MODERN PHYSICS, VOLUME 89, JANUARY–MARCH 2017 Electron-phonon interactions from first principles Feliciano Giustino Department of Materials, University of Oxford, Parks Road, Oxford OX1 3PH, United Kingdom (published 16 February 2017) This article reviews the theory of electron-phonon interactions in solids from the point of view of ab initio calculations. While the electron-phonon interaction has been studied for almost a century, predictive nonempirical calculations have become feasible only during the past two decades. Today it is possible to calculate from first principles many materials properties related to the electron-phonon interaction, including the critical temperature of conventional superconductors, the carrier mobility in semiconductors, the temperature dependence of optical spectra in direct and indirect-gap semiconductors, the relaxation rates of photoexcited carriers, the electron mass renormalization in angleresolved photoelectron spectra, and the nonadiabatic corrections to phonon dispersion relations. In this article a review of the theoretical and computational framework underlying modern electronphonon calculations from first principles as well as landmark investigations of the electron-phonon interaction in real materials is given. The first part of the article summarizes the elementary theory of electron-phonon interactions and their calculations based on density-functional theory. The second part discusses a general field-theoretic formulation of the electron-phonon problem and establishes the connection with practical first-principles calculations. The third part reviews a number of recent investigations of electron-phonon interactions in the areas of vibrational spectroscopy, photoelectron spectroscopy, optical spectroscopy, transport, and superconductivity. DOI: 10.1103/RevModPhys.89.015003 CONTENTS I. Introduction II. Historical Development A. Early approaches to the electron-phonon interaction 1. Metals 2. Semiconductors 3. Ionic crystals B. The pseudopotential method C. Ab initio self-consistent field calculations III. Electron-phonon Interaction in Density-functional Theory A. Lattice vibrations in crystals B. Electron-phonon coupling Hamiltonian 1. Kohn-Sham Hamiltonian 2. Electron-phonon coupling Hamiltonian to first and second order in the atomic displacements 3. Calculation of electron-phonon matrix elements using density-functional perturbation theory 4. The dielectric approach 5. Connection with early formulations IV. Field-theoretic Approach to the Electron-phonon Interaction A. Operators and distinguishability B. Electron Green’s function 1. Equation of motion and self-energy 2. The screened Coulomb interaction 3. Nuclear contribution to the screened Coulomb interaction C. Phonon Green’s function D. Hedin-Baym equations V. From a Many-body Formalism to Practical Calculations A. Effects of the electron-phonon interaction on phonons 1. Phonons in the Born-Oppenheimer adiabatic approximation 2. Phonons beyond the adiabatic approximation 0034-6861=2017=89(1)=015003(63) 2 3 3 3 4 5 5 6 7 7 8 8 9 10 11 12 13 13 14 14 16 17 18 20 20 21 21 22 3. Expressions for the phonon self-energy used in ab initio calculations B. Effects of the electron-phonon interaction on electrons 1. Electron self-energy: Fan-Migdal and Debye-Waller terms 2. Expressions for the electron self-energy used in ab initio calculations 3. Temperature dependence of electronic band structures 4. Carrier lifetimes 5. Kinks and satellites 6. Model Hamiltonians, polarons, and the cumulant expansion VI. Efficient Calculations of Matrix Elements and Their Integrals A. Wannier interpolation 1. Maximally localized Wannier functions 2. Interpolation of electron-phonon matrix elements 3. Electron-phonon matrix elements in polar materials B. Fermi-surface harmonics VII. Nonadiabatic Vibrational Frequencies and Linewidths VIII. Electron-phonon Interactions in Photoelectron Spectroscopy A. Electron mass enhancement in metals IX. Electron-phonon Effects in the Optical Properties of Semiconductors A. Temperature dependence of band gaps and band structures 1. Perturbative calculations based on the Allen-Heine theory 2. Nonperturbative adiabatic calculations B. Phonon-assisted optical absorption X. Carrier Dynamics and Transport A. Electron linewidths and lifetimes 015003-1 23 25 25 27 28 30 31 32 32 33 33 33 34 36 36 38 41 41 41 41 44 44 45 45 © 2017 American Physical Society Feliciano Giustino: Electron-phonon interactions from first … B. Phonon-limited mobility XI. Phonon-mediated Superconductors A. McMillan–Allen-Dynes formula B. Anisotropic Migdal-Eliashberg theory C. Density-functional theory for superconductors XII. Electron-phonon Interactions Beyond the Local Density Approximation to DFT XIII. Conclusions Acknowledgments Appendix A: Born–Von Kármán Boundary Conditions Appendix B: Ladder Operators in Extended Systems References 46 47 47 48 49 50 51 52 52 52 54 I. INTRODUCTION The interaction between fermions and bosons is one of the cornerstones of many-particle physics. It is therefore not surprising that, despite being one of the most thoroughly studied chapters of solid state physics, the interaction between electrons and phonons in solids continues to attract unrelenting attention. Electron-phonon interactions (EPIs) are ubiquitous in condensed matter and materials physics. For example, they underpin the temperature dependence of the electrical resistivity in metals and the carrier mobility in semiconductors, they give rise to conventional superconductivity, and they contribute to optical absorption in indirect-gap semiconductors. In addition, EPIs enable the thermalization of hot carriers, determine the temperature dependence of electron energy bands in solids, and distort band structures and phonon dispersion relations of metals, leading to characteristic kinks and Kohn anomalies in photoemission and Raman and neutron spectra. EPIs also play a role in the areas of spintronics and quantum information, for example, by coupling lattice and spin degrees of freedom in electromagnons, or by modulating the lifetimes of electron spins in color centers. Given the fundamental and practical importance of electron-phonon interactions, it is perhaps surprising that the majority of theoretical studies in this area still rely on semiempirical model Hamiltonians, especially in times when ab initio calculations have become pervasive in every area of condensed matter and materials physics. The reason for this lag can be found in the complexity of electron-phonon calculations: while density-functional theory (DFT) calculations of total energies and structural properties were already well established in the early 1980s (Martin, 2004), systematic ab initio calculations of EPIs had to wait for the development of density-functional perturbation theory (DFPT) for lattice dynamics between the late 1980s and the mid 1990s (Baroni, Giannozzi, and Testa, 1987; Gonze, Allan, and Teter, 1992; Savrasov, 1992). Despite this delayed start, the past two decades have witnessed tremendous progress in this area, and new exciting applications are becoming accessible as first-principles techniques for studying EPIs catch up with more established DFT methods. These advances are driving the evolution from qualitative and descriptive theories of electron-phonon effects in model solids to quantitative and predictive theories of real materials. As the methodology for calculating EPIs from first Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 principles is rapidly reaching maturity, it appears that the time is ripe for reviewing this vast, complex, and fascinating landscape. One of the most authoritative reviews on the theory of EPIs is the classic book by Grimvall (1981). This monumental work represents an unmissable reference for the specialist. However, as this book predates the rise of ab initio computational methods based on DFT, it inevitably misses the most recent developments in this area. The present article constitutes an attempt at filling this gap by reflecting on what DFT calculations can contribute to the study of electron-phonon physics. In addition, this article is also an opportunity to establish a unified conceptual and mathematical framework in this incredibly diverse landscape, shed light on the key approximations, and identify some of the challenges and opportunities ahead. As emphasized by the title “Electron-phonon interactions from first principles,” the aim of this article is to review the ab initio theory of EPIs and to survey modern advances in ab initio calculations of EPIs. The reader interested in the fundamentals of electron-phonon physics or in theoretical developments relating to model Hamiltonians is referred to the outstanding monographs by Ziman (1960), Grimvall (1981), Schrieffer (1983), Mahan (1993), and Alexandrov and Devreese (2010). Among significant recent advances that are covered in this review we mention the zero-point renormalization and the temperature dependence of electronic band structures, the calculation of phonon-assisted optical absorption spectra, the electron mass renormalization and the kinks in angleresolved photoemission spectra, the thermalization of hot carriers in semiconductors, the calculation of phonon-limited mobility, the development of efficient computational techniques for calculating EPIs, and efforts to improve the predictive power of EPI calculations by going beyond standard density-functional theory. The review is organized as follows: Sec. II provides an historical perspective on the development of theories of the EPI, from early semiempirical approaches to modern firstprinciples calculations. In Sec. III we examine the various components of DFT calculations of EPIs in solids and set the formalism which will be used throughout this article. Section IV provides a synthesis of the most advanced fieldtheoretic approaches employed to study EPIs, and Sec. V makes the link between the most general formalism and DFT calculations for real materials. In this section the reader will find a number of expressions which are useful for practical implementations. Section VI reviews advanced computational techniques for performing calculations of EPIs efficiently and accurately, such as Wannier interpolation and Fermi-surface harmonics. Here we also discuss recent progress in the study of electron-phonon couplings in polar semiconductors. In Sec. VII we discuss recent calculations of phonons beyond the adiabatic Born-Oppenheimer approximation. Section VIII reviews calculations of EPIs in the context of photoelectron spectroscopy. Section IX focuses on the optical properties of semiconductors and insulators, in particular, the temperature dependence of the band structure and phonon-assisted optical processes. In Sec. X we review calculations on the effects of EPIs on carrier dynamics and transport, including carrier 015003-2 Feliciano Giustino: Electron-phonon interactions from first … thermalization rates and mobilities. Section XI discusses EPI calculations in the area of phonon-mediated superconductivity. Attempts at improving the accuracy and predictive power of ab initio EPI calculations by using more sophisticated electronic structure methods are discussed in Sec. XII. Finally in Sec. XIII we highlight the most pressing challenges in the study of EPIs from first principles, and we present our conclusions. The Appendixes give some notational remarks and more technical discussions. II. HISTORICAL DEVELOPMENT The notion of “electron-phonon interactions” is as old as the quantum theory of solids. In fact, in the very same work where Bloch (1929) discussed the formal solutions of the Schrödinger equation in periodic potentials, Sec. V begins with the all-telling title: “The interaction of the electrons and the elastic waves of the lattice.” In this work the first quantum theory of the temperature-dependent electrical resistivity of metals was developed. It took only a few years for Bloch’s “elastic waves” to be replaced by the brand-name “phonon” by Frenkel (1932), thus establishing a tradition that continues unaltered almost a century later (Walker and Slack, 1970). In order to discuss the early approaches to the electronphonon problem, it is useful to state right from the start the standard form of the Hamiltonian describing a coupled electron-phonon system: Ĥ ¼ X εnk ĉ†nk ĉnk þ nk þ N p−1=2 " þ N −1 p X ℏωqν ðâ†qν âqν þ 1=2Þ qν X gmnν ðk; qÞĉ†mkþq ĉnk ðâqν þ â†−qν Þ k;q mnν X 0 † gDW mnνν0 ðk; q; q Þĉmkþqþq0 ĉnk k;q;q0 mnνν0 × ðâqν þ â†−qν Þðâq0 ν0 # þ â†−q0 ν0 Þ : ð1Þ In this equation the first line describes the separate electron and phonon subsystems using the usual second-quantized formalism, while the second line specifies the mutual coupling between electrons and phonons to first order in the atomic displacements (Mahan, 1993). Here εnk is the single-particle eigenvalue of an electron with crystal momentum k in the band n, ωqν is the frequency of a lattice vibration with crystal momentum q in the branch ν, and ĉ†nk and ĉnk (â†qν and âqν ) are the associated fermionic (bosonic) creation and destruction operators. N p is the number of unit cells in the Born–von Kármán (BvK) supercell (see Appendix A). The third and fourth lines of Eq. (1) describe the electron-phonon coupling Hamiltonian to second order in the atomic displacements. This contribution is rarely found in the early literature (hence the square brackets), but it plays an important role in the theory of temperature-dependent band structures (Sec. V.B.1). 0 The matrix elements gmnν ðk; qÞ and gDW mnνν0 ðk; q; q Þ measure the strength of the coupling between the electron and the phonon subsystems and have physical dimensions of an Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 energy. Here the superscript “DW” stands for Debye-Waller and relates to the Debye-Waller self-energy discussed in Sec. V.B.2. Complete details as well as a derivation of Eq. (1) are provided in Sec. III. The formal simplicity of Eq. (1) conceals some important difficulties that one faces when attempting to use this equation for predictive calculations. For example, the electronic Hamiltonian relies on the assumption that the system under consideration can be described in terms of well-defined quasiparticle excitations. Similarly, the phonon term is meaningful only within the harmonic and the adiabatic approximations. More importantly, Eq. (1) does not provide us with any prescription for determining the numerical parameters 0 εnk , ωqν , gmnν ðk; qÞ, and gDW mnνν0 ðk; q; q Þ. In a sense, the history of the study of electron-phonon interactions is really the history of how to calculate the parameters entering Eq. (1) using procedures that can be at once rigorous, reliable, and practical. As will become clear in Sec. IV, despite great progress in this area, some conceptual difficulties still remain. A. Early approaches to the electron-phonon interaction 1. Metals A clear account of the theory of EPIs until the late 1950s is given by Ziman (1960). In the following we highlight only those aspects that are relevant to the subsequent discussion in this article. Early studies of electron-phonon interactions in solids were motivated by the quest for a quantum theory of the electrical resistivity in metals (Hoddeson and Baym, 1980). The common denominator of most early approaches is that the electronic excitations in Eq. (1) were described using the free electron gas model εnk ¼ ℏ2 k2 =2me − εF , with me being the electron mass and εF the Fermi energy; the lattice vibrations were described as acoustic waves using the Debye model ωqν ¼ vs jqj, where vs is the speed of sound in the solid. Both approximations were reasonable given that the systems of interest included almost exclusively elemental metals and primarily monovalent alkali and noble metals (Mott and Jones, 1936). While these approximations were fairly straightforward, it was considerably more challenging to determine the EPI matrix elements gmnν ðk; qÞ using realistic approximations. The very first expression of the electron-phonon matrix element was derived by Bloch (1929); using contemporary notation it can be written as gmnν ðk; qÞ ¼ −i ℏ 2N p Mκ ωqν 1=2 q · eκν ðqÞV 0 : ð2Þ Here M κ is the mass of the κth nucleus, and eκν ðqÞ is the polarization of the acoustic wave corresponding to the wave vector q and mode ν. The term V 0 represents a unit-cell average of the “effective” potential experienced by the electrons in the crystal. Equation (2) was meant to describe the scattering from an initial electronic state with wave vector k to a final state with wave vector k þ q, via an acoustic phonon of wave vector q and frequency ωqν. The formula was 015003-3 Feliciano Giustino: Electron-phonon interactions from first … developed for free electron metals and neglects so-called “umklapp” (folding) processes, i.e., scattering events whereby k goes into k þ q þ G with G being a reciprocal lattice vector. A derivation of Eq. (2) is provided in Sec. III.B.5. In order to determine V 0 Bloch (1929) argued that the crystal may be described as a continuous deformable medium. Starting from this assumption he reached the conclusion that the average potential can be approximated as V 0 ¼ ℏ2 =ð16me a20 Þ (a0 is the Bohr radius). Even though Bloch’s matrix element is no longer in use, this model provides helpful insight into the nature of EPIs in monovalent metals. For example the so-called “polarization factor” in Eq. (2), q · eκν ðqÞ, shows that (in the absence of umklapp processes) only longitudinal sound waves scatter electrons. Nordheim (1931) proposed a refinement of Bloch’s model whereby the average potential V 0 in Eq. (2) is replaced by the Fourier component V κ ðqÞ of the ionic Coulomb potential (see Sec. III.B.5). The key assumption underlying this model is that the effective potential experienced by the electrons is simply the sum of the individual bare ionic potentials of each nucleus. When a nucleus is displaced from its equilibrium position, the corresponding potential also shifts rigidly. This is the so-called “rigid-ion” approximation. The main difficulty that arises with the rigid-ion model is that the Fourier transform of the Coulomb potential diverges as q−2 for q ¼ jqj → 0; this leads to unrealistically strong EPIs. In order to circumvent this difficulty Mott and Jones (1936) proposed to truncate the ionic potential at the boundary of the Wigner-Seitz unit cell of the crystal. This choice represents the first attempt at including the electronic screening of the nuclear potential in a rudimentary form. In practice Mott and Jones (1936) calculated the Fourier transform of V κ ðrÞ by restricting the integration over a Wigner-Seitz cell; the resulting potential is no longer singular at long wavelengths. A detailed discussion of this model can be found in Ziman (1960). Despite some initial successes in the study of the electrical conductivity of metals, the descriptive power of these early models was undermined by the complete neglect of the electronic response to the ionic displacements. The first attempt at describing the effect of the electronic screening was made by Bardeen (1937). In his model the average potential V 0 in Eq. (2) is replaced by V 0 → V κ ðqÞ=ϵðqÞ; ð3Þ where ϵðqÞ is the Lindhard function (Mahan, 1993): ϵðqÞ ¼ 1 þ ðkTF =qÞ2 Fðq=2kF Þ: ð4Þ Here kTF and kF are the Thomas-Fermi screening wave vector and the Fermi wave vector, respectively, and FðxÞ ¼ 1=2 þ ð4xÞ−1 ð1 − x2 Þ log j1 þ xj=j1 − xj. A derivation of Bardeen’s model is provided in Sec. III.B.5. Since ϵðqÞ → ðkTF =qÞ2 for q → 0, the singularity of the electron-nuclei potential is removed in Bardeen’s matrix element. The work of Bardeen (1937) can be considered as a precursor of modern ab initio approaches, insofar as the calculation of the matrix element was carried out using a self-consistent field method Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 within the linearized Hartree theory. This strategy is similar in spirit to modern DFPT calculations. The key qualitative difference between the approach of Bardeen (1937) and modern techniques lies in the neglect of exchange and correlation effects in the screening. A possible route to overcome this limitation was proposed by Bardeen and Pines (1955). In this work they considered the role of a screened exchange interaction in the electron-phonon problem (see Appendix B of their work); however, the mathematical complexity of the formalism prevented further progress in this direction. Similar efforts were undertaken by Hone (1960), and a more detailed account of the early approximations to exchange and correlation can be found in Grimvall (1981). The most interesting aspect of the work by Bardeen and Pines (1955), as well as previous work along the same lines by Nakajima (1954), is that for the first time the electron-phonon problem was addressed using a field-theoretic approach. One interesting feature in the theory of Bardeen and Pines is that their field-theoretic formulation naturally leads to a retarded electron-phonon vertex: the effective potential experienced by electrons upon the displacement of nuclei depends on how fast this displacement takes place. In this approach the effective potential V 0 in Eq. (2) is replaced by the dynamically screened potential: V 0 → V κ ðqÞ=ϵðq; ωqν Þ: ð5Þ Here ϵðq; ωÞ is the frequency-dependent Lindhard function (Mahan, 1993), and the effect of electronic screening is evaluated at the phonon frequency ω ¼ ωqν. Somewhat surprisingly, this development was not followed up in the literature on ab initio calculations of EPIs. 2. Semiconductors While the investigation of electron-phonon effects was initially restricted to monovalent metals, the formal developments were soon extended to the case of more complex systems such as semiconductors. Carriers in semiconductors are typically confined within a narrow energy range near the band extrema; consequently it is expected that the dominant electron-phonon scattering mechanisms will involve longwavelength phonons (q → 0). This concept was formalized by Bardeen and Shockley (1950) and Shockley and Bardeen (1950), laying the foundations of the “deformation-potential” method. In the deformation-potential approach it is assumed that the atomic displacements can be described by long-wavelength acoustic waves, and these can be related in turn to the elastic strain of the crystal. Using concepts from the effective mass theory, Bardeen and Shockley showed that in this approximation the potential V 0 in Eq. (2) can be replaced by V 0 → E1;nk ¼ Ω∂εnk =∂Ω; ð6Þ where Ω represents the volume of the unit cell, and the electron eigenvalues correspond to the valence or conduction band extrema. The derivation of this result can be found in Appendix B of Bardeen and Shockley (1950). The deformation potentials E1 were obtained empirically; for example, 015003-4 Feliciano Giustino: Electron-phonon interactions from first … Bardeen and Shockley determined these values for the band extrema of silicon by fitting mobility data. More complex scenarios such as anisotropic constant-energy surfaces in semiconductors were subsequently addressed by considering the effects of shear deformations (Dumke, 1956). While the concept of deformation potentials has become a classic in semiconductor physics, this method relies on a semiempirical approach and lacks predictive power. 3. Ionic crystals A class of materials that played an important role in the development of the theory of EPIs is that of ionic crystals. The qualitative difference between ionic solids and the systems discussed in Secs. II.A.1 and II.A.2 is that the atomic displacements can generate long-ranged electric fields; these fields provide a new scattering channel for electrons and holes. The theory of polar electron-phonon coupling started with the investigation of the electron mean free path in ionic crystals in search for a theoretical model of dielectric breakdown in insulators (Fröhlich, 1937; Fröhlich and Mott, 1939). The central idea of these models is that in insulators the density of free carriers is very low; therefore it is sensible to consider a single electron interacting with the polarization field of the ionic lattice. The Fröhlich model is similar in spirit to the contemporary work of Bardeen (1937) for metals. The main difference is that Fröhlich considered the screening arising from the dielectric polarization of an insulating crystal, while Bardeen considered the screening arising from the response of the Fermi sea. Fröhlich, Pelzer, and Zienau (1950) showed that in the case of isotropic ionic crystals the effective potential V 0 appearing in Eq. (2) must be replaced by e2 Mκ ω2qν 1 1 1=2 1 − : V0 → − ϵ0 Ω ϵ∞ ϵ0 jqj2 ð7Þ In this expression e is the electron charge, ϵ0 is the dielectric permittivity of a vacuum, and ϵ0 and ϵ∞ are the static and the high-frequency relative permittivities, respectively. This result is derived in Sec. VI.A.3. Using Eqs. (2) and (7) we see that when ϵ0 > ϵ∞ the matrix element gmnν ðk; qÞ diverges as jqj−1 at long wavelengths. This singular behavior can lead to very strong EPIs and provides the physical basis for the phenomenon of electron self-trapping in polarons (Pekar, 1946; Emin, 2013). The initial studies in this area were rapidly followed by more refined approaches based on field-theoretic methods (Lee, Low, and Pines, 1953). A comprehensive discussion of the various models can be found in the original review article by Fröhlich (1954). B. The pseudopotential method The approximations underpinning the models discussed in Sec. II.A become inadequate when one tries to study EPIs for elements across the periodic table. This and other limitations stimulated the development of the pseudopotential method, starting in the late 1950s with the work of Phillips and Kleinman (1959). The theory of pseudopotentials is too vast to be summarized in a few lines, and the reader is referred to Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Chapter 11 of Martin (2004) for a thorough discussion. Here we highlight only the aspects that are relevant to the calculation of EPIs. The genesis of the pseudopotential method is linked with the question of how the valence electrons of metals could be described using the electron gas model, even though the orthogonality to the core states imposes rapid fluctuations of the valence wave functions near the atomic cores. In order to address this question, it is useful to go through the key steps of the orthogonalized plane wave method (OPW) (Herring, 1940). In this method one considers plane waves jk þ Gi for the wave vector k þ G and projects out the component belonging to the Hilbert subspace spanned by core electrons. This is done by defining jk þ GiOPW ¼ jk þ Gi − P c jϕc ihϕc jk þ Gi, where jϕc i represents the core states of all atoms in the system. The functions jk þ GiOPW are by construction orthogonal to core states, and therefore they can be used to expand the valence electron wave functions jψ nk i using only a few basis elements: jψ nk i ¼ P G ck ðGÞjk þ GiOPW . In the language of pseudopotential theory jψ nk i is referred to asPthe “all-electron” wave function, while the function jψ~ nk i ¼ G ck ðGÞjk þ Gi is referred to as the “pseudo” wave function. The all-electron and the pseudo wave functions are simply related as follows: jψ nk i ¼ T̂ jψ~ nk i; with T̂ ¼ 1 − X jϕc ihϕc j: ð8Þ c Here we used a modern notation borrowed from the projectoraugmented wave (PAW) method of Blöchl (1994). By construction, the pseudo wave function jψ~ nk i does not exhibit rapid fluctuations near the atomic cores. The projector operator T̂ is now used to rewrite the single-particle Schrödinger equation for the all-electron wave function [e.g., the Kohn-Sham (KS) equations] in terms of the pseudo wave functions. Using Ĥjψ nk i ¼ εnk jψ nk i and Eq. (8) we have T̂ † Ĥ T̂ jψ~ nk i ¼ εnk T̂ † T̂ jψ~ nk i; ð9Þ which is a generalized eigenvalue problem. By replacing the definition of T̂ given earlier one finds (Phillips and Kleinman, 1959) ðĤ þ V̂ rep Þjψ~ nk i ¼ εnk jψ~ nk i; ð10Þ P with V̂ rep ¼ c ðεnk − εc Þjϕc ihϕc j and εc the eigenvalue of a core electron. Clearly the additional potential V̂ rep is strongly repulsive and is localized near the atomic cores. Cohen and Heine (1961) showed that this extra potential largely cancels the attractive potential of the nuclei. This is the reason why valence electrons in metals behave almost like free electrons. The practical consequence of these developments is that it is possible to define smooth effective “pseudopotentials” for systematic band structure calculations, whose form factors include only a few Fourier components (Phillips, 1958; Heine and Abarenkov, 1964; Animalu and Heine, 1965; Cohen and Bergstresser, 1966). 015003-5 Feliciano Giustino: Electron-phonon interactions from first … The use of pseudopotentials in electron-phonon calculations started with the works of Sham (1961) and Sham and Ziman (1963). Sham (1961) showed that if the pseudopotential can be described by a local function, then the electronphonon matrix element gmnν ðk; qÞ can be calculated by replacing the all-electron potentials and wave functions by the corresponding pseudopotentials and pseudo wave functions. In this approach the pseudopotentials move around rigidly with the ionic cores; therefore we are dealing effectively with an improved version of the rigid-ion approximation discussed in Sec. II.A. The pseudopotential method was employed by Shuey (1965) in order to calculate the electron-phonon matrix elements in germanium. Shortly afterward many calculations of electron-phonon interactions based on the pseudopotential method appeared in the literature, including work on the resistivity of metals (Carbotte and Dynes, 1967; Dynes and Carbotte, 1968; Hayman and Carbotte, 1971; Kaveh and Wiser, 1972), the electron mass enhancement in metals (Ashcroft and Wilkins, 1965; Grimvall, 1969; Allen and Cohen, 1970, 1972; Allen, 1972a), the superconducting transition temperatures within the McMillan formalism (Allen et al., 1968; Allen and Cohen, 1969), the mobility of semiconductors (Ralph, 1970), and the temperature dependence of semiconductor band structures (Allen and Cardona, 1981, 1983). These calculations were mostly based on phonon dispersion relations extracted from neutron scattering data, and the results were in reasonable agreement with experiment. It seems fair to say that the pseudopotential method enabled the evolution from qualitative to quantitative calculations of electron-phonon interactions. Before proceeding we note that, although Eqs. (8) and (9) were introduced starting from the method of orthogonalized plane waves, there exists considerable freedom in the choice of the operator T̂ . In practice T̂ can be chosen so as to make ψ~ nk as smooth as possible, while retaining information on the all-electron wave functions near the ionic cores. This was achieved by the PAW method of Blöchl (1994). Broadly speaking it is also possible to reinterpret the historical development of the pseudopotential method as the evolution of the projector T̂ . In fact Blöchl showed how the most popular pseudopotential methods (Hamann, Schlüter, and Chiang, 1979; Bachelet, Hamann, and Schlüter, 1982; Vanderbilt, 1990; Troullier and Martins, 1991) can be derived from the PAW method under specific approximations. C. Ab initio self-consistent field calculations Predictive calculations of EPIs became possible with the development of ab initio DFT techniques. The key advantage of DFT methods is the possibility of calculating electron band structures, phonon dispersion relations, and electron-phonon matrix elements entirely from first principles. Historically, DFT started with the works of Hohenberg and Kohn (1964) and Kohn and Sham (1965). However, its widespread use had to wait for the development of accurate parametrizations of the exchange and correlation energy of the electron gas (Hedin and Lundqvist, 1971; von Barth and Hedin, 1972; Gunnarsson, Lundqvist, and Wilkins, 1974; Ceperley and Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Alder, 1980; Perdew and Zunger, 1981). An introduction to DFT techniques can be found in the books by Parr and Yang (1994) (advanced), Martin (2004) (intermediate), and Giustino (2014) (elementary). The first calculation of electron-phonon interactions using DFT was carried out by Dacorogna, Cohen, and Lam (1985) using a “frozen-phonon” approach (see Sec. III.B.3). In this work they computed electron bands, phonon dispersions, and electron-phonon matrix elements of Al entirely from first principles. Quoting from the original manuscript: “This calculation is ab initio since only information about the Al atom, i.e., the atomic number and atomic mass, is used as input.” Dacorogna et al. calculated the so-called electronphonon coupling strength λqν for several phonon branches ν and momenta q throughout the Brillouin zone, as well as the phonon linewidths arising from the EPI (see Secs. VII and XI.A). The average coupling strength was found to be in good agreement with that extracted from the superconducting transition temperature. In the approach of Chang et al. (1985), Dacorogna, Chang, and Cohen (1985), Dacorogna, Cohen, and Lam (1985), and Lam, Dacorogna, and Cohen (1986) the electron-phonon matrix element was calculated using gmnν ðk; qÞ ¼ humkþq jΔqν vKS junk iuc ; ð11Þ with unk and umkþq being the Bloch-periodic components of the Kohn-Sham electron wave functions, Δqν vKS is the phonon-induced variation of the self-consistent potential experienced by the electrons, and the integral extending over one unit cell. Equation (11) is discussed in Sec. III.B.2. The scattering potential Δqν vKS was calculated by explicitly taking into account the rearrangement of the electronic charge following a small displacement of the nuclei. The inclusion of the self-consistent response of the electrons constitutes a considerable step forward beyond the rigid-ion approximation of Sec. II.B. The next and most recent step in the evolution of electronphonon calculations came with the development of DFPT for lattice dynamics (Baroni, Giannozzi, and Testa, 1987; Gonze, Allan, and Teter, 1992; Savrasov, 1992). In contrast to frozenphonon calculations, which may require large supercells, DFPT enables the calculations of vibrational frequencies and eigenmodes at arbitrary wave vectors in the Brillouin zone. This innovation was critical in the context of electronphonon physics, since the calculation of many physical quantities requires the evaluation of nontrivial integrals over the Brillouin zone. The first calculations of EPIs using DPFT were reported by Savrasov, Savrasov, and Andersen (1994), Liu and Quong (1996), Mauri et al. (1996), and Bauer et al. (1998). They calculated the electrical resistivity, thermal conductivity, mass enhancement, and superconducting critical temperature of a number of elemental metals (e.g., Al, Au, Cu, Mo, Nb, Pb, Pd, Ta, V, and Te), and reported good agreement with experiment. By the late 1990s most of the basic ingredients required for the ab initio calculation of EPIs were available. Subsequent studies focused on using these techniques for calculating a variety of material properties and on improving the efficiency 015003-6 Feliciano Giustino: Electron-phonon interactions from first … and accuracy of the methodology. The most recent advances are reviewed in Secs. VI–XII. for the equilibrium structure. The second derivatives of the total energy with respect to the nuclear coordinates define the matrix of “interatomic force constants”: III. ELECTRON-PHONON INTERACTION IN DENSITY-FUNCTIONAL THEORY Cκαp;κ0 α0 p0 ¼ ∂ 2 U=∂τκαp ∂τκ0 α0 p0 : In this section we review the basic formalism underlying the calculation of EPIs using DFT, and we establish the link with the Hamiltonian in Eq. (1). We start by introducing the standard formalism for lattice vibrations and the electronphonon coupling Hamiltonian. Then we briefly summarize established methods of DFPT for calculating electron-phonon matrix elements. For the time being we describe electrons and phonons as separate subsystems; a rigorous theoretical framework for addressing the coupled electron-phonon system will be discussed in Sec. IV. A. Lattice vibrations in crystals U ¼ U0 þ 1X ∂ 2U Δτ Δτ 0 0 0 ; 2 καp ∂τκαp ∂τκ0 α0 p0 καp κ α p ð12Þ κ 0 α0 p0 where U 0 denotes the total energy calculated for the ions in their equilibrium positions, and the derivatives are evaluated Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 The Fourier transform of the interatomic force constants yields the “dynamical matrix” (Maradudin and Vosko, 1968): −1=2 0 Ddm κα;κ 0 α0 ðqÞ ¼ ðM κ M κ Þ X Cκα0;κ0 α0 p expðiq · Rp Þ; ð14Þ p where M κ is the mass of the κth ion. The superscript “dm” is there to distinguish this quantity from the many-body phonon propagators Dð12Þ and Dκαp;κ0 α0 p0 that will be introduced in Sec. IV.B. The dynamical matrix is Hermitian and therefore admits real eigenvalues, which we denote as ω2qν : X The formalism for studying lattice dynamics in crystals is covered in many excellent textbooks such as Born and Huang (1954), Ziman (1960), Kittel (1963, 1976), and Ashcroft and Mermin (1976). Here we introduce the notation and summarize those aspects which will be useful for subsequent discussions in this section and in Secs. IV and V. We consider M nuclei or ions in the unit cell. The position vector and Cartesian coordinates of the nucleus κ in the primitive unit cell are denoted by τ κ and τκα , respectively. We describe the infinitely extended solid using BvK boundary conditions. In this approach, periodic boundary conditions are applied to a large supercell which contains N p unit cells, identified by the direct lattice vectors Rp , with p ¼ 1; …; N p . The position of the nucleus κ belonging to the unit cell p is indicated by τ κp ¼ Rp þ τ κ. The Bloch wave vectors q are taken to define a uniform grid of N p points in one unit cell of the reciprocal lattice, and the vectors of the reciprocal lattice are indicated by G. In Appendix A we provide additional details on the notation, and we state the Fourier transforms between the direct and reciprocal lattices. Using standard DFT techniques it is possible to calculate the total potential energy of electrons and nuclei in the BvK supercell. This quantity is denoted as Uðfτ κp gÞ, where the braces are a short-hand notation for the coordinates of all the ions. The total potential energy refers to electrons in their ground state, with the nuclei being represented as classical particles clamped at the coordinates τ κp . Every DFT software package available today provides the quantity U as a standard output. In order to study lattice vibrations, one begins by making the harmonic approximation. Accordingly, the total potential energy is expanded to second order in the displacements Δτκαp of the ions in the BvK supercell away from their equilibrium positions τ 0κp : ð13Þ κ 0 α0 2 0 0 Ddm κα;κ 0 α0 ðqÞeκ α ;ν ðqÞ ¼ ωqν eκα;ν ðqÞ: ð15Þ In classical mechanics, each ωqν corresponds to the vibrational frequency of an independent harmonic oscillator. The Hermiticity of the dynamical matrix allows us to choose the eigenvectors eκα;ν ðqÞ to be orthonormal for each q: X ν eκ0 α0 ;ν ðqÞeκα;ν ðqÞ ¼ δκκ0 δαα0 ; X κα eκα;ν ðqÞeκα;ν0 ðqÞ ¼ δνν0 : ð16Þ ð17Þ Here the index ν runs from 1 to 3M. The column vectors eκα;ν ðqÞ for a given ν are called the “normal modes of vibration” or the “polarization” of the vibration wave. The following relations can be derived from Eq. (14): ω2−qν ¼ ω2qν ; eκα;ν ð−qÞ ¼ eκα;ν ðqÞ: ð18Þ These relations between normal modes carry a degree of arbitrariness in the choice of phases; here we have chosen to follow the same phase convention as Maradudin and Vosko (1968). Using Eqs. (12) and (13) the Hamiltonian for nuclei considered as quantum particles can be written as Ĥp ¼ X ℏ2 ∂ 2 1X Cκαp;κ0 α0 p0 Δτκαp Δτκ0 α0 p0 − ; 2M κ ∂τ2καp 2 καp καp ð19Þ κ0 α0 p0 where the ground-state energy U0 has been omitted and the last term is the kinetic energy operator. The Hamiltonian in Eq. (19) corresponds to the energy of an entire BvK supercell. Equation (19) relies on two approximations: (i) the harmonic approximation, which coincides with the truncation of Eq. (12) to second order in the displacements; and (ii) the Born-Oppenheimer adiabatic approximation. This latter approximation is made when one calculates the interatomic force constants with the electrons in their ground state. The scope and validity of the adiabatic approximation are 015003-7 Feliciano Giustino: Electron-phonon interactions from first … discussed in detail in Sec. V.A.1. We note incidentally that, strictly speaking, the Born-Oppenheimer approximation does not need to be invoked were one to use the generalization of DFT to multicomponent systems introduced by Kreibich and Gross (2001) and Kreibich, van Leeuwen, and Gross (2008). For practical purposes it is convenient to rewrite Eq. (19) by introducing the quanta of lattice vibrations. This is accomplished by defining the standard creation (â†qν ) and destruction (âqν ) operators for each phonon of energy ℏωqν and polarization eκα;ν ðqÞ. This operation is not entirely trivial and is described in detail in Appendix B. The formal definition of the ladder operators is given in Eqs. (B13) and (B14). These operators obey the commutation relations ½âqν ; â†q0 ν0 ¼ δνν0 δqq0 and ½âqν ; âq0 ν0 ¼ ½â†qν ; â†q0 ν0 ¼ 0, where δ is the Kronecker symbol. From these relations we know that the quanta of the harmonic oscillations in crystals obey BoseEinstein statistics. Appendix B shows that the atomic displacements can be expressed in terms of the ladder operators as follows: Δτκαp ¼ M0 N p Mκ 1=2 X eiq·Rp eκα;ν ðqÞlqν ðâqν þ â†−qν Þ; electron-phonon matrix elements gmnν ðk; qÞ are almost invariably calculated by using the KS Hamiltonian (Hohenberg and Kohn, 1964; Kohn and Sham, 1965). A justification for these choices is provided in Sec. V; for now we limit ourselves to outline the key elements of practical calculations. 1. Kohn-Sham Hamiltonian Let us denote the KS eigenfunctions by ψ nk ðrÞ and use k to indicate both the wave vector and the spin. We restrict ourselves to systems with collinear spins. The KS eigenfunctions satisfy the equation ĤKS ψ nk ðrÞ ¼ εnk ψ nk ðrÞ, with the Hamiltonian given by Ĥ KS ¼ − ℏ2 2 ∇ þ V KS ðr; fτκαp gÞ: 2me ð23Þ Here the potential V KS is the sum of the nuclear (or ionic) contribution V en , the Hartree electronic screening V H , and the exchange and correlation potential V xc (Martin, 2004): V KS ¼ V en þ V H þ V xc : ð24Þ qν ð20Þ The potentials appearing in Eq. (24) are defined as follows. The electron-nuclei potential energy is given by where lqν is the “zero-point” displacement amplitude: lqν ¼ ½ℏ=ð2M 0 ωqν Þ1=2 : ð21Þ Here M 0 is an arbitrary reference mass which is introduced to ensure that lqν has the dimensions of a length and is similar in magnitude to Δτκαp . Typically M 0 is chosen to be the proton mass. Using Eqs. (13)–(21) the nuclear Hamiltonian can be written in terms of 3MN p independent harmonic oscillators as follows: Ĥ p ¼ X qν ℏωqν ðâ†qν âqν þ 1=2Þ; V en ðr; fτκαp gÞ ¼ ð22Þ where the sum is over all wave vectors. The ground-state wave function of this Hamiltonian is a product of Gaussians, and all other states can be generated by acting on the ground state with the operators â†qν . In the case of jqj ¼ 0 there are three normal modes for which ωqν ¼ 0. For these modes, which correspond to global translations of the crystal, the zero-point displacement lqν is not defined. Throughout this article it is assumed that these modes are skipped in summations containing zero-point amplitudes. A detailed derivation of Eq. (22) and a discussion of the eigenstates of Ĥp are provided in Appendix B. V κ ðrÞ ¼ − V κ ðr − τ κp − TÞ; ð25Þ e2 Z κ ; 4πϵ0 jrj ð26Þ where Zκ is the atomic number of the nucleus κ. In the case of pseudopotential implementations V κ is a function that goes as in Eq. (26) at large jrj, but remains finite at jrj ¼ 0. Furthermore the nuclear charge is replaced by the ionic charge, which is the difference between the nuclear charge and the number of core electrons described by the pseudopotential. In all modern pseudopotential implementations V κ ðrÞ is nonlocal due to the separation of the angular momentum channels (Martin, 2004). However, since this nonlocality is short ranged and is inconsequential in the following discussion, it will be ignored here in order to maintain a light notation. The Hartree term is obtained from the electron density nðr0 ; fτκαp gÞ: B. Electron-phonon coupling Hamiltonian Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 κp;T where V κ ðrÞ is the interaction between an electron and the nucleus κ located at the center of the reference frame, and T denotes a lattice vector of the BvK supercell. In the case of allelectron DFT calculations, V κ ðrÞ is the Coulomb interaction: V H ðr; fτκαp gÞ ¼ Having outlined the standard formalism for addressing lattice vibrations in crystals, we now proceed to make the connection between DFT calculations and the remaining terms of Eq. (1). The electronic band structure εnk and X e2 X 4πϵ0 T Z nðr0 ; fτκαp gÞ 0 dr ; 0 sc jr − r − Tj ð27Þ where the integral extends over the supercell. The exchange and correlation potential is the functional derivative of the exchange and correlation energy with respect to the electron density (Kohn and Sham, 1965): 015003-8 Feliciano Giustino: Electron-phonon interactions from first … V xc ðr; fτκαp gÞ ¼ δExc ½n=δnjnðr;fτκαp gÞ : The eigenfunctions ψ nk of Ĥ following Bloch form: KS ð28Þ ð29Þ with unk a lattice-periodic function. The wave function ψ nk is taken to be normalized to one in the supercell, while the one in the crystal unit periodic part unk ðrÞ is normalized toP cell. The electron density is nðrÞ ¼ vk jψ vk ðrÞj2 , where v indicates occupied states. In order to determine ψ nk and εnk the Kohn-Sham equations are solved self-consistently. This requires one to start from a reasonable guess for the electron density (for example, a superposition of atomic electron densities), calculate the potentials in Eq. (24), and determine the solutions of the KS Hamiltonian in Eq. (23). The electron density is recalculated using these solutions, and the cycle is repeated until convergence. In order to establish the link with Eq. (1), we can regard the KS Hamiltonian as an effective one-body operator and make the transition to a second quantized formalism by using the standard prescription (Merzbacher, 1998): X nk;n0 k0 hψ nk jĤKS jψ n0 k0 iĉ†nk ĉn0 k0 ¼ X εnk ĉ†nk ĉnk : ð30Þ nk This expression is useful for performing formal manipulations in the study of coupled electron-phonon systems. However, Eq. (30) implicitly introduces the drastic approximation that the electronic system can be described in terms of sharp quasiparticle excitations. A field-theoretic approach that does not rely on any such approximation is discussed in Sec. IV. 2. Electron-phonon coupling Hamiltonian to first and second order in the atomic displacements Within the DFT Kohn-Sham formalism, the coupling Hamiltonian appearing in the second line of Eq. (1) is obtained by expanding the Kohn-Sham effective potential in terms of the nuclear displacements Δτ κp from their equilibrium positions τ 0κp . The potential to first order in the displacements is V KS ðfτ κp gÞ ¼ V KS ðfτ 0κp gÞ þ X ∂V KS καp ∂τκαp Δτκαp : ð31Þ This expression can be rewritten into normal mode coordinates using Eq. (20): V KS X ¼ V KS ðfτ 0κp gÞ þ N p−1=2 Δqν V KS ðâqν þ â†−qν Þ; X p can be expressed in the ψ nk ðrÞ ¼ N p−1=2 unk ðrÞeik·r ; Ĥe ¼ ∂ κα;q vKS ¼ e−iq·ðr−Rp Þ ∂V KS : ∂τκα r−Rp ð35Þ From the last expression we see that ∂ κα;q vKS and Δqν vKS are lattice-periodic functions. The transition to second quantization is performed as in Eq. (30) (Merzbacher, 1998): Ĥep ¼ X nk;n0 k0 hψ nk jV KS ðfτ κp gÞ − V KS ðfτ 0κp gÞjψ n0 k0 iĉ†nk ĉn0 k0 ; ð36Þ where the bra and ket indicate an integral over the supercell. After using Eqs. (29), (32)–(35), and (A1) we have Ĥep ¼ N p−1=2 X gmnν ðk; qÞĉ†mkþq ĉnk ðâqν þ â†−qν Þ; ð37Þ k;q mnν where the electron-phonon matrix element is given by gmnν ðk; qÞ ¼ humkþq jΔqν vKS junk iuc : ð38Þ Here the subscript “uc” indicates that the integral is carried out within one unit cell of the crystal. The coupling Hamiltonian in Eq. (37) yields the energy of an entire supercell. In the case of the three translational modes at jqj ¼ 0 we set the matrix elements gmnν ðk; qÞ to zero, as a consequence of the acoustic sum rule (see discussion in Sec. IX.A.1). Taken together, Eqs. (22), (30), and (37) constitute the starting point of most first-principles calculations of electronphonon interactions. It remains to be seen how one calculates the electron-phonon matrix elements gmnν ðk; qÞ; the most common procedures are described in Sec. III.B.3. Before proceeding, we briefly discuss the second-order coupling Hamiltonian which appears in the third and fourth lines of Eq. (1). The rationale for incorporating this extra term is that the expansion of the Kohn-Sham potential to first order in the atomic displacements, Eq. (31), is somewhat inconsistent with the choice of expanding the total potential energy in Eq. (12) to second order in the atomic displacements. This aspect was discussed by Allen and Heine (1976) and Allen (1978). In order to obtain an electron-phonon coupling Hamiltonian including terms of second order in the displacements, we must include the second derivatives of the KohnSham potential in Eq. (31) and follow the same steps which ð2Þ led to Eq. (37). By calling the extra term Ĥ ep we have ð2Þ Ĥep ¼ N −1 p ð32Þ X 0 † gDW mnνν0 ðk; q; q Þĉmkþqþq0 ĉnk k;q;q0 mnνν0 qν × ðâqν þ â†−qν Þðâq0 ν0 þ â†−q0 ν0 Þ; ð39Þ having defined where Δqν V KS ¼ eiq·r Δqν vKS ; Δqν v KS X ¼ lqν ðM 0 =Mκ Þ1=2 eκα;ν ðqÞ∂ κα;q vKS ; κα Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 ð33Þ ð34Þ 1 0 KS 0 0 0 gDW mnνν0 ðk; q; q Þ ¼ 2humkþqþq jΔqν Δq ν v junk iuc : The variations Δqν are the same as in Eqs. (33)–(35). 015003-9 ð40Þ Feliciano Giustino: Electron-phonon interactions from first … The second-order coupling Hamiltonian in Eq. (39) is considerably more involved than its first-order counterpart. The increased complexity partly explains why in the literature this term has largely been ignored. So far the Hamiltonian ð2Þ Ĥep has been described using only an approximation based on first-order perturbation theory (Allen and Heine, 1976). In this special case, the only terms in Eq. (39) that can modify the electron excitation spectrum are those with q0 ¼P −q. The corresponding energy shift is Δεnk ¼ −1 N p qν gDW nnνν ðk; q; −qÞð2nqν þ 1Þ, with nqν the number of phonons in each mode. We come back to this point in Sec. IX.A.1. 3. Calculation of electron-phonon matrix elements using density-functional perturbation theory In this section we review how the scattering potential Δqν vKS appearing in Eq. (38) is calculated in first-principles approaches. The most intuitive approach is to evaluate the derivatives appearing in Eq. (35) by using finite atomic displacements in a supercell: ∂V KS ≃ ½V KS ðr; τ0καp þ bÞ − V KS ðr; τ0καp Þ=b: ∂τκαp τ 0κp ð41Þ ð42Þ The variation of the ionic potential is obtained from Eqs. (25) and (35). The result is conveniently expressed in reciprocal space Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 ð43Þ where the Rconvention for the Fourier transform is fðGÞ ¼ Ω−1 uc dre−iG·r fðrÞ, and Ω is the volume of the unit cell. In order to keep the presentation as general as possible we avoid explicitly indicating the nonlocality of V κ which arises in pseudopotential implementations. The adaptation of this equation and the following ones to the case of nonlocal pseudopotentials, ultrasoft pseudopotentials, and the projector-augmented wave method can be found in Giannozzi et al. (1991), Dal Corso, Pasquarello, and Baldereschi (1997), and Audouze et al. (2006), respectively. The variation of the Hartree and exchange-correlation contributions to the KohnSham potential is obtained from the self-consistent charge density response to the perturbation in Eq. (43). After a few manipulations using Eqs. (27) and (35) one obtains ∂ κα;q vH ðGÞ ¼ ΩvC ðq þ GÞ∂ κα;q nðGÞ; ð44Þ R where vC ðqÞ ¼ Ω−1 dre−iq·r e2 =4πϵ0 jrj is the Fourier transform of the Coulomb potential. For the exchange and correlation potential we use Eq. (28) and the Taylor expansion of a functional to find ∂ κα;q vxc ðGÞ ¼ Ω In this expression b is a small displacement of the order of the zero-point amplitude (∼0.1 Å), and the atom κ in the unit cell p is displaced along the direction α. The first calculations of electron-phonon interactions within DFT employed a variant of this “supercell approach” whereby all atoms are displaced according to a chosen vibrational eigenmode (Chang et al., 1985; Dacorogna, Chang, and Cohen, 1985; Dacorogna, Cohen, and Lam, 1985; Lam, Dacorogna, and Cohen, 1986). This strategy is usually referred to as the frozen-phonon method. One disadvantage of the frozen-phonon method is that the supercell may become impractically large when evaluating matrix elements corresponding to long-wavelength phonons. This difficulty can be circumvented by using DFPT (Baroni, Giannozzi, and Testa, 1987; Gonze, Allan, and Teter, 1992; Savrasov, 1992). The main strength of DFPT is that the scattering potential Δqν vKS in Eq. (38) is obtained by performing calculations within a single unit cell. Since the computational workload of standard (not linear-scaling) DFT calculations scales as the cube of the number of electrons, the saving afforded by DFPT over the frozenphonon method is proportional to N 2p , and typically corresponds to a factor > 103. In the DFPT approach of Baroni et al. (2001) one calculates the lattice-periodic scattering potential ∂ κα;q vKS defined by Eq. (35). By differentiating Eq. (24) via Eq. (35) this potential is written as ∂ κα;q vKS ¼ ∂ κα;q ven þ ∂ κα;q vH þ ∂ κα;q vxc : ∂ κα;q ven ðGÞ ¼ −iðq þ GÞα V κ ðq þ GÞe−iðqþGÞ·τ κ ; X G0 fxc ðq þ G; q þ G0 Þ∂ κα;q nðG0 Þ; ð45Þ where f xc indicates the standard exchange and correlation kernel, which is the second-order functional derivative of the exchange and correlation energy Exc with respect to the electron density (Hohenberg and Kohn, 1964) δ2 Exc ½n f ðr; r Þ ¼ : δnðrÞδnðr0 Þnðr;fτ 0κp gÞ xc 0 ð46Þ In the case of the local density approximation (LDA) to DFT, the exchange and correlation kernel reduces to a local function (Parr and Yang, 1994), and Eq. (45) is more conveniently evaluated in real space. Today DFPT calculations can be performed using one of several exchange and correlation kernels. The effect of the kernel on the calculation of latticedynamical properties of solids has been analyzed in several works; see, for example, Dal Corso (2013) and He et al. (2014). The formal structure of the DFPT equations discussed in this section remains unchanged if we replace the DFT kernel in Eq. (46) by more sophisticated versions. For example, both DFPT calculations based on Hubbard-corrected DFT (Floris et al., 2011) and DFPT coupled with dynamical mean-field theory (Savrasov and Kotliar, 2003) have been demonstrated. It should be noted that in Eqs. (45) and (46) we are implicitly assuming a spin-unpolarized system. The adaptation of these equations as well as the other DFPT equations to the most general case of noncollinear spin systems can be found in Dal Corso (2007, 2008) and Verstraete et al. (2008). From Eqs. (44) and (45) we see that the evaluation of gmnν ðk; qÞ goes through the calculation of the variation of the electron density induced by the perturbation ∂ κα;q vKS ðrÞeiq·r . Within DFPT such a variation is obtained by evaluating the 015003-10 Feliciano Giustino: Electron-phonon interactions from first … change of the Kohn-Sham wave functions to first order in perturbation theory. After inspection of the perturbed Hamiltonian it becomes evident that the wave function change must be of the form ∂unk;q eiq·r , with ∂unk;q a lattice-periodic function. Using this observation the first-order variation of the Kohn-Sham equations can be written as a Sternheimer equation (Sternheimer, 1954) KS ðĤ KS kþq − εvk Þ∂uvk;q ¼ −∂ κα;q v uvk ; ð47Þ −iðkþqÞ·r KS iðkþqÞ·r Ĥ e . In this equation the where ĤKS kþq ¼ e index v indicates an occupied state. For jqj ¼ 0 one needs also to consider a shift of the energy eigenvalues which introduces an additional term huvk j∂ κα;0 vjuvk iuc uvk on the right-hand side of Eq. (47). In practice this term is canceled by the use of the projectors described in Eq. (48), unless one is dealing with metallic systems. This aspect is discussed in detail by de Gironcoli (1995) and Baroni et al. (2001). The principal advantage of Eq. (47) over standard perturbation theory is that it does not involve unoccupied electronic states. A practical problem arises when attempting to solve Eq. (47): the linear system on the left-hand side is ill conditioned owing to small eigenvalues corresponding to εvk ≃ εv0 kþq ; furthermore, in the case of accidental degeneracies εvk ¼ εv0 kþq , the system becomes singular. In order to make the system nonsingular, Giannozzi et al. (1991) noted that the variation of the electron density involves only the component of ∂uvk;q belonging to the unoccupied manifold of Kohn-Sham states. As a consequence, what is really needed where P̂occ is only ∂ u~ vk;q ¼ ð1 − P̂occ kþq Þ∂uvk;q, kþq ¼ P ju ihu j is the projector over the occupied states vkþq v vkþq with wave vector k þ q. The equation for this “trimmed” wave function variation is simply obtained by projecting both occ sides of Eq. (47) onto ð1 − P̂occ kþq Þ and noting that P̂kþq and ĤKS kþq do commute KS ~ vk;q ¼ −ð1 − P̂occ ðĤKS kþq Þ∂ κα;q v uvk : kþq − εvk Þ∂ u ð48Þ At this point it is possible to remove all small or null eigenvalues of the operator on the left-hand side by adding a term αP̂occ kþq to the Hamiltonian. This term has no effect on ~ vk;q ¼ 0 by conthe wave function variation, since P̂occ kþq ∂ u struction. The operator is made nonsingular by choosing the parameter α larger than the valence bandwidth (Baroni et al., 2001). From the wave function variation obtained by solving Eq. (48), it is now possible to construct the following density response associated with the wave vector q: ∂nκα;q ðrÞ ¼ 2N −1 p X uvk ∂ u~ vk;q : ð49Þ vk For simplicity a spin-degenerate system has been assumed (a factor of 2 is implicitly included in the sum over k), and time-reversal symmetry has been used in order to make the expression more compact (yielding the factor of 2 on the righthand side). In practical DFPT calculations, Eq. (48) is solved using an iterative procedure which is similar to standard DFT total Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 energy calculations. One sets the starting perturbation ∂ κα;q vKS to be equal to the electron-nuclei potential in Eq. (43). By solving Eq. (48) for each occupied state v and each wave vector k using standard linear algebra techniques, one obtains the induced density in Eq. (49). The new density is now used to construct the variations of the Hartree and exchange-correlation potentials in Eqs. (44) and (45). These induced potentials are added to the electronnuclei potential, yielding a “screened” perturbation ∂ κα;q vKS in Eq. (48). The cycle is repeated until the change of ∂nκα;q between two successive cycles is smaller than a set tolerance. It can be shown that the screened perturbation ∂ κα;q vKS described in this section is also the key ingredient required for calculating the interatomic force constants in Eq. (13) (Baroni et al., 2001). As a practical consequence, every software implementation that supports DFPT calculations already contains all the information necessary for evaluating the electron-phonon matrix elements gmnν ðk; qÞ. All the quantities introduced in this section can equivalently be calculated using an alternative, variational formulation of density-functional perturbation theory (Gonze, Allan, and Teter, 1992; Gonze, 1995a, 1997; Gonze and Lee, 1997). A thorough discussion of the connection between the Sternheimer approach and the variational approach to DFPT is provided by Gonze (1995b). 0 The second-order matrix elements gDW mn;νν0 ðk; q; q Þ given by Eq. (40) involve the second derivative of the KohnSham potential with respect to the nuclear displacements. The evaluation of these quantities requires the solution of second-order Sternheimer equations for the second variations of the Kohn-Sham wave functions. The general structure of second-order Sternheimer equations can be found in Sec. IV.H of Gonze (1995b). Since these calculations are rather involved, most practical implementations employ an approximation whereby the Debye-Waller matrix elements are expressed in terms of products of the standard matrix elements gmnν ðk; qÞ. Such an alternative formulation was developed by Allen and Heine (1976) and Allen and Cardona (1981) and is discussed in Sec. IX.A.1. All recent ab initio calculations of electron-phonon interactions based on DFPT employed this latter approach.1 4. The dielectric approach Besides the DFPT method described in the previous section, it is also possible to calculate the screened perturbation ∂ κα;q vKS using the so-called “dielectric approach” (Pick, Cohen, and Martin, 1970; Quong and Klein, 1992). This latter approach did not find as widespread an application as those of Baroni, Giannozzi, and Testa (1987), Gonze, Allan, and Teter (1992), and Savrasov (1992), but it is useful to establish a link between DFT calculations of electron-phonon matrix elements and the field-theoretic formulation discussed in Sec. IV. 1 See, for example, Marini (2008), Giustino, Louie, and Cohen (2010), Gonze, Boulanger, and Côté (2011), Cannuccia and Marini (2013), Antonius et al. (2014), Kawai et al. (2014), Poncé, Antonius, Boulanger et al. (2014), Poncé, Antonius, Gillet et al. (2014), and Poncé et al. (2015). 015003-11 Feliciano Giustino: Electron-phonon interactions from first … For consistency with Sec. III.B.3, we derive the key expressions of the dielectric approach starting from DFPT. To this aim we expand the variation of the wave function ∂ u~ vk;q using the complete set of states unkþq (with n referring to both occupied and empty Kohn-Sham states). Then we replace this expansion inside Eq. (48), project onto an arbitrary conduction state, and insert the result into Eq. (49). After taking into account time-reversal symmetry, these steps lead to the following result: Z ∂ κα;q nðrÞ ¼ uc dr0 χ 0q ðr; r0 Þ∂ κα;q vKS ðr0 Þ; ð50Þ having defined χ 0q ðr; r0 Þ ¼ N −1 p X fnk − fmkþq mnk εnk − εmkþq × unk ðrÞumkþq ðrÞumkþq ðr0 Þunk ðr0 Þ: ð51Þ In this expression f nk and fmkþq are the occupations of each state, and the indices run over all bands. A factor of 2 for the spin degeneracy is implicitly included in the sum over k. The quantity χ 0q in Eq. (51) is the lattice-periodic component for the wave vector q of the “independent-electron polarizability” (Adler, 1962; Wiser, 1963; Pick, Cohen, and Martin, 1970; Quong and Klein, 1992). For ease of notation we write Eq. (50) in symbolic form as ∂n ¼ χ 0 ∂vKS . Using the same symbolic notation it is also possible to formally rewrite Eqs. (42), (44), and (45) as follows: ∂vKS ¼ ∂ven þ ðvC þ fxc Þχ 0 ∂vKS ; ð52Þ from which one obtains ∂vKS ¼ ðϵHxc Þ−1 ∂ven ; ð53Þ having defined the dielectric matrix ϵHxc ¼ 1 − ðvC þ fxc Þχ 0 : ð54Þ The superscript “Hxc” refers to the Hartree and exchange and correlation components of the screening. In the language of many-body perturbation theory ϵHxc is referred to as the “test electron” dielectric matrix, hinting at the fact that the electron density redistribution in response to a perturbation arises both from classical electrostatics (the Hartree term vC χ 0 ) and from quantum effects (the exchange and correlation terms fxc χ 0 ). If we neglect the kernel fxc in this expression, then we obtain the “test charge” dielectric matrix, which is most commonly known as the dielectric matrix in the random-phase approximation (RPA) (Pines and Bohm, 1952) ϵH ¼ 1 − vC χ 0 : ð55Þ The symbolic expressions outlined here remain almost unchanged when using a reciprocal space representation. As an example, Eq. (55) becomes simply Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 2 0 ϵH GG0 ðqÞ ¼ δGG − Ω X χ 0G00 G0 ðqÞvC ðq þ GÞδGG00 : ð56Þ G00 Taken together Eqs. (38) and (53) show that the calculation of electron-phonon matrix elements using DFPT is equivalent to screening the bare electron-nucleus interaction using ϵHxc . In this case we say that the screening is described at the “RPA þ xc” level of approximation. At this point it is worth pointing out that so far we considered only the screening of static perturbations: in fact ∂ven was implicitly taken to be frequency independent. Physically this choice corresponds to describing phonons as quasistatic perturbations, so that at each set of instantaneous atomic positions during a vibration cycle, the electrons have enough time to readjust and reach their ground state. This is a statement of the adiabatic approximation (Born and Oppenheimer, 1927). The importance of retardation effects in the electron-phonon problem was already recognized in the early work of Bardeen and Pines (1955), but the first ab initio calculations of these effects appeared much later [see Lazzeri and Mauri (2006)]. The formal framework required to incorporate retardation in the study of EPIs is presented in Sec. IV. 5. Connection with early formulations For completeness, we illustrate the link between electronphonon matrix elements obtained within DFPT (Sec. III.B.3) and the early approaches of Bloch (1929) and Bardeen (1937) (Sec. II.A). The Bloch matrix element can be derived as follows. We assume that the scattering potential is unscreened and corresponds to the bare pseudopotentials V κ in Eq. (43), that there is only one atom at the origin of the unit cell, and the Kohn-Sham wave functions can be described by free electrons unk ðrÞ ¼ Ω−1=2 expðiGn · rÞ. In the last expression, the subscript in Gn is used in order to stress the one-to-one correspondence between the reciprocal lattice vectors and the energy bands of the free electron gas in the reduced-zone scheme. Using these approximations in Eqs. (21), (34), (38), and (43), we find gmnν ðk; qÞ ¼ −i½ℏ=ð2N p M κ ωqν Þ1=2 V κ ðq þ Gm − Gn Þ × ðq þ Gm − Gn Þ · eκ;ν ðqÞ: ð57Þ By further neglecting umklapp processes (Gm ≠ Gn ) the previous result becomes (Grimvall, 1981, Sec. 3.4) gmnν ðk; qÞ ¼ −i½ℏ=ð2N p M κ ωqν Þ1=2 q · eκ;ν ðqÞV κ ðqÞ: ð58Þ The expression obtained by Bloch (1929) and reproduced in Eq. (2) is simply obtained by replacing V κ ðqÞ with the effective potential V 0 . The Bardeen matrix element is more elaborate and can be derived as follows. We describe the screening of the bare ionic potential within the RPA approximation and determine the dielectric matrix by replacing the Kohn-Sham wave functions by free electrons. Using unk ðrÞ ¼ Ω−1=2 expðiGn · rÞ and 015003-12 Feliciano Giustino: Electron-phonon interactions from first … εnk ¼ ℏ2 ðk þ Gn Þ2 =2me − εF in Eq. (51), the polarizability reduces to χ 0GG0 ðqÞ ¼ − me kF Fðjq þ Gj=2kF ÞδGG0 ; π 2 ℏ2 Ω ð59Þ where F is the function defined below Eq. (4). The derivation of this result requires making the transition from the first Brillouin zone to the extended-zone scheme. If we use Eq. (59) inside Eq. (56), neglect the exchange and correlation kernel and use the Fourier transform of the Coulomb potential, we find ϵGG0 ðqÞ ¼ δGG0 ½1 þ ðk2TF =jq þ Gj2 ÞFðjq þ Gj=2kF Þ; ð60Þ where the Thomas-Fermi screening length is given by kTF ¼ ½4me2 kF =ð4πε0 πℏ2 Þ1=2 . Equation (60) is the wellknown Lindhard dielectric matrix, and the diagonal matrix elements are the same as in Eq. (4) [see Mahan (1993) and Giuliani and Vignale (2005) for in-depth discussions of the Lindhard function]. By following the same steps that led to Eq. (58), replacing the bare ionic potential by its screened counterpart, and using Eq. (53) with ϵ instead of ϵHxc , we obtain gmnν ðk; qÞ ¼ −i½ℏ=ð2N p M κ ωqν Þ1=2 q · eκ;ν ðqÞV κ ðqÞ=ϵðqÞ: ð61Þ Here we considered only one atom at the center of the unit cell, and we neglected umklapp processes. This is essentially the result derived by Bardeen (1937) and reproduced in Eq. (3). IV. FIELD-THEORETIC APPROACH TO THE ELECTRON-PHONON INTERACTION In Sec. III we discussed how the material parameters entering the electron-phonon Hamiltonian in Eq. (1), namely, εnk , ωqν , and gmnν ðk; qÞ can be calculated from first principles using DFT and DFPT. Today the formalism and techniques described in Sec. III constitute de facto the standard tool in quantitative studies of electron-phonon interactions in solids (see Secs. VII–XII). However, note that the DFT approach to EPIs does not rest on strong theoretical foundations. For one, the evaluation of the EPI matrix elements via Eq. (38) relies on the assumption that the interaction between electrons and nuclei is governed by the effective Kohn-Sham potential. Therefore we can expect the matrix elements to be sensitive to the exchange and correlation functional (see Sec. XII). Furthermore, the very definition of phonons starting from Eq. (12) relies on the Born-Oppenheimer approximation, and one might ask whether this choice is accurate enough in metals and narrowgap semiconductors (see Sec. VII). Finally, if one were to go beyond the Born-Oppenheimer approximation, then it would seem sensible to also incorporate retardation effects in the calculation of the EPI matrix elements. On top of these practical points, and at a more fundamental level, we expect that the electron-phonon interaction will Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 modify both the electronic structure and the lattice dynamics of a solid, and these modifications will in turn affect the coupling between electrons and phonons. It is therefore clear that a complete theory of interacting electrons and phonons must be self-consistent. In order to address these issues it is necessary to formulate the electron-phonon problem using a rigorous and general theory of interacting electrons and phonons in solids. The most systematic and elegant approach is based on quantum field theory (Schwinger, 1951) and is tightly connected to the development of the GW method (Hedin, 1965). The first attempts in this direction were from Nakajima (1954), Bardeen and Pines (1955), Migdal (1958), and Engelsberg and Schrieffer (1963). However, from the point of view of the present article, these works are of limited usefulness since they were mostly developed around the homogeneous electron gas. A completely general formulation of the problem, which seamlessly applies to metals, semiconductors, and insulators, was first provided by Baym (1961) and subsequently by Hedin and Lundqvist (1969). The formalism developed in these articles constitutes today the most complete theory of the electron-phonon problem. In fact, many aspects of this formalism are yet to be explored within the context of ab initio calculations. After these seminal works several others contributed to clarifying various aspects of the many-body theory of the coupled electron-phonon system, including Sjölander and Johnson (1965), Keating (1968), Gillis (1970), Maksimov (1976), and Vogl (1976), and more recently van Leeuwen (2004) and Marini, Poncé, and Gonze (2015). In particular, van Leeuwen focused on the issues of translational and rotational invariance of the resulting theory, while Marini et al. analyzed the connection between many-body perturbation theory approaches and DFT calculations. Since the mathematical notation of the original articles is obsolete and rather difficult to follow, in Secs. IV.A–IV.D we cover the theory in some detail using contemporary notation. The following derivations can be found across the works of Kato, Kobayashi, and Namiki (1960), Baym (1961), Hedin and Lundqvist (1969), and Maksimov (1976). Here we provide a synthesis of these contributions using a unified notation, and we fill the gaps wherever it is necessary. The presentation requires some familiarity with field operators [see, for example, Merzbacher (1998) for a succinct introduction]. A. Operators and distinguishability The starting point for studying EPIs using a field-theoretic approach is to define the Fock space and the field operators for electrons and nuclei. In the case of electrons the choice is unambiguous, since any many-body state can be represented as a linear combination of Slater determinants constructed using a basis of single-particle wave functions. In the case of nuclei the situation is slightly more ambiguous: in principle we might proceed in a very general way by choosing to focus on the nuclei as our quantum particles, as opposed to their displacements from equilibrium. In practice this choice leads to a dead end for two reasons. First, the quantum statistics of nuclei would be dependent on their spin, and therefore we 015003-13 Feliciano Giustino: Electron-phonon interactions from first … would end up with an unwieldy mix of fermions and bosons depending on the solid. Second, the notion of indistinguishable particles, which is central to second quantization, does not apply to nuclei in solids (at least in thermodynamic equilibrium and far from a solid-liquid phase transition). In fact, in many cases we can directly label the nuclei, for example, by means of experimental probes such as scanning tunneling microscopy and electron diffraction. In order to avoid these issues, it is best to study the electron-phonon problem by considering (i) indistinguishable electrons, for which it is convenient to use second-quantized operators; (ii) distinguishable nuclei, for which it is best to use first quantization in the displacements; and (iii) indistinguishable phonons, resulting from the quantization of the nuclear displacements. In this latter case the distinction between first and second quantization is irrelevant. These aspects are briefly mentioned by Baym (1961) and Maksimov (1976). With these choices, the dynamical variables of the problem are the electronic field operators ψ̂ (discussed later) and the nuclear displacements from equilibrium Δτ̂ (discussed in Sec. IV.C). In this theory the equilibrium coordinates of the nuclei are regarded as external parameters and are to be obtained, for example, from crystallography or DFT calculations. Throughout this section, we limit ourselves to consider equilibrium Green’s functions at zero temperature. As a result, all expectation values will be evaluated for the electronnuclei ground state j0i. The extension of the main results to finite temperature is presented in Sec. V. We do not specify how to obtain the ground state, since the following discussion is independent of the precise shape of this state. In order to derive expressions that are useful for first-principles calculations, at the very end the ground state will be approximated using standard DFT wave functions and phonons (see Sec. V). The electronic field creation and destruction operators are denoted by ψ̂ † ðxÞ and ψ̂ðxÞ, where the variable x indicates both the position r and the spin label σ. These operators obey the anticommutation relations (Merzbacher, 1998) fψ̂ðxÞ; ψ̂ðx0 Þg ¼ fψ̂ † ðxÞ; ψ̂ † ðx0 Þg ¼ 0 and fψ̂ðxÞ; ψ̂ † ðx0 Þg ¼ δðx − x0 Þ. The most general nonrelativistic Hamiltonian for a system of coupled electrons and nuclei can be written as Ĥ ¼ T̂ e þ T̂ n þ Û ee þ Ûnn þ Û en ; In Eqs. (63) and (64) the integrals are over the entire crystal. This corresponds to considering a supercell of infinite size (therefore the lattice vectors T of the supercell drop out) and a dense sampling of wave vectors q in the Brillouin zone. This choice is useful in order to maintain the formalism as light as possible. Accordingly, all sums over q are replaced using R P −1 N −1 → Ω dq, where the integral is over the Brillouin p q BZ the closure relations in zone of volume ΩBZ . Similarly R Eq. (A1) are replaced by dq expðiq · Rp Þ ¼ ΩBZ δp0 and P p expðiq · Rp Þ ¼ ΩBZ δðqÞ. The nuclear kinetic energy operator is the same as the last term in Eq. (19). Using the same notation as in Sec. III the nucleus-nucleus interaction energy is Û nn ¼ 1 X Z Z 0 vðτ 0κp þ Δτ̂ κp ; τ 0κ0 p0 þ Δτ̂ κ0 p0 Þ: 2 κ0 p0 ≠κp κ κ ð65Þ Here τ 0κp denotes the classical equilibrium position of each nucleus, and the displacement operators Δτ̂ κp will later be expressed in terms of the ladder operators from Appendix B. The electron-nucleus interaction energy is Z Û en ¼ Z dr dr0 n̂e ðrÞn̂n ðr0 Þvðr; r0 Þ; ð66Þ where the nuclear charge density operator is given by n̂n ðrÞ ¼ − X κp Zκ δðr − τ 0κp − Δτ̂ κp Þ: ð67Þ Here the density operators are expressed in units of the electron charge, so that the expectation value of the total charge density is −eh0jn̂ðrÞj0i with n̂ðrÞ ¼ n̂e ðrÞ þ n̂n ðrÞ. We underline the asymmetry between Eqs. (64) and (65): in the case of electrons one considers the electrostatic energy of a continuous distribution of charge, and the unphysical self-interaction is removed by the Dirac delta. Whereas in the case of nuclei, the particles are distinguishable and therefore one has to take into account all pairwise interactions individually. ð62Þ B. Electron Green’s function where each term is introduced hereafter. The electron kinetic energy is T̂ e ¼ − ℏ2 2me Z dxψ̂ † ðxÞ∇2 ψ̂ðxÞ; ð63Þ R the with me the electron mass, and the integrals dx denoting P R sum over spin and the integration over space σ dr. The electron-electron interaction is Û ee ¼ 1 2 Z Z dr dr0 n̂e ðrÞ½n̂e ðr0 Þ − δðr − r0 Þvðr; r0 Þ; ð64Þ 1. Equation of motion and self-energy In this section we focus on the electrons. By combining Eqs. (62)–(66) and using the anticommutation relations for the field operators one finds the following standard expression: Z ℏ2 2 Ĥ ¼ T̂ n þ Û nn þ dxψ̂ † ðxÞ − ∇ þ V̂ n ðrÞ ψ̂ðxÞ 2me Z 1 dxdx0 vðr; r0 Þψ̂ † ðxÞψ̂ † ðx0 Þψ̂ðx0 Þψ̂ðxÞ; ð68Þ þ 2 where the nuclear potential V̂ n is given by where the P electron particle density operator is given by n̂e ðrÞ ¼ σ ψ̂ † ðxÞψ̂ðxÞ, and vðr; r0 Þ ¼ e2 =ð4πε0 jr − r0 jÞ is the Coulomb interaction between two particles of charge e. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 015003-14 Z V̂ n ðrÞ ¼ dr0 vðr; r0 Þn̂n ðr0 Þ: ð69Þ Feliciano Giustino: Electron-phonon interactions from first … In order to study the excitation spectrum of the many-body Hamiltonian Ĥ at equilibrium we need to determine the timeordered one-electron Green’s function (Kato, Kobayashi, and Namiki, 1960; Fetter and Walecka, 2003). At zero temperature this function is defined as i Gðxt; x0 t0 Þ ¼ − h0jT̂ψðxtÞψ † ðx0 t0 Þj0i; ℏ ð70Þ where T̂ is Wick’s time-ordering operator for fermions and ensures that the times of the subsequent operators increase toward the left. The formal definition of the Wick operator is T̂ψðxtÞψ † ðx0 t0 Þ ¼ θðt − t0 ÞψðxtÞψ † ðx0 t0 Þ − θðt0 − tÞψ † ðx0 t0 Þ ψðxtÞ, where θ is the Heaviside function. Based on this definition we see that for t > t0 the Green’s function in Eq. (70) corresponds to the scalar product between the initial state ψ † ðx0 t0 Þj0i and the final state ψ † ðxtÞj0i. This product is precisely the probability amplitude for finding an electron in the position x at the time t, after having introduced an electron in x0 at an earlier time t0 . In the case t < t0 the situation is reversed and the Green’s function describes the propagation of a hole created in the system at the time t. In order to determine Gðxt; x0 t0 Þ we need to establish an equation of motion for the field operators. This can be done by describing the time dependence of the operators within the Heisenberg picture: ψ̂ðxtÞ ¼ eitĤ=ℏ ψ̂ðxÞe−itĤ=ℏ ; ð71Þ where Ĥ was defined in Eq. (68). From this definition it follows immediately that ∂ iℏ ψ̂ðxtÞ ¼ ½ψ̂ðxtÞ; Ĥ: ∂t ð72Þ By combining Eqs. (68) and (72) and using the anticommutation relations for the field operators one obtains iℏ Z ∂ ℏ2 2 ψ̂ðxtÞ ¼ − ∇ þ dr0 vðr; r0 Þn̂ðr0 tÞ ψ̂ðxtÞ; 2me ∂t ð73Þ 0 where the time dependence in n̂ðr tÞ is to be understood in the Heisenberg sense, as in Eq. (71). This equation of motion allows us to write the corresponding equation for the electron Green’s function in Eq. (70): ∂ ℏ2 2 þ ∇ − φðrtÞ Gðxt; x0 t0 Þ ∂t 2me Z i dr00 dt00 vðrt; r00 t00 Þ ¼ δðxt; x0 t0 Þ − ℏ ð75Þ In this and the following expressions δ=δφðr00 t00 Þ denotes the functional derivative with respect to φðr00 t00 Þ and should not be confused with the Dirac delta functions δðxt; x0 t0 Þ. Equation (75) is proven by Kato, Kobayashi, and Namiki (1960), Appendix II, and by Hedin and Lundqvist (1969), Appendix B.a. After identifying â and b̂ with ψ̂ðxtÞ and ψ̂ † ðx0 t0 Þ, respectively, Eq. (74) becomes Z ∂ ℏ2 2 þ ∇ − V tot ðrtÞ − iℏ dr00 dt00 vðrt þ η; r00 t00 Þ ∂t 2me δ Gðxt; x0 t0 Þ ¼ δðxt; x0 t0 Þ; ð76Þ × δφðr00 t00 Þ iℏ Z ð74Þ Here vðrt; r00 t00 Þ ¼ vðr; r00 Þδðt − t00 Þ, the bra and ket h i are a short-hand notation for h0j j0i, and the additional term φ is discussed later. In order to obtain Eq. (74) we used once again the anticommutation relations, and we noted that the derivative of the Heaviside function is a Dirac delta. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 δhT̂ âðt1 Þb̂ðt2 Þi i ¼ − hT̂½n̂ðr00 t00 Þ − hn̂ðr00 t00 Þiâðt1 Þb̂ðt2 Þi: δφðr00 t00 Þ ℏ where η is a positive infinitesimal arising from the time ordering, and V tot ðrtÞ is the total potential acting on the electronic and nuclear charges, averaged over the many-body quantum state j0i iℏ × hT̂ n̂ðr00 t00 ÞψðxtÞψ † ðx0 t0 Þi: The new term φðrtÞ which appeared in Eq. (74) is a scalar electric potential which couples to both electronic and nuclear charges. This potential has been introduced in order to Rperturb the system via the additional Hamiltonian Ĥ1 ðtÞ ¼ drn̂ðrtÞφðrtÞ. The physical idea behind this choice is to use φðrtÞ in order to induce forced oscillations in the system. When the system resonates with the perturbation we know that the resonant frequency must correspond to a free oscillation, i.e., a many-body eigenmode. From a formal point of view, the potential φðrtÞ is introduced in order to exploit Schwinger’s functional derivative technique (Kato, Kobayashi, and Namiki, 1960, Appendix II) and is set to zero at the end of the derivation. One complication arising from the introduction of φðrtÞ in Eq. (74) is that the time evolution in Eq. (71) is no longer valid, since the perturbed Hamiltonian now depends on the time variable. The way around this complication is to switch from the Heisenberg picture to the interaction picture. This change amounts to replacing the exponentials in Eq. (71) by the time-ordered Dyson series ÛðtÞ ¼ R T̂ exp ½−iℏ−1 0t Ĥðt0 Þdt0 (Fetter and Walecka, 2003). Since this would lead to an overlong derivation, we prefer to leave this aspect aside and refer the interested reader to Aryasetiawan and Gunnarsson (1998) for a more comprehensive discussion. In order to write Eq. (74) in a manageable form, we use the identity (Kato, Kobayashi, and Namiki, 1960) V tot ðrtÞ ¼ dr0 vðr; r0 Þhn̂ðr0 tÞi þ φðrtÞ: ð77Þ Equation (76) was first derived by Kato, Kobayashi, and Namiki (1960). In order to avoid a proliferation of variables, it is common practice to replace the letters by integer numbers, using the convention ðxtÞ or ðrtÞ → 1, ðx0 t0 Þ or ðr0 t0 Þ → 2, 015003-15 Feliciano Giustino: Electron-phonon interactions from first … Z ðrt þ ηÞ → 1þ , and so on. Using this convention the last two equations become ∂ ℏ2 2 iℏ þ ∇ ð1Þ − V tot ð1Þ−iℏ ∂t1 2me Z d3vð1þ 3Þ δ Gð12Þ δφð3Þ ¼ δð12Þ ð78Þ dð34ÞGð13ÞΓð324ÞWð41þ Þ; Σð12Þ ¼ iℏ ð85Þ which in turn contains the “screened Coulomb interaction” W defined as Z Wð12Þ ¼ Z −1 d3ϵ ð13Þvð32Þ ¼ dð3Þvð13Þϵ−1 ð23Þ: ð86Þ and Z V tot ð1Þ ¼ d2vð12Þhn̂ð2Þi þ φð1Þ: ð79Þ In these expressions the spin labels are implied for the Green’s function and for the Dirac delta. At this point, a set of self-consistent equations for coupled electrons and phonons can be generated by eliminating the functional derivative in Eq. (78). For this purpose one first relates the total screened electrostatic potential V tot to the external potential φ by introducing the inverse dielectric matrix ϵ−1 as a functional derivative: ϵ−1 ð12Þ ¼ δV tot ð1Þ=δφð2Þ: ð80Þ The function ϵ−1 ð12Þ is the many-body counterpart of the dielectric matrix discussed in Sec. III.B.4. The form given by Eq. (80) is the most general field-theoretic formulation for a system of interacting electrons and nuclei. The next step is to rewrite δG=δφ inside Eq. (78) in terms ofR the inverse Green’s function G−1 . By using the fact that δ d2Gð12ÞG−1 ð23Þ ¼ 0 and the rule for the functional derivative of a product (Kadanoff and Baym, 1962) one obtains δGð12Þ ¼− δφð3Þ Z dð45ÞGð14Þ δG−1 ð45Þ Gð52Þ: δφð3Þ δG−1 ð45Þ ¼ δφð3Þ d6 δG−1 ð45Þ δV tot ð6Þ : δV tot ð6Þ δφð3Þ Γð123Þ ¼ δð12Þδð13Þ Z δΣð12Þ Gð46ÞGð75ÞΓð673Þ: þ dð4567Þ δGð45Þ ð82Þ 2. The screened Coulomb interaction The following equation for the screened Coulomb interaction can be found by combining Eqs. (79), (80), and (86): Z Wð12Þ ¼ vð12Þ þ ð83Þ dð34Þvð13Þ Pð12Þ ¼ ∂ ℏ2 2 þ ∇ ð1Þ − V tot ð1Þ Gð12Þ iℏ ∂t1 2me Z − d3Σð13ÞGð32Þ ¼ δð12Þ; δhn̂ð1Þi ; δV tot ð2Þ ð89Þ Z Wð12Þ ¼ vð12Þ þ dð34Þvð13ÞPð34ÞWð42Þ: ð90Þ This result can be combined with Eq. (86) in order to express the dielectric matrix in terms of the polarization: Z ϵð12Þ ¼ δð12Þ − ð84Þ having introduced the following so-called “electron selfenergy” Σ: Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 ð88Þ the previous expression takes the usual form (Hedin, 1965) By combining Eqs. (78) and (80)–(83) one finds δhn̂ð3Þi Wð42Þ: δV tot ð4Þ By defining the “polarization propagator” as It is customary to call “vertex” the three-point quantity defined by Γð123Þ ¼ −δG−1 ð12Þ=δV tot ð3Þ: ð87Þ The derivation of this result is rather lengthy: it requires the use of the chain rule, in symbols δ=δV tot ¼ ðδG=δV tot Þδ=δG, as well as Eq. (81) with Σ and V tot instead of G and φ, respectively. Equations (84)–(87) form a nonlinear system of equations for the electron Green’s function G, the electron self-energy Σ, the total screened Coulomb interaction W, and the vertex Γ. In order to close the loop it remains to specify the relation between W and the other quantities. The next section is devoted to this aspect. ð81Þ In order to eliminate any explicit reference to φ we can express the functional derivative on the right-hand side using the chain rule for functional differentiation (Kadanoff and Baym, 1962): Z The last equality can be obtained by observing that δhn̂ð1Þi=δφð2Þ ¼ δhn̂ð2Þi=δφð1Þ after Eq. (75); therefore Wð12Þ ¼ Wð21Þ. Now, by inverting Eq. (84) and using Eq. (83), we can express the vertex Γ in terms of Σ and G: dð3Þvð13ÞPð32Þ: ð91Þ We now consider the special case whereby the nuclei are regarded as classical point charges clamped to their equilibrium positions. In this situation, the variation of the charge density δhn̂i in Eq. (89) corresponds to the redistribution of the electronic charge in response to the perturbation δV tot . In order to describe this special case it is convenient to introduce 015003-16 Feliciano Giustino: Electron-phonon interactions from first … a new polarization propagator Pe associated with the electronic response only: X δhn̂e ð1Þi ¼ −iℏ Pe ð12Þ ¼ δV tot ð2Þ σ1 Z The comparison between Eqs. (97) and (98) yields δhn̂n ð1Þi δhn̂ð2Þi ¼ : δφð2Þ δJð1Þ þ dð34ÞGð13ÞGð41 ÞΓð342Þ: ð92Þ This can be restated by using the chain rule δhn̂e i=δJ ¼ δhn̂e i=δV tot × δV tot =δhni × δhni=δJ: The last equality in this expression is obtained by using Eq. (81) with V tot instead of φ, together with Eq. (83), and by considering that the electron density is related to the Green’s function via hn̂e ð1Þi ¼ −iℏ X Gð11þ Þ: ð93Þ σ1 δhn̂ð1Þi ¼ δJð2Þ Z dð34Þvð13ÞPe ð34ÞW e ð42Þ; ð94Þ as well as the associated dielectric matrix, in analogy with Eq. (91): Z ϵe ð12Þ ¼ δð12Þ − d3vð13ÞPe ð32Þ: ð95Þ Taken together, Eqs. (84)–(87) with W replaced by W e constitute the well-known Hedin’s equations for a system of interacting electrons when the nuclei are clamped to their equilibrium positions (Hedin, 1965). In order to go back to the most general case whereby the nuclei are not clamped to their equilibrium positions, one has to describe the readjustment of both electronic and nuclear charges. To this aim we combine Eqs. (80), (86), (88), (92), (94), and (95). The result is Z Wð12Þ ¼ W e ð12Þ þ dð34ÞW e ð13Þ δhn̂n ð3Þi vð42Þ: δφð4Þ δhn̂n ð1Þi i ¼ − hT̂½n̂ð2Þ − hn̂ð2Þi½n̂n ð1Þ − hn̂n ð1Þii: δφð2Þ ℏ ð97Þ RIn addition, if we introduce a second perturbation Ĥ2 ðtÞ ¼ drn̂n ðrtÞJðrtÞ, which couples only to the nuclear charges, we can repeat the same reasoning as in Eq. (97) after replacing φ by J and n̂ by n̂n : δhn̂ð1Þi i ¼ − hT̂½n̂n ð2Þ − hn̂n ð2Þi½n̂ð1Þ − hn̂ð1Þii: δJð2Þ ℏ Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 ð98Þ d3ϵ−1 e ð13Þ δhn̂n ð3Þi : δJð2Þ δhn̂n ð1Þi i ¼ − hT̂½n̂n ð2Þ − hn̂n ð2Þin̂n ð1Þi; δJð2Þ ℏ ð100Þ ð101Þ and since hn̂n − hn̂n ii ¼ 0 this can also be rewritten as δhn̂n ð1Þi=δJð2Þ ¼ Dð21Þ; ð102Þ having defined i Dð12Þ ¼ − hT̂½n̂n ð1Þ − hn̂n ð1Þi½n̂n ð2Þ − hn̂n ð2Þii: ℏ ð103Þ This quantity is called the “density-density correlation function” for the nuclei. Finally, we combine Eqs. (96), (99), (100), and (103) to obtain Wð12Þ ¼ W e ð12Þ þ W ph ð12Þ; ð104Þ where W ph is the nuclear contribution to the screened Coulomb interaction and is given by Z ð96Þ An explicit expression for δhn̂n i=δφ can be obtained using the following reasoning. We go into the details since this is a delicate passage. Equation (75) provides a recipe for evaluating the variation of any operator with respect to a potential φðrtÞ which couples to the total charge density operator n̂ðrtÞ R via Ĥ1 ðtÞ ¼ drn̂ðrtÞφðrtÞ. Therefore we can replace â b̂ in Eq. (75) by n̂n to obtain Z The variation δhn̂n i=δJ on the right-hand side can be expressed as in Eq. (98): In conjunction with Pe it is natural to define the Coulomb interaction screened by the electronic polarization only: W e ð12Þ ¼ vð12Þ þ ð99Þ W ph ð12Þ ¼ dð34ÞW e ð13ÞDð34ÞW e ð24Þ: ð105Þ This important result was first derived by Hedin and Lundqvist (1969). 3. Nuclear contribution to the screened Coulomb interaction In view of the forthcoming discussion, it is useful to derive a more explicit expression for the screened interaction W ph in Eq. (105). Here we follow Baym (1961) and Maksimov (1976). The Taylor expansion of the Dirac delta to second order in the displacement u reads δðr − uÞ ¼ δðrÞ − u · ∇δðrÞ þ 12u · ∇∇δðrÞ · u; ð106Þ where u · ∇∇ P · u is a short-hand notation for the second-order derivative αα0 uα uα0 ∇α ∇α0 . Equation (106) derives from the Fourier representation of the Dirac delta. Using Eq. (106) inside Eq. (67) we deduce 015003-17 Feliciano Giustino: Electron-phonon interactions from first … n̂n ðrÞ ¼ n0n ðrÞ þ X κp − Zκ Δτ̂ κp · ∇δðr − τ 0κp Þ 1X Z Δτ̂ · ∇∇δðr − τ 0κp Þ · Δτ̂ κp ; 2 κp κ κp ð107Þ where n0n ðrÞ is the density of nuclear point charges at the classical equilibrium positions τ 0κp . After taking into account the time evolution in the Heisenberg picture as in Eq. (71), we can replace this expansion inside Eq. (103) to obtain X Dð12Þ ¼ Zκ ∇1;α δðr1 − τ 0κp ÞDκαp;κ0 α0 p0 ðt1 t2 Þ καp κ0 α0 p0 × Zκ0 ∇2;α0 δðr2 − τ 0κ0 p0 Þ: ð108Þ On the right-hand side we introduced the “displacementdisplacement correlation function”: i Dκαp;κ0 α0 p0 ðtt0 Þ ¼ − hT̂Δτ̂καp ðtÞΔτ̂κ0 α0 p0 ðt0 Þi: ℏ In the following we describe the procedure originally devised by Baym (1961), and subsequently analyzed by Keating (1968), Hedin and Lundqvist (1969), Gillis (1970), and Maksimov (1976). The starting point is the equation of motion for the displacement operators Δτ̂καp ðtÞ. In analogy with Eq. (72) we have iℏ∂=∂tΔτ̂ κp ðtÞ ¼ ½Δτ̂ κp ðtÞ; Ĥ. Since we are considering the harmonic approximation and we expect the nuclei to oscillate around their equilibrium positions, it is convenient to aim for an expression resembling Newton’s equation. This can be done by taking the time derivative of the equation of motion ð109Þ Mκ ∂2 M Δτ̂ κp ¼ − 2κ ½½Δτ̂ κp ; Ĥ; Ĥ: 2 ∂t ℏ After evaluating the commutators using Eqs. (62)–(66) and performing the derivatives with respect to the nuclear displacements by means of Eq. (106), we obtain (the steps are laborious but straightforward) If we insert the last two equations into Eq. (105) we find W ph ð12Þ ¼ XZ καp κ 0 α0 p 0 ð111Þ ∂2 M κ 2 Δτ̂ κp ðtÞ ¼ Zκ ∂t 0 dð34Þϵ−1 e ð13Þ∇3;α V κ ðr3 − τ κp Þ Z drdr0 n̂ðκpÞ ðrtÞvðr; r0 Þ × f−∇0 δðr0 − τ 0κp Þ 0 × Dκαp;κ0 α0 p0 ðt3 t4 Þϵ−1 e ð24Þ∇4;α0 V κ 0 ðr4 − τ κ 0 p0 Þ: þ ∇0 ½∇0 δðr0 − τ 0κp Þ · Δτ̂ κp ðtÞg: ð112Þ ð110Þ In this expression V κ is the bare Coulomb potential of a nucleus or its ionic pseudopotential. At this point in the derivation, Hedin and Lundqvist introduced the approximation in which the electronic dielectric matrix in Eq. (110) can be replaced by its static counterpart. This choice implies the Born-Oppenheimer adiabatic approximation. In view of keeping the formalism as general as possible, we prefer to retain retardation effects, following the earlier works by Bardeen and Pines (1955) and Baym (1961). We come back to this aspect in Secs. V.A.3 and V.B.2. We stress the fact that the sole approximation used until this point is to truncate the density operator for the nuclei to the second order in the atomic displacements. This is the standard harmonic approximation. Apart from this approximation, which is useful to express W ph in a tractable form, no other assumptions are made. Gillis (1970) proposed a generalization of the results by Baym (1961) which does not use the harmonic approximation. However, the resulting formalism is exceedingly complex and has not been followed up. C. Phonon Green’s function In order to complete the set of self-consistent many-body equations for the coupled electron-phonon system, it remains to specify a prescription for calculating the displacementdisplacement correlation function Dκαp;κ0 α0 p0 ðtt0 Þ. This function is seldom referred to as the “phonon Green’s function,” even though strictly speaking this name should be reserved for the quantity −ði=ℏÞhT̂ âqν ðtÞâ†q0 ν0 ðt0 Þi discussed in Sec. V.A.1. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Here n̂ðκpÞ ðrÞ is the total charge density of electrons and nuclei, after removing the contribution of the nucleus κ in the unit cell p. In the second line ∇0 indicates that the derivatives are taken with respect to the variable r0 . At this point, we can use the functional derivative technique as in Sec. IV.B in order to determine an expression involving the displacementdisplacement correlation function from Eq. (109). Here, instead of using JðrÞ as in Sec. IV.B.2 for the nuclear density, it is convenient to work with the individual displacements and P introduce a third perturbation Ĥ3 ðtÞ ¼ κp Fκp ðtÞ · Δτ̂ κp ðtÞ. The extra terms Fκp ðtÞ have the meaning of external forces acting on the nuclei. Using this perturbation, it is possible to write the displacement-displacement correlation function in a manner similar to Eq. (101) δhΔτ̂καp ðtÞi ¼ Dκαp;κ0 α0 p0 ðtt0 Þ: δFκ0 α0 p0 ðt0 Þ ð113Þ This result was derived by Baym (1961) using a finitetemperature formalism. As in the case of the electron Green’s function in Sec. IV.B, it can be obtained only by working in the interaction picture and by taking into account the explicit time dependence of the Hamiltonian Ĥ þ Ĥ3 ðtÞ. Also in the present case, we omit these details for conciseness. If we take the expectation value of Eq. (112) in the ground state, after having added the new force term −Fκp ðtÞ, and carry out the functional derivative with respect to Fκ0 p0 ðt0 Þ, we obtain 015003-18 Feliciano Giustino: Electron-phonon interactions from first … Mκ ∂2 Dκαp;κ0 α0 p0 ðtt0 Þ ∂t2 ¼ −δκαp;κ0 α0 p0 δðtt0 Þ þ Zκ × − Z drdr0 δhn̂ðκpÞ ðrtÞi vðr; r0 Þ∇0α δðr0 − τ 0κp Þ δFκ0 α0 p0 ðt0 Þ þ hn̂ðκpÞ ðrtÞivðr; r0 Þ∇0α ∇0γ δðr0 − τ 0κp ÞDκγp;κ0 α0 p0 ðtt0 Þ ; ð114Þ where the sum over the Cartesian directions γ is implied. The derivation of this result is rather cumbersome and involves the following considerations: (i) the Dirac deltas in the first line come from the force terms −Fκp added to the Hamiltonian; (ii) within the harmonic approximation the expectation value hn̂ðκpÞ Δτ̂ κp i can be replaced by hn̂ðκpÞ ihΔτ̂ κp i (Baym, 1961); and (iii) the expectation value hΔτ̂ κp i can be set to zero, because at the end of the derivation one sets jFκp j ¼ 0, hence the expectation values of the displacements vanish. We note that Hedin and Lundqvist (1969) omitted the last line of Eq. (114) in their derivation, but this term was correctly included by Baym (1961) and Maksimov (1976). The remaining functional derivative in Eq. (114) can be expressed in terms of the nuclear charge density using the same strategy which led to Eq. (100). The result is Z 00 00 δhn̂ðκpÞ ðrtÞi 00 dt00 ϵ−1 ðrt; r00 t00 Þ δhn̂n ðr t Þi ¼ dr e δFκ0 α0 p0 ðt0 Þ δFκ0 α0 p0 ðt0 Þ X − Zκ Dκγp;κ0 α0 p0 ðtt0 Þ∇γ δðr − τ 0κp Þ: ð115Þ γ By inserting this result inside Eq. (114) and using the expansion in Eq. (107), we finally obtain the equation of motion for the displacement-displacement correlation function: 2 Mκ ∂ Dκαp;κ0 α0 p0 ðtt0 Þ ∂t2 0 ¼ −δκαp;κ0 α0 p0 δðtt Þ − X Z dt00 Πκαp;κ00 α00 p00 ðtt00 Þ κ 00 α00 p00 × Dκ00 α00 p00 ;κ0 α0 p0 ðt00 t0 Þ: ð116Þ The quantity Πκpα;κ0 p0 α0 ðtt0 Þ in this expression is called the “phonon self-energy” and is given by Πκαp;κ0 α0 p0 ðtt0 Þ Z ¼ drdr0 ½Zκ ∇α δðr − τ 0κp ÞW e ðrt; r0 t0 ÞZκ0 ∇0α0 δðr0 − τ 0κ0 p0 Þ 0 þ δκp;κ0 p0 δðtt Þ∇α hn̂ðrÞivðr; r 0 ÞZκ0 ∇0α0 δðr0 − τ 0κ0 p0 Þ: X κ 00 α00 p00 ½Mκ ω2 δκαp;κ00 α00 p00 − Πκαp;κ00 α00 p00 ðωÞ × Dκ00 α00 p00 ;κ0 α0 p0 ðωÞ ¼ δκαp;κ0 α0 p0 ; ð118Þ whereas the phonon self-energy in the frequency domain at equilibrium reads Z Πκαp;κ0 α0 p0 ðωÞ ¼ drdr0 ½Zκ ∇α δðr − τ 0κp ÞW e ðr; r0 ; ωÞ þ δκp;κ0 p0 ∇α hn̂ðrÞivðr; r0 ÞZκ0 ∇0α0 δðr0 − τ 0κ0 p0 Þ: ð119Þ The second line in this expression is conveniently rewritten by making use of the acoustic sum rule. This sum rule is well known in the theory of lattice dynamics of crystals (Born and Huang, 1954) and can be generalized to the case of manybody Green’s function approaches as follows (Hedin and Lundqvist, 1969): X Πκαp;κ0 α0 p0 ðω ¼ 0Þ ¼ 0 for any α; α0 : ð120Þ κ 0 p0 This relation was first derived by Baym (1961) by imposing the condition that the nuclei in the crystal must remain near their equilibrium positions due to fictitious restoring forces. Physically this condition corresponds to considering a crystal which is held fixed in the laboratory reference frame. In this approach, the crystal cannot translate or rotate as a whole. Similar relations were derived by Sjölander and Johnson (1965) and Gillis (1970). If we combine Eqs. (119) and (120), perform integrations by parts, and carry out the integrations in r and r0 we obtain X ∂ 2 Πκαp;κ0 α0 p0 ðωÞ ¼ Zκ Zκ00 ∂rα ∂r0α0 r¼τ 0κp ;r0 ¼τ 0 κ 00 p00 κ00 p00 0 ½δκ0 p0 ;κ00 p00 W e ðr; r ; ωÞ − δκp;κ0 p0 W e ðr; r0 ; 0Þ; ð117Þ The derivation of Eq. (117) is nontrivial and is not found consistently in the literature. It requires converting the derivatives with respect to the position variables r, r0 into derivatives with respect to the nuclear coordinates; integrating by parts in order to rearrange the derivatives with respect to r and r0 ; invoking the harmonic approximation; and considering that, after setting the forces Fkp ðtÞ ¼ 0 and the field φðrtÞ ¼ 0 at the Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 end, the expectation value hn̂ðrtÞi does not depend on time. The term in the third line of Eq. (117) is what Baym (1961) called the “static force,” since it arises from the forces experienced by the nuclei in their equilibrium configuration. In order to simplify Eq. (117) it is convenient to move from the time to the frequency domain. We use the following convention Fourier transform of a function fðtÞ: R ∞ for the iωt fðωÞ ¼ −∞ dtfðtÞe . Since we are considering equilibrium properties in the absence of time-dependent external potentials, the time variables enter in these quantities only as differences (Abrikosov, Gor’kov, and Dzyaloshinski, 1975); for example, W e ðrt; r0 t0 Þ ¼ W e ðr; r0 ; t − t0 Þ. As a consequence, Eq. (116) is rewritten as ð121Þ which fulfills the sum rule in Eq. (120). Equations (118) and (121) completely define the nuclear dynamics in the harmonic approximation. After obtaining the displacement-displacement correlation function Dκαp;κ0 α0 p0 ðtt0 Þ by solving this set of equations, it is possible to construct the expectation value of the nuclear density using Eqs. (107) and (109) 015003-19 Feliciano Giustino: Electron-phonon interactions from first … TABLE I. Self-consistent Hedin-Baym equations for the coupled electron-phonon system in the harmonic approximation. Eq. Description (93) Electronic charge density (122) Nuclear charge density (79) Total electrostatic potential (84) Equation of motion, electrons (118) Equation of motion, nuclei (85) Electron self-energy (94) Screened Coulomb, electrons (92) Electronic polarization (95) Electronic dielectric matrix (87) Vertex (110) Screened Coulomb, nuclei (121) P Expression þ hn̂e ð1Þi ¼ −iℏ σ1 Gð11 Þ P hn̂n ðrtÞi ¼ n0n ðrÞ − ðiℏ=2Þ κp;αα0 Zκ ∂ 2 δðr − τ 0κp Þ=∂rα ∂rα0 Dκαp;κα0 p ðtþ tÞ R V tot ð1Þ ¼ d2vð12Þ½hn̂e ð2Þi þ hn̂n ð2Þi R ½iℏ∂=∂t1 þ ðℏ2 =2me Þ∇2 ð1Þ − V tot ð1ÞGð12Þ − d3Σð13ÞGð32Þ ¼ δð12Þ P 2 κ 00 α00 p00 ½M κ ω δκαp;κ 00 α00 p00 − Πκαp;κ 00 α00 p00 ðωÞDκ 00 α00 p00 ;κ 0 α0 p0 ðωÞ ¼ δκαp;κ 0 α0 p0 R Σð12Þ ¼ iℏ dð34ÞGð13ÞΓð324Þ½W e ð41þ Þ þ W ph ð41þ Þ R W e ð12Þ ¼ vð12Þ þ dð34Þvð13ÞPe ð34ÞW e ð42Þ P R Pe ð12Þ ¼ −iℏ σ1 dð34ÞGð13ÞGð41þ ÞΓð342Þ R ϵe ð12Þ ¼ δð12Þ − dð3Þvð13ÞPe ð32Þ R Γð123Þ ¼ δð12Þδð13Þ þ dð4567Þ½δΣð12Þ=δGð45ÞGð46ÞGð75ÞΓð673Þ R P 0 W ph ð12Þ ¼ καp;κ0 α0 p0 dð34Þϵ−1 e ð13Þ∇3;α V κ ðr3 − τ κp Þ 0 ×Dκαp;κ0 α0 p0 ðt3 t4 Þϵ−1 e ð24Þ∇4;α0 V κ 0 ðr4 − τ κ 0 p0 Þ P Πκαp;κ0 α0 p0 ðωÞ ¼ κ00 p00 Zκ Zκ00 ð∂ 2 =∂rα ∂r0α0 Þ Phonon self-energy ×½δκ0 p0 ;κ00 p00 W e ðr; r0 ; ωÞ − δκp;κ0 p0 W e ðr; r0 ; 0Þr¼τ 0κp ;r0 ¼τ 0 κ00 p00 hn̂n ðrtÞi ¼ n0n ðrÞ − iℏ X ∂ 2 δðr − τ 0κp Þ Z Dκαp;κα0 p ðtþ tÞ: 2 κp;αα0 κ ∂rα ∂rα0 ð122Þ We emphasize that, according to Eq. (121), the coupling of the nuclear displacements to the electrons is completely defined by the electronic dielectric matrix through W e . Similarly, the nuclei affect the electronic structure via the dielectric matrix which enters W ph in Eq. (110) and via the nuclear density inside V tot in Eq. (79). From these considerations it should be clear that the electronic dielectric matrix ϵe ðr; r0 ; ωÞ plays an absolutely central role in the field-theoretic approach to the electron-phonon problem. D. Hedin-Baym equations Apart from making use of the harmonic approximation, the set of equations given by Eqs. (79), (84), (85), (87), (92), (93), (94), (95), (110), (118), (121), and (122) describe the coupled electron-phonon system entirely from first principles. This set of equations can be regarded as the most sophisticated description of interacting electrons and phonons available today. Since the self-consistent equations for the electrons were originally derived by Hedin (1965), and those for the nuclei were derived first by Baym (1961), we refer to the complete set as the Hedin-Baym equations. Given the importance of these relations, we summarized them schematically in Table I. The standard Hedin’s equations for interacting electrons in the potential of clamped nuclei (Hedin, 1965) are immediately recovered from the Hedin-Baym equations by setting to zero the displacement-displacement correlation function of the nuclei Dκpα;κ0 p0 α0 ¼ 0. Table I provides a closed set of self-consistent equations whose solution yields the Green’s functions of a fully interacting electron-phonon system, within the harmonic approximation. We stress that these relations are Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 fundamentally different from diagrammatic approaches. In fact, here the coupled electron-phonon system is not addressed using Feynman-Dyson perturbation theory as was done, for example, by Keating (1968). Instead, in Table I, electrons and phonons are described nonperturbatively by means of a coupled set of nonlinear equations for the exact propagators. In particular, we emphasize that this approach does not require the Born-Oppenheimer adiabatic approximation, and therefore it encompasses insulators, intrinsic as well as doped semiconductors, metals, and superconductors. Almost every property related to electron-phonon interactions in solids that can be calculated today from first principles can be derived from these equations. Examples to be discussed in Secs. V–X include the renormalization of the Fermi velocity, the band gap renormalization in semiconductors and insulators, the nonadiabatic corrections to vibrational frequencies, the Frölich interaction, and the lifetimes of electrons and phonons. The generalization of these results to the case of finite temperature should also be able to describe phonon-mediated superconductivity, although this phenomenon is best addressed by directly studying the propagation of Cooper pairs (see Sec. XI). Baym’s theory can in principle be extended to go beyond the harmonic approximation (Gillis, 1970). However, the mathematical complexity of the resulting formalism is formidable, due to the appearance of many additional terms which are neglected in the harmonic approximation. V. FROM A MANY-BODY FORMALISM TO PRACTICAL CALCULATIONS The Hedin-Baym equations summarized in Table I define a rigorous formalism for studying interacting electrons and phonons in metals, semiconductors, and insulators entirely from first principles. However, a direct numerical solution of these equations for real materials is currently out of reach, and approximations are needed for practical calculations. 015003-20 Feliciano Giustino: Electron-phonon interactions from first … The following sections establish the connection between the Hedin-Baym equations and standard expressions which are currently in use in ab initio calculations of electron-phonon interactions. A. Effects of the electron-phonon interaction on phonons 1. Phonons in the Born-Oppenheimer adiabatic approximation The vibrational eigenmodes of the nuclei can be identified with the resonances of the displacement-displacement correlation function Dκpα;κ0 p0 α0 ðtt0 Þ in the frequency domain. If we denote by M the diagonal matrix having the nuclear masses Mκ along its diagonal, then the formal solution of Eq. (118) can be written as DðωÞ ¼ ½Mω2 − ΠðωÞ−1 ; ð123Þ In the early literature it is common to find a different partitioning, whereby the noninteracting system is defined by the bare interatomic force constants, corresponding to nuclei in the absence of electrons (Grimvall, 1981). This alternative choice is not useful in modern calculations, because the resulting noninteracting phonon dispersions are very different from the fully interacting dispersions. The present choice of using instead adiabatic phonons as the noninteracting system is more convenient in the context of modern ab initio techniques, since calculations of adiabatic phonon spectra are routinely performed within DFPT. In the remainder of this section we concentrate on the adiabatic term, and we defer the discussion of the nonadiabatic self-energy to Sec. V.A.2. Using Eq. (121), we can rewrite the adiabatic self-energy as follows: X ΠA ðδκ0 p0 ;κ00 p00 − δκp;κ0 p0 Þ καp;κ 0 α0 p0 ¼ κ00 p00 Z where D is the matrix with elements Dκpα;κ0 p0 α0 . The resonant frequencies of the system correspond to the solutions of the nonlinear equations Ων ðωÞ − ω ¼ 0; Ω2ν ðωÞ with ν ¼ 1; …; 3M; −1=2 −1=2 ð125Þ with ΠA ¼ Πðω ¼ 0Þ. As we will see, the adiabatic term ΠA will be taken to describe “noninteracting” phonons, and the nonadiabatic self-energy ΠNA will be used to describe the effects of electron-phonon interactions. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 dr ∂hn̂e ðrÞi ∂V en ðrÞ ∂ 2 Unn : þ ∂τκαp ∂τκ00 α0 p00 ∂τκ00 α0 p00 ∂τκαp ð126Þ ð124Þ is an eigenvalue of M ΠðωÞM , parawhere metric in the variable ω. As expected, the study of lattice vibrations within a field-theoretic framework resembles the standard eigenvalue problem reviewed in Sec. III.A. In particular, the matrix ΠðωÞ represents the many-body counterpart of the matrix of interatomic force constants Cκαp;κ0 α0 p0 introduced in Eq. (13). However, despite its formal simplicity, Eq. (124) conceals the full wealth of information associated with the many-body electronic screening ϵe ðr; r0 ; ωÞ via Eq. (121). In fact, the phonon self-energy is generally complex and frequency dependent. Therefore we can expect to find roots of Eq. (124) outside of the real frequency axis, as well as multiple roots for the same “eigenmode.” The link between Eq. (124) and phonon calculations by means of DFT is established by noting that DFT relies on the Born-Oppenheimer adiabatic approximation. In the adiabatic approximation the nuclei are considered immobile during characteristic electronic time scales. Formally, this approximation is introduced by setting ω ¼ 0 in Eq. (121) (Keating, 1968). In practice, this assumption corresponds to stating that ϵe ðr; r0 ; ωÞ can be replaced by ϵe ðr; r0 ; 0Þ in the frequency range of the vibrational excitations. Obviously this is not always the case, and important exceptions are discussed in Sec. V.A.2. In order to see more clearly the connection with the formalism discussed in Sec. III.A, we partition the phonon self-energy into “adiabatic” and “nonadiabatic” contributions: ΠðωÞ ¼ ΠA þ ΠNA ðωÞ; × In this expression U nn is the nucleus-nucleus interaction energy from Eq. (65), V en is the electron-nuclei interaction from Eq. (25), and all the derivatives are taken at the equilibrium coordinates. The derivation of Eq. (126) requires the use of the identity ∂hn̂e ðrÞi ¼ −Zκ ∂τ0καp Z 0 0 0 0 0 dr0 ½ϵ−1 e ðr; r ; 0Þ − δðr; r Þ∇α δðr − τ κp Þ: ð127Þ This identity follows from the same reasoning leading to Eq. (100), after considering an external potential which modifies the position of the nucleus κ in the cell p. Equation (126) can be recast in a familiar form by exploiting the acoustic sum rule in Eq. (120). Indeed after a few tedious but straightforward manipulations we obtain Z ΠA καp;κ 0 α0 p0 ¼ þ ∂hn̂e ðrÞi ∂V en ðrÞ dr þ ∂τκ0 α0 p0 ∂τκαp ∂ 2 U nn : ∂τκαp ∂τκ0 α0 p0 Z drhn̂e ðrÞi ∂ 2 V en ðrÞ ∂τκαp ∂τκ0 α0 p0 ð128Þ In this form, one can see that the adiabatic self-energy gives precisely the interatomic force constants that we would obtain using the Born-Oppenheimer approximation and the Hellman-Feynman theorem; compare Eq. (128), for example, with Eq. (10) of Baroni et al. (2001). The difference between ΠA καp;κ 0 α0 p0 in Eq. (128) and Cκαp;κ0 α0 p0 in Eq. (13) is that, in the former case, the electron density response to atomic displacements is governed by the exact many-body dielectric matrix ϵe ðr; r0 ; 0Þ and electron density hn̂e ðrÞi, as shown by Eqs. (127) and (128). As a result, ΠA καp;κ 0 α0 p0 corresponds to force constants and electron density dressed by all many-body interactions of the system (both electron-electron and electron-phonon interactions). In 015003-21 Feliciano Giustino: Electron-phonon interactions from first … contrast, when the force constants in Eq. (13) are calculated using DFT, the electron density response to an atomic displacement is evaluated using the RPA þ xc screening, that is, ϵHxc ðr; r0 Þ from Sec. III.B.4, and the ground-state electron density is calculated at clamped nuclei. The use of the adiabatic approximation in the study of phonons carries the important advantage that the many-body force constants ΠA form a real and symmetric matrix. This can be seen by rewriting Eq. (121) for ω ¼ 0, and using W e ðr; r0 ; ωÞ ¼ W e ðr0 ; r; −ωÞ which follows from the property Wð12Þ ¼ Wð21Þ (see Sec. IV.B). Since ΠA is real and symmetric, all its eigenvalues are guaranteed to be real. In this approximation, the excitations of the lattice correspond to sharp resonances in the displacement-displacement correlation function DðωÞ, and it is meaningful to talk about phonons as long-lived excitations of the system. In fact these excitations are infinitely long lived in the harmonic approximation. In practical calculations, the many-body ΠA is invariably replaced by the DFT interatomic force constants, and in this case the agreement of the calculated phonon frequencies with experiment is excellent in most cases. Illustrative examples can be found among others in Yin and Cohen (1982), Giannozzi et al. (1991), Dal Corso et al. (1993), Lee, Ghosez, and Gonze (1994), Kresse, Furthmüller, and Hafner (1995), Bungaro, Rapcewicz, and Bernholc (2000), Dal Corso and de Gironcoli (2000), Karki et al. (2000), Baroni et al. (2001), Díaz-Sánchez, Romero, and Gonze (2007), and Dal Corso (2013). The most obvious criticism to the adiabatic approximation is that, in the case of metals, the assumption ϵe ðr; r0 ; ωÞ ≃ ϵe ðr; r0 ; 0Þ is inadequate. This can intuitively be understood by recalling that the dielectric function of the homogeneous electron gas diverges when ω; q → 0 (Mahan, 1993). In practical calculations, this divergence is connected with vanishing denominators in Eq. (51) for q → 0. An approximate, yet successful strategy for overcoming this problem is to replace the occupation numbers in Eq. (51) by smoothing functions such as the Fermi-Dirac distribution and to describe the singular terms analytically (de Gironcoli, 1995). Most first-principles calculations of phonon dispersion relations in metals have been carried out using this strategy. Improvements to this strategy are discussed in Sec. V.A.2. The adiabatic approximation leads naturally to the definition of an adiabatic propagator DA ðωÞ, which can be obtained from Eq. (123) after replacing the phonon selfenergy by its static limit DA ðωÞ ¼ ½Mω2 − ΠA −1 : ð129Þ Now, if we identify ΠA καp;κ 0 α0 p0 with the interatomic force constant Cκαp;κ0 α0 p0 in Eq. (13), we can obtain an explicit expression for the adiabatic phonon propagator in terms of the eigenmodes eκα;ν ðqÞ and eigenfrequencies ωqν introduced in Sec. III.A. To this end we invert Eq. (129) using Eqs. (14)–(17) and recall that the dynamical matrix is Hermitian and obeys dm Ddm; κα;κ 0 α0 ðqÞ ¼ Dκα;κ0 α0 ð−qÞ (Maradudin and Vosko, 1968). After tedious but straightforward steps we find Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 DA καp;κ 0 α0 p0 ðωÞ ¼ X Z dq 2ωqν Sqν;καp Sqν;κ0 α0 p0 2 ; Ω ω − ω2qν BZ ν ð130Þ with the definition Sqν;καp ¼ eiq·Rp ð2Mκ ωqν Þ−1=2 eκα;ν ðqÞ: ð131Þ This result suggests that, as expected, the propagator should take a simple form in the eigenmodes representation. In fact, by using the inverse transform of Eq. (131) we have 0 A DA qν;q0 ν0 ðωÞ ¼ ΩBZ δðq − q ÞDqνν0 ðωÞ, with 2 2 0 DA qνν0 ðωÞ ¼ 2ωqν =ðω − ωqν Þδνν : ð132Þ This result can alternatively be obtained starting from the ladder operators of Appendix B. In fact, after using Eqs. (20), (109), and (131) we find † † 0 0 0 0 DA qνν0 ðtt Þ ¼ −ihT̂½âqν ðtÞâqν ðt Þ þ â−qν ðtÞâ−qν ðt Þiδνν : ð133Þ An explicit evaluation of the right-hand side using the Heisenberg time evolution generated by the phonon Hamiltonian in Eq. (22) yields precisely Eq. (132), with the added advantage that it is easier to keep track of the time ordering. The result is DA qνν ðωÞ ¼ 1 1 − ; ω − ωqν þ iη ω þ ωqν − iη ð134Þ with η a positive real infinitesimal. This alternative approach is very common in textbooks; see, for example, Schrieffer (1983) and Schäfer and Wegener (2002). However, it does not carry general validity in a field-theoretic framework since it rests on the adiabatic approximation. 2. Phonons beyond the adiabatic approximation In order to go beyond the adiabatic approximation, it is necessary to determine the complete propagator DðωÞ in Eq. (123). Formally this can be done by combining Eqs. (123) and (125) to obtain the following Dyson-like equation: DðωÞ ¼ DA ðωÞ þ DA ðωÞΠNA ðωÞDðωÞ: ð135Þ In this form it is apparent that the nonadiabatic phonon self-energy ΠNA ðωÞ “dresses” the noninteracting phonons obtained within the adiabatic approximation, as shown schematically in Fig. 1(a). It is convenient to rewrite the Dyson equation in such a way as to show more clearly the poles of the propagator. Using Eqs. (131) and (132) we find D−1 qνν0 ðωÞ ¼ 1 ½δ 0 ðω2 − ω2qν Þ − 2ωqν ΠNA qνν0 ðωÞ; 2ωqν νν ð136Þ −1 where ΠNA qνν0 and Dqνν0 are obtained using the transform of Eq. (131) and its inverse, respectively. 015003-22 Feliciano Giustino: Electron-phonon interactions from first … From Eq. (136) we see that the nonadiabatic self-energy ΠNA modifies the adiabatic phonon spectrum in four distinct ways: (i) the real part of the diagonal elements ΠNA qνν shifts the adiabatic frequencies; (ii) the imaginary part introduces spectral broadening; (iii) the off-diagonal elements of ΠNA qνν0 introduce a coupling between the adiabatic vibrational eigenmodes; and (iv) the frequency dependence of ΠNA qνν ðωÞ might lead to multiple poles for the same mode ν, thereby introducing new structures in the phonon spectrum. Today it is relatively common to calculate phonon linewidths arising from electron-phonon interactions (Allen, 1972b; Bauer et al., 1998). Recently it has also become possible to study the frequency renormalization due to nonadiabatic effects (Saitta et al., 2008; Calandra, Profeta, and Mauri, 2010). The possibility of observing new features in vibrational spectra arising from the EPI has not been studied from first principles, but the underlying phenomenology should be similar to that of plasmon satellites in photoelectron spectra (see Sec. V.B.6). Generally speaking we expect satellites whenever ϵe ðr; r0 ; ωÞ exhibits dynamical structure close to vibrational frequencies. This can happen, for example, in the case of degenerate polar semiconductors, when phonon and plasmon energies are in resonance. In these cases, phonons and plasmons can combine into “coupled plasmon-phonon modes” (Richter, 1984), which are the electronic analog of photon polaritons (Yu and Cardona, 2010). This phenomenon was predicted theoretically (Varga, 1965) and subsequently confirmed by Raman measurements on GaAs (Mooradian and Wright, 1966). We speculate that it should be possible to obtain coupled plasmon-phonon modes from the frequency dependence of the phonon self-energy in Eq. (136); it would be interesting to perform first-principles calculations in order to shed light on these aspects. In practical calculations the nonadiabatic corrections to the adiabatic phonon spectrum are evaluated from Eq. (136) using first-order perturbation theory, by retaining only the diagonal elements of ΠNA . If we denote the complex zeros of D−1 qνν ðωÞ ~ qν ¼ Ωqν − iγ qν, in the case of nondegenerate eigenmby Ω odes Eq. (136) gives ~ 2qν ¼ ω2qν þ 2ωqν ΠNA ~ Ω qνν ðΩqν Þ; ð137Þ therefore γ qν ¼ − ωqν ImΠNA qνν ðΩqν − iγ qν Þ; Ωqν Ω2qν ¼ ω2qν þ γ 2qν þ 2ωqν ReΠNA qνν ðΩqν − iγ qν Þ: γ 2qν ð138Þ ð139Þ Apart from the small term in Eq. (139), these expressions are identical to those provided by Allen (1972b) and Grimvall (1981). Since nonadiabatic corrections are usually small as compared to the adiabatic phonon frequencies, Eqs. (138) and (139) are often simplified further by using the additional approximations jΩqν − ωqν j ≪ ωqν and jγ qν j ≪ ωqν , leading NA to γ qν ≃ −ImΠNA qνν ðωqν Þ and Ωqν ≃ ωqν þ ReΠqνν ðωqν Þ. In these forms it becomes evident that the real part of the Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 self-energy shifts the adiabatic phonon frequencies, and the imaginary part is responsible for the spectral broadening of the resonances. Using these expressions in Eq. (136) and going back to the time domain, it is seen that, as a result of the EPI, −1 phonons acquire a finite lifetime given by τph qν ¼ ð2γ qν Þ . 3. Expressions for the phonon self-energy used in ab initio calculations In the literature on electron-phonon interactions, the phonon self-energy Π is almost invariably expressed in terms of an electron-phonon vertex g and the electron Green’s function G as Π ¼ jgj2 GG in symbolic notation; see, for example, Grimvall (1981). While this has become common practice also in ab initio calculations, the origin of this choice is not entirely transparent. One could derive this expression directly from Eq. (1), using standard Green’s function techniques. However, this procedure does not answer the key question of how to calculate the electron-phonon matrix elements g. A closer inspection of the theory reveals that this is a rather nontrivial point. In fact, on the one hand, a straightforward expansion of the second-quantized Hamiltonian of Eq. (68) in terms of the nuclear coordinates leads to “bare” electronphonon matrix elements gb , which contain the bare Coulomb interaction between electrons and nuclei. On the other hand, if we go back to Sec. III.B.2, we see that the electron-phonon matrix elements in DFT are dressed by the self-consistent response of the electrons. The difference between the bare and the dressed vertex is not only quantitative, but also qualitative: for example, in metals the bare vertex is long ranged, while the screened vertex is short ranged. The relation between bare and dressed electron-phonon vertices and the derivation of explicit expressions for the phonon self-energy have been discussed by many; see, for example, Scalapino (1969) and Rickayzen (1980). In short, the argument is that the lowest-order Feynman diagram starting and ending with a phonon line must contain precisely two bare electron-phonon vertices, as shown in Fig. 1(b). By construction this diagram corresponds to having Π ¼ jgb j2 GG. In order to make the transition from the bare vertex to the dressed vertex it is necessary to collect together all the proper electronic polarization diagrams around the vertex. However, these steps have been carried out only for the homogeneous electron gas (Scalapino, 1969; Rickayzen, 1980). In the following we show how the dressed electronphonon vertex emerges from a nonperturbative analysis based on the Hedin-Baym equations. The nonadiabatic phonon self-energy ΠNA introduced in Sec. V.A.2 can be written explicitly by combining Eqs. (119) and (125): Z ΠNA καp;κ 0 α0 p0 ðωÞ ¼ drdr0 Zκ ∇α δðr − τ 0κp Þ × ½W e ðr;r0 ;ωÞ − W e ðr;r0 ;0ÞZκ0 ∇0α0 δðr0 − τ 0κ0 p0 Þ: ð140Þ Using the Dyson equation for the screened Coulomb interaction, it can be seen that this expression does indeed contain electron-phonon matrix elements. In fact, by inserting Eq. (94) 015003-23 Feliciano Giustino: Electron-phonon interactions from first … where V en is the potential of the nuclei from Eq. (25); in practical calculations this quantity is replaced by the usual ionic pseudopotentials. The meaning of the variation Δqν is the same as in Eqs. (33)–(35). The dressed couplings g and gcc are defined as (Hedin and Lundqvist, 1969) Z gqν ðr; ωÞ ¼ Z gcc qν ðr; ωÞ ¼ FIG. 1. Diagrammatic representation of the phonon Green’s function and self-energy. (a) Dyson equation for the phonon propagator, Eq. (135). The thick wavy line represents the fully interacting, nonadiabatic propagator; the thin wavy line is the adiabatic propagator; the disk is the nonadiabatic self-energy. (b) Lowest-order diagrammatic expansion of the phonon selfenergy in terms of the bare electron-phonon vertices and the RPA electronic polarization. The small dots are the bare electronphonon coupling functions, and the thin lines are the noninteracting (for example, Kohn-Sham) electron Green’s functions. This diagram is the simplest possible term which begins and ends with a phonon line. (c) Nonperturbative representation of the phonon self-energy in terms of the bare coupling, the dressed coupling (large gray disk), the fully interacting electron Green’s functions (thick lines), and the vertex Γ from Eq. (83). This diagram was proposed by Keating (1968) and describes the first line of Eq. (141). (d) Schematic representation of the relation between the dressed electron-phonon coupling g and the bare coupling gb , from Eq. (144). Vogl (1976) reports a similar diagram, although with the bare coupling function on the far right; the difference stems from the present choice of using the irreducible polarization P ¼ GGΓ instead of the reducible polarization employed by Vogl. into Eq. (140) we find terms like vPe W e , and the electronphonon matrix elements will arise from taking the gradients of v and W e . By working in the eigenmodes representation via Eq. (131), after lengthy manipulations this procedure yields Z ℏΠNA qν;q0 ν0 ðωÞ ¼ − Z 0 drdr0 gbqν ðrÞPe ðr; r0 ; ωÞgcc q0 ν0 ðr ; ωÞ drdr0 gbqν ðrÞPe ðr; r0 ; 0Þgq0 ν0 ðr0 ; 0Þ; ð141Þ where we introduced electron-phonon “coupling functions” as follows. The bare coupling gb is defined as gbqν ðrÞ ¼ Δqν V en ðrÞ; Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 ð142Þ 0 b 0 dr0 ϵ−1 e ðr; r ; ωÞgqν ðr Þ; ð143Þ b; 0 0 dr0 ϵ−1 e ðr; r ; ωÞgqν ðr Þ: ð144Þ Since the dielectric matrix is real at ω ¼ 0, we have the simple relation gcc qν ðr; 0Þ ¼ gqν ðr; 0Þ. In order to derive Eq. (141) it is best to carry out the algebra in the time domain. We emphasize that the result expressed by Eq. (141) is nonperturbative and relies solely on the harmonic approximation. Equation (141) is in agreement with the standard result for the homogeneous electron gas (Scalapino, 1969). The same expression was also obtained by Keating (1968) using a detailed diagrammatic analysis. Keating’s diagrammatic representation of the self-energy is shown in Fig. 1(c) and can be obtained from Eq. (141) by noting that, in symbolic notation, Pe ¼ GGΓ from Eq. (92); therefore Π ¼ gb GGΓg. For completeness we also show in Fig. 1(d) a diagrammatic representation of the dressed electron-phonon coupling function g as given by Eq. (144). This representation is obtained by observing that g ¼ ϵ−1 gb , ϵ ¼ 1 − vP, and P ¼ GGΓ; therefore g ¼ gb þ vGGΓg. In view of practical first-principles calculations it is useful to have a simplified expression for the nonadiabatic phonon self-energy in Eq. (141). To this aim we make the following approximations: (i) The vertex function in Eq. (92) is set to Γð123Þ ¼ δð12Þδð13Þ. This is the same approximation at the center of the GW method (Hedin, 1965; Hybertsen and Louie, 1986; Onida, Reining, and Rubio, 2002). (ii) The fully interacting electron Green’s function G is replaced by its noninteracting counterpart, using the Kohn-Sham eigenstates and eigenvalues evaluated with the nuclei held in their equilibrium positions. (iii) The fully interacting dielectric matrix in Eq. (144) is replaced by the RPA þ xc response obtained from a DFT calculation, as discussed in Sec. III.B.2. (iv) The frequency dependence of the screened electronphonon coupling defined in Eq. (144) is neglected: cc gcc qν ðr; ωÞ ≃ gqν ðr; 0Þ ¼ gqν ðr; 0Þ. This approximation is ubiquitous in the literature but it is never mentioned explicitly. (v) For notational simplicity, we consider a spindegenerate system with time-reversal symmetry; this simplification is easily removed. Using these assumptions we can rewrite the component of Eq. (141) for q ¼ q0 as 015003-24 Feliciano Giustino: Electron-phonon interactions from first … ℏΠNA qνν0 ðωÞ X Z dk ¼2 gb ðk; qÞgmnν0 ðk; qÞ ΩBZ mnν mn fmkþq − f nk fmkþq − fnk − : × εmkþq − εnk − ℏðω þ iηÞ εmkþq − εnk ð145Þ We note that the components of the phonon self-energy for q ≠ q0 vanish due to the periodicity of the crystalline lattice. In Eq. (145) the sums run over all the Kohn-Sham states, with occupations fnk , and η is a real positive infinitesimal. In this case we indicate explicitly the factor of 2 arising from the spin degeneracy. The matrix element gmnν ðk; qÞ is the same as in Eq. (38), and it is precisely the quantity calculated by most linear-response codes. The matrix element gbmnν ðk; qÞ is obtained from gmnν ðk; qÞ by replacing the variation of the Kohn-Sham potential by the corresponding variation of the ionic (pseudo)potentials. The field-theoretic phonon selfenergy given by Eq. (145) is in agreement with the expression derived by Calandra, Profeta, and Mauri (2010) starting from time-dependent density-functional perturbation theory. The presence of both the bare electron-phonon matrix element and the screened matrix element in Eq. (145) has not been fully appreciated in the literature, and most ab initio calculations employ an approximate self-energy whereby gb is replaced by g. The replacement of the bare matrix elements by their screened counterparts in the phonon self-energy goes a long way back and can be found already in the seminal work by Allen (1972b). As a result many investigators (including myself) calculated phonon lifetimes using the following expression (Grimvall, 1981): 1 τph qν Z 2π X dk ¼ 2 jg ðk; qÞj2 ðfnk − fmkþq Þ ℏ mn ΩBZ mnν × δðεmkþq − εnk − ℏωqν Þ: ð146Þ This is obtained from Eq. (145) by taking the imaginary part and by making the replacement gb → g. While Eq. (146) can be derived from the Fermi golden rule in an independentparticle approximation [see Albers et al. (1976), Appendix B], the choice of the electron-phonon matrix elements is somewhat arbitrary. In future calculations of the phonon self-energy it will be important to assess the significance of using the correct vertex structure, that is, replacing jgmnν ðk; qÞj2 by gbmnν ðk; qÞgmnν ðk; qÞ in Eq. (146). In general, the effects of the nonadiabatic self-energy on the phonon spectrum are expected to be significant only in the case of metals and small-gap semiconductors. In fact, by combining Eqs. (138), (139), and (145) it is seen that ΠNA can be large only when occupied and empty single-particle states are separated by an energy of the order of the characteristic phonon energy. In such a case, we can expect a shift of the adiabatic phonon frequencies and a concomitant broadening of the lines. A clear illustration of these effects was provided by Maksimov and Shulga (1996), who analyzed a simplified model of a metal with linear bands near the Fermi level. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Calculations of phonon linewidths based on Eq. (146) have been reported by several2 and have become commonplace in first-principles studies of electron-phonon physics. On the other hand, calculations of the nonadiabatic phonon frequencies using Eq. (145) have been reported only by Lazzeri and Mauri (2006), Caudal et al. (2007), Piscanec et al. (2007), Saitta et al. (2008), and Calandra, Profeta, and Mauri (2010), using the approximation that the bare vertex gb can be replaced by the screened vertex g. Examples of such calculations are reviewed in Sec. VII. Equation (145) suggests several avenues worth exploring in the future: first, the use of the bare vertex should not pose a challenge in practical calculations, since this quantity is already being calculated in linear-response DFT codes. Testing the impact of the bare vertex on phonon linewidths and frequency renormalizations will be important. Second, Eq. (145) contains off-diagonal couplings, which are usually ignored. It will be interesting to check the effect of using the complete matrix self-energy. Third, the dynamical structure of the self-energy may contain interesting information such as, for example, spectral satellites and coupled phonon-plasmon modes. Last, the move from Eq. (141) to Eq. (145) involves the approximation that the frequency dependence of the electron-phonon matrix elements can be neglected. The validity of this approximation is uncertain, and there are no reference ab initio calculations on this. However, we note that frequency-dependent electron-phonon matrix elements have been employed systematically in theoretical models of doped semiconductors (Mahan, 1993, Sec. 6.3). Before closing this section we note that the formalism discussed here is based on zero-temperature Green’s functions. In order to extend the present results to finite temperature it is necessary to repeat all derivations using the Matsubara representation and then perform the analytic continuation of the self-energy to the real frequency axis. Detailed derivations can be found in Baym (1961) and Gillis (1970) and will not be repeated here. Fortunately it turns out that Eq. (145) can be extended to finite temperature by simply replacing the occupation factors fnk and fmkþq by the corresponding Fermi-Dirac distributions.3 B. Effects of the electron-phonon interaction on electrons 1. Electron self-energy: Fan-Migdal and Debye-Waller terms In Sec. V.A we discussed the link between the Hedin-Baym equations summarized in Table I and ab initio calculations of phonons. We first identified a Hermitian eigenvalue problem for the vibrational frequencies via the adiabatic approximation, and then we improved upon this description by means of 2 See, for example, Butler, Pinski, and Allen (1979), Bauer et al. (1998), Shukla et al. (2003), Lazzeri et al. (2006), Giustino, Cohen, and Louie (2007), Park, Giustino, Cohen, and Louie (2008), and Heid et al. (2010). 3 Throughout this article, when fnk and nqν have the meaning of Fermi-Dirac and Bose-Einstein distributions, respectively, they are defined as follows: f nk ¼ f½ðεnk − εF Þ=kB T with fðxÞ ¼ 1=ðex þ 1Þ, where εF is the Fermi energy; nqν ¼ nðℏωqν =kB TÞ with nðxÞ ¼ 1=ðex − 1Þ. 015003-25 Feliciano Giustino: Electron-phonon interactions from first … a nonadiabatic self-energy. In this section, we adopt a similar strategy in order to discuss electronic excitation energies: first we identify an approximation to the Hedin-Baym equations which does not include any electron-phonon interactions, and then we introduce an electron self-energy to incorporate such interactions. The single most common approximation in first-principles electronic structure calculations is to describe nuclei as classical particles clamped in their equilibrium positions. Within this approximation the expectation value of the nuclear charge density operator in Eq. (67), hn̂n ðrÞi, is replaced by the first term in Eq. (107), n0n ðrÞ. From Eq. (122) we see that this approximation formally corresponds to setting to zero the displacement-displacement correlation function of the nuclei. This observation suggests that, in order to unambiguously single out electron-phonon interactions in the Hedin-Baym equations, we need to define a noninteracting problem by setting Dκαp;κ0 α0 p0 ¼ 0 and identify the electron-phonon interaction with the remainder. In the following, we write an equation of motion for the electrons analogous to Eq. (84), except with the nuclei clamped in their equilibrium positions; then we use a Dyson-like equation to recover the fully interacting electron Green’s function. The equation of motion for the electron Green’s function at clamped nuclei, which we denote as Gcn , reads ∂ ℏ2 2 cn iℏ þ ∇ ð1Þ − V tot ð1Þ Gcn ð12Þ ∂t1 2me Z cn − d3Σcn e ð13ÞG ð32Þ ¼ δð12Þ: ð147Þ Here the potential V cn tot differs from its counterpart V tot of Eq. (79) in that the total density of electrons and nuclei hn̂i is replaced by the density calculated at clamped nuclei hn̂cn i: Z V cn tot ð1Þ ¼ d2vð1; 2Þhn̂cn ð2Þi; ð148Þ where hn̂cn ð1Þi ¼ −iℏ X σ1 Gcn ð11þ Þ þ n0n ðr1 Þ: ð149Þ The term Σcn e in Eq. (147) represents the electronic part of Hedin’s self-energy in Eq. (85), evaluated at clamped nuclei: Z Σcn e ð12Þ ¼ iℏ þ dð34ÞGcn ð13ÞΓcn ð324ÞW cn e ð41 Þ: ð150Þ In this expression, the vertex Γcn and the screened Coulomb interaction W cn e are both evaluated via the Hedin-Baym equations at clamped nuclei. Equations (147)–(150) lead directly to the well-known Hedin’s equations (Hedin, 1965). Hedin’s equations and the associated GW method at clamped nuclei are addressed in a number of excellent reviews (Hedin and Lundqvist, 1969; Hybertsen and Louie, 1986; Aryasetiawan and Gunnarsson, 1998; Onida, Reining, and Rubio, 2002); hence they will not be discussed here. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 In order to recover the complete Hedin-Baym equation of motion, Eq. (84), starting from Eqs. (147)–(150), it is sufficient to introduce the Dyson equation Z Gð12Þ ¼ Gcn ð12Þ þ dð34ÞGcn ð13ÞΣep ð34ÞGð42Þ; ð151Þ together with the electron self-energy Σep arising from electron-phonon interactions Σep ¼ ΣFM þ ΣDW þ ΣdGW ; ð152Þ where Z Σ FM ð12Þ ¼ iℏ dð34ÞGð13ÞΓð324ÞW ph ð41þ Þ; ð153Þ d3vð13Þ½hn̂ð3Þi − hn̂cn ð3Þiδð12Þ; ð154Þ Z ΣDW ð12Þ ¼ ΣdGW ð12Þ ¼ Σe ð12Þ − Σcn e ð12Þ: ð155Þ We emphasize that Eqs. (147)–(155) are just an alternative formulation of the Hedin-Baym equations in Table I. The advantage of this formulation is that it better reflects standard practice, whereby the DFT equations and the GW quasiparticle corrections are evaluated at clamped nuclei. Equations (147)–(155) are formally exact within the harmonic approximation. A schematic representation of the Dyson equation for the electron Green’s function and the decomposition of the electron self-energy are given in Fig. 2. The self-energy contribution ΣFM in Eq. (153) is a dynamic correction to the electronic excitation energies and is analogous to the GW self-energy at clamped nuclei. Indeed, in the same way as the correlation part of the standard GW self-energy describes the effect of the dynamic electronic polarization upon the addition of electrons or holes to the system, the term GW ph in Eq. (153) describes the effect of the dynamic polarization of the lattice. In the semiconductor community, the self-energy obtained from Eq. (153) by setting Γð123Þ ¼ δð13Þδð23Þ is commonly referred to as the Fan self-energy (Fan, 1951; Allen and Heine, 1976; Allen and Cardona, 1981; Cardona, 2001). In the metal and superconductor communities, the same term is traditionally referred to as the self-energy in the Migdal approximation (Migdal, 1958; Engelsberg and Schrieffer, 1963; Scalapino, 1969; Schrieffer, 1983). By extension we refer to the self-energy ΣFM in Eq. (153) as the “Fan-Migdal” (FM) self-energy. The static term ΣDW in Eq. (154) corresponds to the difference between the self-consistent potential V tot calculated for the fully interacting system and the same potential evaluated with the nuclei clamped in their equilibrium positions V cn tot . Intuitively this term corresponds to a timeindependent correction to the “crystal potential” that arises from the fuzziness of the nuclear charge density around the equilibrium nuclear positions. This term is similar to the one appearing in the study of the temperature dependence of x-ray 015003-26 Feliciano Giustino: Electron-phonon interactions from first … corresponds to a fraction of the GWΓ quasiparticle corrections at clamped nuclei. Since ΣdGW has never been investigated so far, we will not discuss this term further. 2. Expressions for the electron self-energy used in ab initio calculations A complete self-consistent solution of Eqs. (147)–(155) from first principles is not possible at present, and one has to replace the various entries of Eq. (152) by the best approximations available. In practice, one resorts either to DFT or to GW calculations; recent progress is reviewed in Secs. VIII and IX. Using Eqs. (110), (130), (131), and (144) we can rewrite the Fan-Migdal self-energy as follows: ΣFM ð12Þ X Z dω dq þ ¼i dð34Þe−iωðt4 −t1 Þ 2π ΩBZ νν0 × Gð13ÞΓð324Þgcc qν ðr4 ; ωÞ × Dqνν0 ðωÞgqν0 ðr1 ; ωÞ: FIG. 2. Diagrammatic representation of the electron Green’s function and electron-phonon self-energy. (a) Dyson equation for the electron Green’s function, Eq. (151). The thick straight line represents the fully dressed electron propagator, the thin straight line is the propagator calculated at clamped nuclei, and the disk is the electron-phonon self-energy. (b) Decomposition of the electron-phonon self-energy into Fan-Migdal self-energy, Eq. (153), Debye-Waller contribution, Eq. (154), and the remainder given by Eq. (155). (c) Fan-Migdal electron-phonon selfenergy expressed in terms of the dressed electron-phonon coupling function (dark gray disk as in Fig. 1), the fully interacting electron Green’s functions (thick straight line), the fully interacting phonon propagator (thick wavy line), and the vertex Γ from Eq. (83). (d) Debye-Waller contribution resulting from the fully interacting phonon propagator (thick wavy line) and the matrix element in Eq. (40) (hatched disk). (e) Correction to Hedin’s GW self-energy arising from the modification of the electronic structure induced by the electron-phonon interaction. W e is the screened Coulomb interaction of Eq. (94) (bold dashed double line). W cn e is the screened Coulomb interaction evaluated at clamped nuclei (thin dashed double line). Γcn is the vertex of Eq. (83), but evaluated at clamped nuclei. diffraction and neutron diffraction spectra (Mermin, 1966; Ashcroft and Mermin, 1976) and is commonly referred to as the Debye-Waller term (Antončík, 1955; Walter et al., 1970; Cardona and Thewalt, 2005). Hedin and Lundqvist (1969) did not include this term in their classic work; however, this contribution was discussed by Allen and Heine (1976) [see also Allen (1978)]. The last term Eq. (152), ΣdGW , is the correction to the standard Hedin self-energy arising from the fact that the fully interacting electron Green’s function and density are slightly different from those evaluated at clamped nuclei, owing to the electron-phonon interaction. The magnitude of this term Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 ð156Þ This shows that the Fan-Migdal self-energy is, in symbolic notation, of the type Σ ¼ g2 DGΓ; a graphical representation of this term is given in Fig. 2(c). In order to make Eq. (156) amenable to ab initio calculations, it is common to make the following approximations, which are similar to those introduced earlier for the phonon self-energy: (i) The vertex Γð123Þ is set to δð13Þδð23Þ. (ii) The fully interacting electron Green’s function is replaced by the Kohn-Sham Green’s function evaluated at clamped nuclei. (iii) The fully interacting phonon propagator Dqνν0 ðωÞ is replaced by the adiabatic propagator DA qνν0 ðωÞ from Eq. (134). (iv) The screened electron-phonon vertex is evaluated using the RPA þ xc electronic screening from a DFT calculation. (v) The frequency dependence of the electron-phonon coupling is neglected, gqν ðr; ωÞ ≃ gqν ðr; 0Þ. After using these approximations in Eq. (156), we obtain the following result for the k ¼ k0 matrix elements of the Fan-Migdal self-energy in the basis of Kohn-Sham states: ΣFM nn0 k ðωÞ ¼ Z 1X dq g ðk; qÞgmn0 ν ðk; qÞ ℏ mν ΩBZ mnν 1 − fmkþq × ω − εmkþq =ℏ − ωqν þ iη fmkþq þ : ω − εmkþq =ℏ þ ωqν − iη ð157Þ Here f mkþq ¼ 1 for occupied Kohn-Sham states and 0 otherwise, and the matrix element gmnν ðk; qÞ is obtained from Eq. (38). As for the phonon self-energy in Eq. (145), in this case the components of the electron self-energy for k ≠ k0 also vanish due to the periodicity of the lattice. The result in Eq. (157) is obtained by closing the contour of the frequency integration in the upper complex plane, owing to 015003-27 Feliciano Giustino: Electron-phonon interactions from first … the tþ 1 in the exponential of Eq. (156). The infinitesimals inside the electron and phonon propagators, which reflect the time ordering, are crucial to obtain the correct result (Schrieffer, 1983). The spin label is omitted in Eq. (157) since this contribution to the self-energy is diagonal in the spin indices. This result is valid only at zero temperature. The extension to finite temperature requires going through the Matsubara representation and then continuing the self-energy from the imaginary axis to the real axis. The procedure is described in many textbooks; see, for example, Sec. 3.5 of Mahan (1993). The result is that at finite temperature the square brackets of Eq. (157) are to be modified as follows: 1 − fmkþq fmkþq þ þ iη − iη 1 − fmkþq þ nqν fmkþq þ nqν þ ; → þ iη þ iη ð158Þ where fmkþq and nqν are now Fermi-Dirac and Bose-Einstein distribution functions, respectively (see footnote 3). The change of sign in the imaginary infinitesimal on the second fraction has to do with the fact that in the Matsubara formalism the analytic continuation from the imaginary frequency axis to the real axis through the upper complex plane leads to the socalled retarded self-energy, that is, a self-energy with all poles below the real axis (Abrikosov, Gor’kov, and Dzyaloshinski, 1975; Mahan, 1993). The Debye-Waller term in Eq. (154) can also be written in a form which is convenient for practical calculations by expanding the total density operator n̂ð3Þ to second order in the atomic displacements. Using Eqs. (79) and (109) we find ΣDW ð12Þ ¼ δð12Þ iℏ X ∂ 2 V tot ð1Þ þ 0 0 0 ðt ; t Þ: D 2 καp ∂τ0καp ∂τ0κ0 α0 p0 καp;κ α p 1 1 κ0 α0 p0 ð159Þ In order to arrive at this result, it is necessary to make the additional approximation that the electronic field operators and the operators for the nuclear displacements are uncorrelated, that is hn̂Δτ̂καp i ¼ hn̂ihΔτ̂καp i, and similarly for the second power of the displacements. This requirement was noted by Gillis (1970) and is trivially satisfied if we describe phonons within the adiabatic approximation of Sec. V.A.1. Equation (159) motivates the diagrammatic representation of the Debye-Waller self-energy shown in Fig. 2(d), whereby the phonon line begins and ends at the same time point. Note that Eq. (159) involves the variation of the screened potential V tot ; this result, which we derived here starting from Schwinger’s functional derivative technique, is also obtained when starting from a perturbative diagrammatic analysis (Marini, Poncé, and Gonze, 2015). The Debye-Waller self-energy can be simplified further if we make use of the following approximations, in the same spirit as for the Fan-Migdal self-energy: (vi) The fully interacting phonon propagator is replaced by the adiabatic propagator DA qνν0 ðωÞ from Eq. (134). Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 (vii) The total many-body potential V tot of Eq. (79) is replaced by the Kohn-Sham potential V KS ðrÞ evaluated at clamped nuclei. Strictly speaking, the Kohn-Sham effective potential also includes contributions from exchange and correlation, which in the Hedin-Baym equations are all contained in the electron self-energy. However, the present discussion is unchanged if we add any local and frequencyindependent potential to V tot in Eq. (84), while removing the same potential from the self-energy (Keating, 1968). Using these simplifications together with Eqs. (130) and (131), we can write the ΣDW in the basis of Kohn-Sham eigenstates as follows: X Z dq DW gDW0 ðk; q; −qÞ; ð160Þ Σnn0 k ¼ ΩBZ nn νν ν where the Debye-Waller matrix element gDW is obtained from Eq. (40), and the presence of only the diagonal terms ν ¼ ν0 is a result of the Kronecker delta in Eq. (132). In going from Eq. (159) to Eq. (160) the frequency integration is performed by using Eq. (134), after closing the contour in the lower half plane. The resulting expression is diagonal in the spin indices. The expression for the Debye-Waller term in Eq. (160) is valid only at zero temperature. In this case the extension to finite temperature is immediate since the self-energy does not involve the electron Green’s function; hence we need to evaluate only the canonical average of Eq. (133) at equal times. The result is that Eq. (160) is simply to be modified as follows: DW gDW nn0 νν ðk; q; −qÞ → gnn0 νν ðk; q; −qÞð2nqν þ 1Þ; ð161Þ with nqν the Bose-Einstein occupations (see footnote 3). The Debye-Waller contribution to the electron self-energy is almost invariably ignored in the literature on metals and superconductors, but it is well known in the theory of temperature-dependent band structures of semiconductors (Allen and Heine, 1976; Allen and Cardona, 1981; Marini, 2008; Giustino, Louie, and Cohen, 2010; Faber et al., 2011). Neglecting ΣDW in metals is partly justified by the fact that this term is frequency independent; therefore it is expected to be a slowly varying function over each Fermi-surface sheet. A detailed first-principles analysis of this aspect is currently lacking. 3. Temperature dependence of electronic band structures Once the electron self-energy has been determined as in Sec. V.B.2, it is possible to study the modification of the electronic structure induced by the EPI. To this aim it is convenient to rewrite Eq. (151) in the basis of Kohn-Sham eigenstates as follows: ep cn;−1 G−1 nn0 k ðωÞ ¼ Gnn0 k ðωÞ − Σnn0 k ðωÞ: ð162Þ Assuming that the electronic structure problem at clamped nuclei has been solved using DFT or DFT þ GW calculations, 015003-28 Feliciano Giustino: Electron-phonon interactions from first … the Green’s function Gcn can be written in terms of simple poles at the Kohn-Sham or quasiparticle eigenvalues εnk (Hedin and Lundqvist, 1969). In this case Eq. (162) reduces to ~ nk Þδnn0 − Σep G−1 nn0 k ðωÞ ¼ ðℏω − ε nn0 k ðωÞ; ð163Þ where ε~ nk ¼ εnk iℏη with the upper and lower signs corresponding to occupied and unoccupied states, respectively. The spin indices are omitted since these self-energy contributions do not mix states with opposite spin. In order to gain insight into the effects of the electronphonon interaction, we start from the approximation that Σep leads only to a small shift of the quasiparticle poles, from the noninteracting energies εnk to the renormalized energies E~ nk ¼ Enk þ iΓnk . In this approximation, the fully interacting Green’s function is expressed as a sum of simple poles, given by the zeros of Eq. (163): ~ Enk ¼ εnk þ ReΣep nnk ðEnk =ℏÞ; ð164Þ ~ Γnk ¼ ImΣep nnk ðEnk =ℏÞ: ð165Þ As in the case of vibrational frequencies in Eq. (137), we are considering for simplicity nondegenerate electronic states and making the assumption that the off-diagonal elements of the 0 self-energy Σep nn0 k with n ≠ n can be neglected. In more general situations the right-hand side of Eq. (163) needs to be diagonalized, or alternatively the off-diagonal terms Σep nn0 k need to be treated perturbatively. The energies Enk obtained from Eq. (164) yield the band structure renormalized by the EPIs, to be discussed later. The imaginary part Γnk in Eq. (165) is connected with the quasiparticle lifetimes and is discussed in Sec. V.B.4. Equation (164) is to be solved self-consistently for Enk and Γnk . When Eq. (164) is used in combination with the standard approximations to the Fan-Migdal and Debye-Waller selfenergies given by Eqs. (157) and (160), the result that one obtains is equivalent to describing electron-phonon couplings to second order in the Brillouin-Wigner perturbation theory (Mahan, 1993). Similarly one recovers the more basic Rayleigh-Schrödinger perturbation theory by making the replacements Enk → εnk and Γnk → 0 in Eq. (164). By combining Eqs. (157) and (158), (160) and (161), and (164), we obtain the temperature-dependent “band structure renormalization” arising from the EPI: Enk ¼ εnk þ X Z dq X jgmnν ðk; qÞj2 Ω BZ ν m 1 − fmkþq þ nqν Enk − εmkþq − ℏωqν þ iΓnk fmkþq þ nqν þ Enk − εmkþq þ ℏωqν þ iΓnk X Z dq þ gDW nnνν ðk; q; −qÞð2nqν þ 1Þ: Ω BZ ν For practical calculations it is important to bear in mind that this result rests on the approximations (i)–(vii) introduced previously, as well as the harmonic approximation. The theory of temperature-dependent band structures developed by Allen and Heine (1976) makes two additional approximations in addition to Eq. (166): the Brillouin-Wigner perturbation theory is replaced by the Rayleigh-Schrödinger perturbation theory, and the phonon energies in the denominators are neglected. Using these additional approximations Eq. (166) becomes Enk X Z dq X jgmnν ðk; qÞj2 ¼ εnk þ ΩBZ m εnk − εmkþq ν þ gDW ðk; q; −qÞ ð2nqν þ 1Þ; nnνν ð167Þ which is referred to as the “adiabatic Allen-Heine formula.” By setting T ¼ 0 the Bose-Einstein factors nqν vanish and we have the so-called “zero-point renormalization” of the energy bands ΔEZP nk ¼ Enk ðT ¼ 0Þ − εnk . This is the modification of the electronic energies evaluated at clamped nuclei, which arises from the zero-point fluctuations of the atoms around their equilibrium sites. An expression that is essentially identical to Eq. (167) can also be obtained directly from Eq. (1) using second-order Raleigh-Schrödinger perturbation theory in Fock space, following the same lines as in Kittel (1963). A detailed derivation of the formalism starting from Eq. (1) was given by Chakraborty and Allen (1978). Historically, the Allen-Heine theory (Allen and Heine, 1976) was developed by starting from a straightforward perturbation theory expansion of the electron energies in terms of the atomic displacements within the adiabatic approximation, followed by a canonical average of the displacements using Bose-Einstein statistics. It is reassuring that, after making a few well-defined approximations, a fieldtheoretic method leads to the same result. Equation (167) was employed in many semiempirical calculations.4 More recently, this expression was used in the context of first-principles DFT calculations by Marini (2008) and Giustino, Louie, and Cohen (2010). DFT calculations of band structure renormalization based on Eqs. (166) or (167) are becoming increasingly popular, and the latest developments are reviewed in Sec. IX.A.1. The nature of the band structure renormalization by electron-phonon interactions can be understood at a qualitative level by considering a drastically simplified model, consisting of a semiconductor with parabolic and nondegenerate valence and conduction bands, with the band extrema coupled to all other states by a dispersionless phonon mode of frequency ω0. If the Debye-Waller matrix elements are much × Re Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 4 ð166Þ See, for example, Allen and Cardona (1981, 1983), Lautenschlager, Allen, and Cardona (1985), Gopalan, Lautenschlager, and Cardona (1987), Zollner, Cardona, and Gopalan (1992), and Olguín, Cardona, and Cantarero (2002). Detailed reviews of early calculations and comparison to experiments can be found in Cardona (2001, 2005) and Cardona and Thewalt (2005). 015003-29 Feliciano Giustino: Electron-phonon interactions from first … band gap renormalization at very low temperature. These effects were recently investigated by Allen and Nery (2017). 4. Carrier lifetimes FIG. 3. Temperature-dependent band gap and lifetimes in an idealized semiconductor or insulator. (a) Temperature dependence of the band gap according to Eq. (168) (thick solid blue line). The straight thin black line is the asymptotic expansion at high temperature; this line intercepts the vertical axis at the band gap calculated with clamped nuclei Ecn g . The difference between the latter value and the band gap at T ¼ 0 including the EPI gives the zero-point renormalization ΔEZP g . (b) Temperature dependence of the electron linewidth (solid blue line) and lifetimes (dashed red line) using the same model as in (a). The zero-point broadening is ΓZP nk . This simplified trend is valid only when the electron energy is at least one phonon energy away from a band extremum, so that both phonon emission and phonon absorption processes are allowed. The parameters of the model are Ecn g ¼ ZP ¼ 100 meV, ℏω ¼ 100 meV, and Γ ¼ 50 meV. 1 eV, ΔEZP g 0 nk These values are representative of common semiconductors. smaller than the Fan-Migdal matrix elements, then the dominant contributions to Eq. (167) arise from denominators such as εnk − εnkþq ≃ ℏ2 jqj2 =2mn , where the upper and lower signs are for the valence and conduction bands, respectively, and mn are the effective masses. As a result the temperature dependence of the band gap takes the form ZP Eg ðTÞ ¼ Ecn g − jΔEg j½1 þ 2nðℏω0 =kB TÞ; ð168Þ ZP where Ecn g is the gap at clamped nuclei and jΔEg j is the zeropoint correction. The negative sign in Eq. (168) arises from the curvatures of the valence and conduction bands. In this example the band gap decreases with temperature: this is a well-known effect in semiconductor physics and is often referred to as the “Varshni effect” (Varshni, 1967). The first measurements of such effects were performed by Becker and Fan (1949) and stimulated the development of the first theory of temperature-dependent band gaps (Fan, 1951). A schematic illustration of this qualitative model is provided in Fig. 3(a). The redshift of the gap as a function of temperature is seen in many, albeit not all, semiconductors. For example, copper halides (Göbel et al., 1998) and lead halide perovskites (D’Innocenzo et al., 2014) exhibit an “inverse Varshni” effect, that is, a blueshift of the gap with temperature; in addition, some chalcopyrites exhibit a nonmonotonic temperature dependence of the band gap (Bhosale et al., 2012). We also point out that the qualitative model shown in Fig. 3(a) does not take into account the subtle temperature dependence of the Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 While the real part of the poles in Eq. (164) describes the energy level renormalization induced by the electron-phonon coupling, the imaginary part Γnk in Eq. (165) carries information on the spectral broadening, discussed in Sec. V.B.5, and on quasiparticle lifetimes, which we discuss next. After transforming Gnn0 k ðωÞ from Eq. (163) into the time domain it is seen that, for an electron or hole added to the system at time t in the state jnki, the probability amplitude to persist in the same state decreases as exp½Γnk ðt0 − tÞ=ℏ. Using Eqs. (157) and (165) it can be seen that Γnk < 0 for an electron added to the system and Γnk > 0 for a hole. Therefore the average time spent by the particle in the state jnki is τnk ¼ ℏ=ð2jΓnk jÞ. A popular expression for the electron and hole lifetimes is obtained by making the replacement E~ nk → εnk in Eq. (157) and by taking the absolute value of the imaginary part. We find 1 2π X ¼ τnk ℏ mν Z dq jg ðk; qÞj2 ΩBZ nmν × jð1 − fmkþq Þδðεnk − ℏωqν − εmkþq Þ − f mkþq δðεnk þ ℏωqν − εmkþq Þj: ð169Þ A more accurate expression is discussed after Eq. (174). The extension of this result to finite temperature is obtained by taking the absolute value of the imaginary part of Eq. (158): 1 2π X ¼ τnk ℏ mν Z dq jg ðk; qÞj2 ΩBZ nmν × ½ð1 − fmkþq þ nqν Þδðεnk − ℏωqν − εmkþq Þ þ ðf mkþq þ nqν Þδðεnk þ ℏωqν − εmkþq Þ: ð170Þ We emphasize that the change of sign in the third line results from the analytic continuation to the retarded self-energy. Equation (170) coincides with the expression that one would obtain by using the standard Fermi golden rule (Grimvall, 1981). The intuitive interpretation of this result is that the quasiparticle lifetime is reduced by processes of phonon emission and absorption, corresponding to the second and third lines of Eq. (170), respectively. We note that in deriving Eq. (170) we did not consider the Debye-Waller self-energy. This is because the diagonal matrix elements of ΣDW are purely real; hence they do not contribute to the quasiparticle widths (Lautenschlager, Allen, and Cardona, 1986). Ab initio calculations of carrier lifetimes using Eq. (170) were first reported by Eiguren et al. (2002) and Eiguren, de Gironcoli et al. (2003). These applications and more recent developments are reviewed in Sec. X.A. If we evaluate Eq. (170) for the same simplified model introduced for the temperature renormalization, and we neglect the phonon energy in the Dirac delta functions, we ZP obtain Γnk ðTÞ ¼ ΓZP nk ½1 þ 2nðℏω0 =kB TÞ, where Γnk is the linewidth at T ¼ 0. The dependence of the linewidth and the corresponding lifetime on temperature for this model are 015003-30 Feliciano Giustino: Electron-phonon interactions from first … shown in Fig. 3(b). This trend is typical in semiconductors (Lautenschlager, Garriga, Logothetidis, and Cardona, 1987; Lautenschlager, Garriga, Vina, and Cardona, 1987). 5. Kinks and satellites In many cases of interest, the use of the Brillouin-Wigner perturbation theory as given by Eqs. (164) and (165) is not sufficient to provide an adequate description of EPIs, and it becomes necessary to go back to the complete Dyson equation (163). Generally speaking a direct solution of the Dyson equation is important in all those cases where the electronic energy scales are comparable to phonon energies, namely, in metals (including superconductors), narrow-gap semiconductors, and doped semiconductors. In order to study these systems, it is convenient to introduce an auxiliary function called the “spectral density function” or simply spectral function. In its simplest version the spectral function is defined as (Abrikosov, Gor’kov, and Dzyaloshinski, 1975; Mahan, 1993) Aðk; ωÞ ¼ − 1X ImGret nnk ðωÞ; π n ð171Þ where the superscript “ret” stands for “retarded” and simply indicates that all poles of the Green’s function Gnn0 k ðωÞ in the upper complex plane must be replaced by their complex conjugate. The spectral function is positive definite and carries the meaning of a many-body momentum-resolved density of states (Abrikosov, Gor’kov, and Dzyaloshinski, 1975). This is precisely the function that is probed by angle-resolved photoelectron spectroscopy experiments (ARPES) (Damascelli, Hussain, and Shen, 2003). Using Eq. (163) the spectral function can be rewritten as Aðk; ωÞ ¼ X n The result expressed by Eq. (173) shows that, in a rigorous field-theoretic approach, the quasiparticle broadening and lifetime given by Eqs. (169) and (170) should be renormalized by Znk and Z−1 nk , respectively, and should be evaluated using the quasiparticle energy Enk instead of εnk . This result can also be derived from Eq. (165) by performing a Taylor expansion of the self-energy along the imaginary axis and using the Cauchy-Riemann conditions. In order to illustrate the typical features of the spectral function, we consider a model system characterized by one parabolic conduction band. The occupied electronic states couple to all states within an energy cutoff via a dispersionless phonon mode and a constant electron-phonon matrix element. A simplified version of this model was discussed by Engelsberg and Schrieffer (1963) by considering a constant density of electronic states. By evaluating the spectral function in Eq. (172) using the Fan-Migdal self-energy and neglecting the Debye-Waller term, we obtain the results shown in Fig. 4 for two sets of parameters. In Fig. 4(a) the Fermi energy is much larger than the characteristic phonon energy. This case is representative of a metallic system with electron bands nearly linear around the Fermi level. Here the electron-phonon interaction leads to (i) a reduction of the band velocity in proximity of the Fermi level, and (ii) a broadening of the spectral function beyond the phonon energy ℏω0. A detailed analysis of these features for a slightly simpler model system, including a discussion of the analytic properties of the Green’s function, can be found in the work by Engelsberg and Schrieffer. −ð1=πÞImΣep nnk ðωÞ : 2 2 ðωÞ þ ½ImΣep ½ℏω − εnk − ReΣep nnk nnk ðωÞ ð172Þ In order to obtain the correct spectral function, it is important to use the retarded self-energy. This is done by using Eq. (158) for the Fan-Migdal term, while the static Debye-Waller term remains unchanged. It is often convenient to approximate the spectral function as a sum of quasiparticle peaks. To this aim, one performs a linear expansion of Eq. (172) around each quasiparticle energy Enk to obtain Aðk; ωÞ ¼ X Znk n −ð1=πÞZnk ImΣep nnk ðEnk =ℏÞ : 2 ½ℏω − Enk 2 þ ½Znk ImΣep nnk ðEnk =ℏÞ ð173Þ This is a sum of Lorentzians with strength Znk and width Znk ImΣep nnk ðEnk =ℏÞ. Here the “quasiparticle strength” is defined as the homonymous quantity appearing in GW calculations (Hedin and Lundqvist, 1969): −1 Znk ¼ ½1 − ℏ−1 ∂ReΣep nnk ðωÞ=∂ωjω¼Enk =ℏ : Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 ð174Þ FIG. 4. Two-dimensional maps of the electron spectral function Aðk; ωÞ for electrons coupled to a dispersionless phonon of frequency ω0. The noninteracting bands are given by εðkÞ ¼ −εF þ ℏ2 jkj2 =2m , and the Fermi level coincides with the top of the energy window. The matrix element is jgj2 ¼ ℏω0 =N F when the electron energies differ by less than the cutoff εmax and zero otherwise (N F is the density of states at the Fermi level). (a) Spectral function for the case εF ¼ 10ℏω0 (white on blue, black), noninteracting band structure (solid line, yellow, light gray), and fully interacting band structure within the Brillouin-Wigner perturbation theory (solid line, red, dark gray). (b) Spectral function for the case εF ¼ 2ℏω0 . The model parameters are m ¼ 0.1me , ℏω0 ¼ 100 meV, η ¼ 20 meV, and εc ¼ 5 eV. For clarity the calculated spectral functions are cut off at the value 3 eV−1 and normalized. The self-energy is shifted by a constant so as to have Σep ð0Þ ¼ 0. This correction guarantees the fulfillment of Luttinger’s theorem about the volume enclosed by the Fermi surface (Luttinger, 1960). 015003-31 Feliciano Giustino: Electron-phonon interactions from first … The solid line (red, dark gray) in Fig. 4(a) shows the renormalized band structure obtained from the BrillouinWigner perturbation theory, Eq. (164). We see that these solutions track the maxima of the spectral function Aðk; ωÞ. The renormalized bands exhibit a characteristic S shape near the Fermi level, corresponding to multiple solutions of Eq. (164) for the same wave vector k. Starting from the late 1990s such S-shaped energy-momentum dispersion curves have been observed in a number of ARPES experiments and have become known in the literature as the “photoemission kink” (Valla, Fedorov, Johnson, and Hulbert, 1999). Firstprinciples calculations of kinks were first reported by Eiguren, de Gironcoli et al. (2003) and Giustino, Cohen, and Louie (2008) and are reviewed in Sec. VIII. In Fig. 4(b) the Fermi energy is comparable to the characteristic phonon energy. This case is representative of a degenerately doped semiconductor close to a conduction band minimum. Here the electron-phonon interaction leads to two distinct spectral features: (i) a parabolic band with a heavier mass, which is well described by the Brillouin-Wigner solutions (solid line, red, dark gray), and (ii) a polaron satellite that is visible farther down. In this example, it is clear that Eq. (164) is unable to describe the satellite and that the spectral function carries qualitatively new information about the system. Polaron satellites resembling Fig. 4(b) have been observed in ARPES experiments on doped oxides (Moser et al., 2013; Chen et al., 2015; Cancellieri et al., 2016; Wang et al., 2016) and were recently calculated from first principles (Verdi, Caruso, and Giustino, 2017). 6. Model Hamiltonians, polarons, and the cumulant expansion At the end of this section it is worth mentioning complementary non-first-principles approaches for studying the effects of EPIs on the electronic properties of solids. Model EPI Hamiltonians can be derived from Eq. (1) by choosing a priori explicit expressions for the electron band energies, the vibrational frequencies, and the coupling matrix elements. Examples of model Hamiltonians are those of Fröhlich (1954), Holstein (1959), and Su, Schrieffer, and Heeger (1979), the Hubbard-Holstein model (Berger, Valášek, and von der Linden, 1995), the Peierls-Hubbard model (Campbell, DeGrand, and Mazumdar, 1984), the t-J Holstein model (Rösch and Gunnarsson, 2004), and the Su-SchriefferHeeger-Holstein model (Perroni et al., 2004). These models involve the tight-binding approximation, the Einstein phonon spectrum, and electron-phonon couplings to first order in the atomic displacements. Using these model Hamiltonians it is possible to go beyond the approximations introduced in Sec. V.B.2 and obtain nonperturbative solutions by means of canonical Lang-Firsov transformations, path-integral methods, exact diagonalization, and variational or quantum Monte Carlo techniques (Alexandrov, 2008; Alexandrov and Devreese, 2010). These models have been used extensively to explore many aspects of polaron physics, for example, the ground-state energy of polarons (weak or strong coupling), their spatial extent (large or small polarons), and transport properties (bandlike or hoppinglike). Given the considerable body of literature on model EPI Hamiltonians, it is natural to ask whether one could bring Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 ab initio calculations of EPIs to a similar level of sophistication. The main limitation of current first-principles approaches is that, given the complexity of the calculations, the electron self-energies are evaluated using the bare propagators, as in Eq. (157). As a consequence, higher-order interaction diagrams beyond the Migdal approximation (Migdal, 1958) are omitted altogether. A promising avenue for going beyond the Migdal approximation consists of introducing higher-order diagrams via the “cumulant expansion” approach (Hedin and Lundqvist, 1969; Langreth, 1970; Aryasetiawan, Hedin, and Karlsson, 1996). In the cumulant expansion method, instead of calculating the electron Green’s function via a Dyson equation, one evaluates the time evolution of the Green’s function by formulating the problem in the interaction picture, in symbols Gnnk ðtÞ ¼ ði=ℏÞ exp½−iðεnk =ℏÞt þ Cnnk ðtÞ (Aryasetiawan, Hedin, and Karlsson, 1996). The distinctive advantage of this approach is that the cumulant Cnnk ðtÞ can be obtained from a low-order self-energy, for example, the Fan-Migdal self-energy in Eq. (157), and the exponential “resummation” automatically generates higher-order diagrams (Mahan, 1993). Detailed discussions of the cumulant expansion formalism are given by Zhou et al. (2015) and Gumhalter et al. (2016). The cumulant method provides an interesting point of contact between ab initio and model Hamiltonian approaches. In fact, the cumulant expansion is closely related to the “momentum average approximation” introduced by Berciu (2006) for studying the Green’s function of the Holstein polaron. The cumulant expansion has proven successful in ab initio calculations of electron-electron interactions, in particular, valence band satellites in semiconductors (Kheifets et al., 2003; Guzzo et al., 2011, 2012, 2014; Lischner, Vigil-Fowler, and Louie, 2013; Kas, Rehr, and Reining, 2014; Caruso and Giustino, 2015; Caruso, Lambert, and Giustino, 2015). In the context of EPIs, the ab initio cumulant expansion method was applied to elemental metals by Story et al. (2014), and to the ARPES spectra of n-doped TiO2 by Verdi, Caruso, and Giustino (2017). In the latter work the cumulant method correctly reproduced the polaron satellites observed in the experiments of Moser et al. (2013). The study of polarons using ab initio many-body techniques is yet to begin. However, a first calculation of the spectral function of Fröhlich polarons and an approximate polaron wave function were recently reported by Verdi, Caruso, and Giustino (2017). VI. EFFICIENT CALCULATIONS OF MATRIX ELEMENTS AND THEIR INTEGRALS The study of EPIs from first principles requires evaluating Brillouin-zone integrals of functions that exhibit strong fluctuations. This requirement can be appreciated by inspecting Eqs. (145) and (157): there the denominators become large whenever the difference between two electronic eigenvalues approaches a phonon energy. As a result, while in DFT total energy calculations the Brillouin zone is typically discretized using meshes of the order of 10 × 10 × 10 points, the numerical convergence of EPI calculations requires much finer grids, sometimes with as many as 106 wave vectors 015003-32 Feliciano Giustino: Electron-phonon interactions from first … (Giustino, Cohen, and Louie, 2007; Poncé et al., 2015). Determining vibrational frequencies ωqν and perturbations Δqν vKS ðrÞ for such a large number of wave vectors is a prohibitive task, since every calculation is roughly as expensive as one total energy minimization. These difficulties stimulated the development of specialized numerical techniques for making calculations of EPIs affordable. In the following sections two such techniques are reviewed: electron-phonon Wannier interpolation and Fermi-surface harmonics. A. Wannier interpolation 1. Maximally localized Wannier functions In addition to the standard description of electrons in solids in terms of Bloch waves, as in Eq. (29), it is possible to adopt an alternative point of view whereby electrons are described as linear combinations of localized orbitals called “Wannier functions” (Wannier, 1937). The most general relation between Wannier functions and Bloch waves can be written as follows. One considers electron bands εnk with eigenfunctions ψ nk , where the index n is restricted to a set of bands that are separated from all other bands by finite energy gaps above and below. These bands are referred to as “composite energy bands” (Marzari and Vanderbilt, 1997). Wannier functions are defined as wmp ðrÞ ¼ N −1 p X eik·ðr−Rp Þ Unmk unk ðrÞ; ð175Þ nk where Unmk is a unitary matrix in the indices m and n. From this definition and Eq. (A1) it follows that Wannier functions are normalized in the supercell hwmp jwm0 p0 isc ¼ δmp;m0 p0 . Furthermore, since unk is lattice periodic, Wannier functions have the property wmp ðrÞ ¼ wm0 ðr − Rp Þ. The inverse transformation of Eq. (175) is obtained by using the unitary character of U nmk together with Eq. (A1): unk ðrÞ ¼ X e−ik·ðr−Rp Þ U†mnk wmp ðrÞ: ð176Þ mp The unitary matrix U nmk is completely arbitrary, and therefore there exists considerable freedom in the construction of Wannier functions. For example, by requiring that U nm;−k ¼ U nmk one can make Wannier functions real valued. Marzari and Vanderbilt exploited this degree of freedom to construct Wannier functions that are maximally localized. A comprehensive and up-to-date review of the theory and applications of maximally localized Wannier functions (MLWFs) is given by Marzari et al. (2012). Here we recall only that, in order to minimize the spatial extent of a function in a periodic solid, one needs to use a modified definition of the position operator, since the standard position operator is unbounded in an infinite crystal. This procedure is now well established and it is linked to the development of the modern theory of dielectric polarization (King-Smith and Vanderbilt, 1993; Resta, 1994). Nowadays it is possible to determine MLWFs routinely (Mostofi et al., 2008). The original algorithm of Marzari and Vanderbilt (1997) was also extended to Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 deal with situations where a composite set of bands cannot be identified. This happens notably in metals for electronic states near the Fermi energy. For these cases, Souza, Marzari, and Vanderbilt (2001) developed a band “disentanglement” procedure, which extracts a subset of composite bands out of a larger set of states. For the purposes of this article, the most important property of MLWFs is that they are exponentially localized in insulators in the sense that jwm0 ðrÞj ∼ jrj−α expð−hjrjÞ for large jrj, with α; h > 0 real parameters. This property was demonstrated in one spatial dimension by Kohn (1959a) and He and Vanderbilt (2001), and in two and three dimensions by Brouder et al. (2007), under the condition that the system exhibits time-reversal symmetry. In the case of metallic systems, no exponential localization is expected. However, the Wannier functions obtained in metals using the disentanglement procedure of Souza, Marzari, and Vanderbilt (2001) are typically highly localized. MLWFs are usually comparable in size to atomic orbitals, and this makes them ideally suited for the Slater-Koster interpolation of band structures as shown by Souza, Marzari, and Vanderbilt (2001). This concept was successfully employed in a number of applications requiring accurate calculations of band velocities, effective masses, density of states, Brillouin-zone integrals, and transport coefficients (Wang et al., 2006, 2007; Yates et al., 2007; Pizzi et al., 2014). 2. Interpolation of electron-phonon matrix elements Wannier functions were introduced in the study of EPIs by Giustino, Cohen, and Louie (2007) and Giustino et al. (2007). The starting point is the following definition of the electronphonon matrix element in the Wannier representation5: gmnκα ðRp ; Rp0 Þ ¼ hwm0 ðrÞj ∂V KS ðr − Rp0 Þjwn0 ðr − Rp Þisc ; ∂τκα ð177Þ where the subscript “sc” indicates that the integral is over the BvK supercell. The relation between these quantities and the standard EPI matrix elements gmnν ðk; qÞ is found by replacing Eq. (176) inside Eq. (38) and using Eqs. (34) and (35) (Giustino, Cohen, and Louie, 2007): gmnν ðk; qÞ ¼ X eiðk·Rp þq·Rp0 Þ pp0 × X m0 n0 κα U mm0 kþq gm0 n0 κα ðRp ; Rp0 ÞU †n0 nk uκα;qν ; ð178Þ where uκα;qν ¼ ðℏ=2M κ ωqν Þ1=2 eκα;ν ðqÞ and eκα;ν ðqÞ are the vibrational eigenmodes of Eq. (15). The inverse relation is We note that gmnκα ðRp ; Rp0 Þ has dimensions of energy by length, at variance with Eq. (38). For consistency here we use a definition that differs from that given in Giustino, Cohen, and Louie (2007) by a factor N p ; this factor is inconsequential. 015003-33 5 Feliciano Giustino: Electron-phonon interactions from first … gmnκα ðRp ; Rp0 Þ ¼ 1 X −iðk·Rp þq·Rp0 Þ e N p N p0 k;q X † × u−1 κα;qν U mm0 kþq gm0 n0 ν ðk; qÞU n0 nk ; m 0 n0 ν ð179Þ −1=2 e ðqÞ. The last two equations with u−1 κα;qν ¼ ðℏ=2M κ ωqν Þ κα;ν define a generalized Fourier transform of the electron-phonon matrix elements between reciprocal space and real space. In Eq. (179) we have N p and N p0 to indicate that the BvK supercells for electronic band structures and phonon dispersions may not coincide. If the quantity gmnκα ðRp ; Rp0 Þ decays rapidly as a function of jRp j and jRp0 j, then only a small number of matrix elements in the Wannier representation will be sufficient to generate gmnν ðk; qÞ anywhere in the Brillouin zone by means of Eq. (178). The dependence of the matrix elements on Rp and Rp0 can be analyzed by considering the following bound: Z jgmnκα ðRp ; Rp0 Þj ≤ drjwm0 ðrÞwn0 ðr − Rp Þj Z drj∂V KS =∂τκα ðr − Rp0 Þj. × FIG. 5. Spatial decay of the electron-phonon matrix elements of sc sc The first term guarantees that the matrix element decays in the variable Rp at least as fast as MLWFs. As a result the worst case scenario corresponds to the choice Rp ¼ 0. In this case, the matrix element jgmnκα ð0; Rp0 Þj decays with the variable Rp0 at the same rate as the screened electric dipole potential generated by the atomic displacement Δτκα . In nonpolar semiconductors and insulators, owing to the analytical properties of the dielectric matrix (Pick, Cohen, and Martin, 1970), this potential decays at least as fast as a quadrupole, that is, jRp0 j−3 . As a result, all matrix elements in reciprocal space are finite for q → 0 (Vogl, 1976) and hence amenable to interpolation. In the case of metals the asymptotic trend of ∂V KS =∂τκα is dictated by Fermi-surface nesting, leading to Friedel oscillations that decay as jRp0 j−4 (Fetter and Walecka, 2003). These oscillations are connected to the Kohn anomalies in the phonon dispersion relations (Kohn, 1959b). In practical calculations, Friedel oscillations are usually not an issue since they are suppressed by the numerical smearing of the FermiDirac occupations, and a Yukawa-type exponential decay is recovered. The case of polar materials is more subtle and is discussed in Sec. VI.A.3. Figure 5 illustrates the spatial decay of jgmnκα ðRp ; Rp0 Þj as a function of Rp and Rp0 for the prototypical case of diamond. The interpolation strategy is entirely analogous to standard techniques for generating phonon dispersion relations using the interatomic force constants (Gonze and Lee, 1997): one first determines matrix elements in the Bloch representation using DFPT on a coarse grid in the Brillouin zone, as in Sec. III.B.3. Then MLWFs are determined using the procedures of Marzari and Vanderbilt (1997) and Souza, Marzari, and Vanderbilt (2001). This yields the rotation matrices Umnk to be used in Eq. (179). The Fourier transform to real space is performed via Eq. (179). At this point, one assumes that Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 diamond in the Wannier representation: (a) max jgmnκα ðRp ; 0Þj vs jRp j, and (b) max jgmnκα ð0; Rp0 Þj vs jRp0 j. The maximum values are taken over all subscript indices, and the data are normalized to the largest value. The insets show the same quantities in logarithmic scale. The calculations were performed using the local density approximation to DFT. From Giustino, Cohen, and Louie, 2007. matrix elements outside of the Wigner-Seitz supercell defined by the coarse Brillouin-zone grid can be neglected and uses Eq. (178) in order to obtain the matrix elements gmnν ðk; qÞ on very fine grids. The last step requires the knowledge of the rotation matrices U mnk also on the fine grids; these matrices are obtained from the Wannier interpolation of the band structures as described by Souza, Marzari, and Vanderbilt (2001). The operation is computationally inexpensive and enables the calculation of millions of electron-phonon matrix elements. The procedure can now be applied routinely (Noffsinger et al., 2010; Poncé et al., 2016). Figure 6 shows the matrix elements obtained using this method as compared to explicit DFPT calculations. Wannier interpolation of electron-phonon matrix elements was successfully employed in a number of applications, ranging from metal and superconductors to semiconductors and nanoscale systems.6 3. Electron-phonon matrix elements in polar materials In the case of polar materials, that is, systems exhibiting nonzero Born effective charges (Pick, Cohen, and Martin, 6 See, for example, Park et al. (2007, 2014), Giustino, Cohen, and Louie (2008), Park, Giustino, McChesney et al. (2008), Noffsinger et al. (2009, 2010, 2012), Calandra, Profeta, and Mauri (2010), Giustino, Louie, and Cohen (2010), Vukmirović, Bruder, and Stojanović (2012), Margine and Giustino (2013, 2014), Bernardi et al. (2014, 2015), Sjakste et al. (2015), and Verdi and Giustino (2015). 015003-34 Feliciano Giustino: Electron-phonon interactions from first … FIG. 6. Comparison between Wannier-interpolated electronphonon matrix elements and explicit DFPT calculations for diamond. The interpolated matrix elements were calculated starting from a coarse 43 Brillouin-zone grid (dotted line, black), a 63 grid (dashed line, blue), and a 83 grid (solid line, red). The dots indicate explicit DFPT calculations. In this example jnki is set to the valence band top at Γ; jmk þ qi spans Λ3 , Δ5 , and Σ2 bands, and the phonon is set to the highest optical branch. From Giustino, Cohen, and Louie, 2007. 1970), the interpolation scheme discussed in Sec. VI.A.2 breaks down. In fact, in these systems the dominant contribution to the potential ∂V KS =∂τκα in Eq. (177) is a dipole, which decays as jRp0 j−2 . As a consequence some of the matrix elements in reciprocal space diverge as jqj−1 for q → 0 and cannot be interpolated straightforwardly from a coarse grid to a fine grid. Physically this singularity corresponds to the “Fröhlich electron-phonon coupling” (Fröhlich, 1954). The adaptation of the Wannier interpolation method to the case of polar materials was recently given by Sjakste et al. (2015) and Verdi and Giustino (2015). In both works the basic idea is to separate the matrix elements into a short-range contribution gSmnν ðk; qÞ, which is amenable to standard Wannier interpolation, and a long-range contribution gLmnν ðk; qÞ, which is singular and is dealt with analytically. The strategy is analogous to that in use for calculating the splitting between longitudinal-optical (LO) and transverseoptical (TO) phonons in polar materials (Gonze and Lee, 1997). The starting point is to define the long-range component of the matrix elements by considering the potential generated by the Born charges of all the atoms, when displaced according to a given vibrational eigenmode. The derivation relies on standard electrostatics and can be found in (Verdi and Giustino, 2015) 1=2 4π e2 X ℏ Ω 4πε0 κ 2N p M κ ωqν X ðq þ GÞ · Zκ · eκν ðqÞ × ðq þ GÞ · ϵ∞ · ðq þ GÞ G≠−q gLmnν ðk; qÞ ¼ i × hψ mkþq jeiðqþGÞ·ðr−τ κ Þ jψ nk isc : ð180Þ In this expression Zκ and ϵ∞ denote the Born effective charge tensors and the electronic permittivity tensor (that is, the permittivity evaluated at clamped nuclei). Equation (180) is the generalization of Fröhlich’s model to the case of anisotropic crystalline lattices and multiple phonon modes (Fröhlich, 1954). The result can be derived alternatively using the analytical Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 FIG. 7. Wannier interpolation of electron-phonon matrix ele- ments for anatase TiO2 . The initial state jnki is set to the bottom of the conduction band at Γ, the final state jmk þ qi spans the bottom of the conduction band along high-symmetry lines, and the phonon is the highest LO mode. The dots correspond to explicit DFPT calculations. The red dashed line is the short-range component of the matrix elements gS . The solid blue curve represents the matrix elements gS þ gL , as obtained from the modified Wannier interpolation of Sec. VI.A.3. The interpolation was performed starting from a coarse 4 × 4 × 4 unshifted grid. From Verdi and Giustino, 2015. properties of the dielectric matrix (Pick, Cohen, and Martin, 1970) as discussed by Vogl (1976). In order to perform Wannier interpolation, one subtracts Eq. (180) from the matrix elements computed on a coarse grid, interpolates the remaining short-range part, and then adds back Eq. (180) on the fine grid. This process requires the interpolation of the bra and ket h isc in the second line of Eq. (180). Verdi and Giustino showed that, for small q þ G, this bra and ket can be interpolated via hψ mkþq jeiðqþGÞ·r jψ nk isc ¼ ½Ukþq U †k mn , where the rotation matrices U mnk are obtained as usual from the procedure of Marzari and Vanderbilt (1997) and Souza, Marzari, and Vanderbilt (2001).7 Figure 7 shows an example of Wannier interpolation for the prototypical polar semiconductor TiO2 : it is seen that the singularity is correctly captured by the modified interpolation method. At the end of this section, we mention that other interpolation schemes are equally possible (Eiguren and Ambrosch-Draxl, 2008b; Prendergast and Louie, 2009; Agapito et al., 2013; Gunst et al., 2016). For example, Eiguren and Ambrosch-Draxl (2008b) proposed to interpolate only the local component of ΔV KS qν , while explicitly calculating the nonlocal part of the perturbation as well as the Kohn-Sham wave functions in the Bloch representation. Furthermore, Eq. (178) remains unchanged if MLWFs are replaced by a basis of localized atomic orbitals, and all concepts discussed in this section remain valid. An 7 Equation (4) of Verdi and Giustino (2015) is missing a factor e ; this factor needs to be retained in order to correctly describe the acoustic modes near q ¼ 0. In practical calculations the G-vector sum in Eq. (180) is restricted to small jq þ Gj via the cutoff 2 function e−ajqþGj . The results are independent of the choice of the cutoff parameter a. −iðqþGÞ·τ κ 015003-35 Feliciano Giustino: Electron-phonon interactions from first … interpolation scheme using local orbitals was recently demonstrated by Gunst et al. (2016). B. Fermi-surface harmonics In the study of metallic systems, one is often interested in describing EPIs only for electronic states in the vicinity of the Fermi surface. In these cases, besides the Wannier interpolation discussed in Secs. VI.A.2–VI.A.3, it is possible to perform efficient calculations using “Fermi-surface harmonics” (FSHs) introduced by Allen (1976) and recently revisited by Eiguren and Gurtubay (2014). The basic idea underlying FSHs is to replace expensive three-dimensional Brillouin-zone integrals by inexpensive one-dimensional integrals in the energy variable. To this aim, Allen (1976) proposed to expand functions of the band index n and wave vector k, say Ank, in products of pairs of functions, one depending on the energy AL ðεÞ and one depending on the wave vector ΦL ðkÞ: Ank ¼ X AL ðεnk ÞΦL ðkÞ: ð181Þ L In this expression, the Fermi-surface harmonics ΦL ðkÞ (to be defined) are constructed so as to obey the following orthogonality condition: N −1 p X δðεnk − εÞΦL ðkÞΦL0 ðkÞ ¼ NðεÞδLL0 ; ð182Þ nk P where NðεÞ ¼ N −1 p nk δðεnk − εÞ is the density of states. Using Eqs. (181) and (182) one finds AL ðεÞ ¼ NðεÞ−1 N −1 p X δðεnk − εÞΦL ðkÞAnk : ð183Þ nk Allen showed that in the FSHs P representation a linear system of the kind RAnk ¼ N −1 p n0 k0 M nk;n0 k0 Bn0 k0 transforms into P 0 0 AL ðεÞ ¼ L0 dε Nðε ÞM LL0 ðε; ε0 ÞBL0 ðε0 Þ. Linear systems of this kind are common in the solution of the Boltzmann transport equation (Sec. X) and the Eliashberg equations for the superconducting gap (Sec. XI.B). If one could perform the expansion using only a few harmonics, then the transformation would be advantageous, since the integrals over the wave vectors would have been absorbed in the expansion coefficients. In the original proposal by Allen, the harmonics ΦL ðkÞ were defined as polynomials in the band velocities; however, the completeness of the basis set was not established. Recently Eiguren and Gurtubay (2014) proposed to construct these functions as eigenstates of a modified Helmholtz equation jvk j∇2k ΦL ðkÞ ¼ ωL ΦL ðkÞ; ð184Þ where vk ¼ ℏ−1 ∇k εnk is the band velocity for states at the Fermi surface, and ωL is the eigenvalue for the harmonic ΦL . The new definition in Eq. (184) maintains the properties of the original FSHs and carries the added advantage that the basis set is complete. In this case the subscript L in ΦL ðkÞ labels the Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 eigenstates of the Helmholtz equation. Eiguren and Gurtubay demonstrated the construction of “Helmholtz FSHs” for prototypical metals such as Cu, Li, and MgB2 . Recent examples of the application of Fermi-surface harmonics to first-principles calculations of EPIs include work on the photoemission kink of YBa2 Cu3 O7 (Heid et al., 2008) and on the Seebeck coefficient of Li (Xu and Verstraete, 2014). VII. NONADIABATIC VIBRATIONAL FREQUENCIES AND LINEWIDTHS As discussed in Secs. V.A.2 and V.A.3, the electron-phonon interaction can lead to a renormalization of the adiabatic vibrational frequencies and to a broadening of the spectral lines. The first ab initio investigations of the effects of the nonadiabatic renormalization of phonon frequencies were reported by Lazzeri and Mauri (2006) and Pisana et al. (2007). In these works they concentrated on the E2g phonon of graphene, which is found at the wave number ω=2πc ¼ 1585 cm−1 at room temperature (c is the speed of light). This phonon corresponds to an in-plane C-C stretching vibration with q ¼ 0 and has been studied extensively via Raman spectroscopy. In the graphene literature this mode is referred to as the “Raman G band.” Figure 8 shows a comparison between calculated and measured E2g phonon frequencies, as a function of doping, from Pisana et al. (2007). The calculations were performed (i) within the adiabatic approximation and (ii) by including the nonadiabatic frequency renormalization using Eq. (145).8 From Fig. 8 we see that the adiabatic theory is unable to reproduce the experimental data. On the contrary, the calculations including nonadiabatic effects nicely follow the measured Raman shift. This is a clear example of the limits of the adiabatic Born-Oppenheimer approximation and a demonstration of the importance of the phonon selfenergy in Eq. (145). The fact that the adiabatic approximation is inadequate for the E2g phonon of doped graphene should have been expected from the discussion in Sec. V.A.3. In fact, graphene is a zerogap semiconductor; therefore electrons residing in the vicinity of the Dirac points can make “virtual” transitions with jqj ¼ 0 and energies comparable to that of the E2g mode. As a result, the condition underlying the adiabatic approximation jεmkþq − εnk j ≫ ℏωqν does not hold in this case. The importance of nonadiabatic effects was also confirmed in the case of metallic single-walled carbon nanotubes (Caudal et al., 2007; Piscanec et al., 2007). In these works, they studied the phonon dispersion relations in the vicinity of jqj ¼ 0 and found that the difference between adiabatic and nonadiabatic dispersions is concentrated around the zone center. This finding is consistent with earlier models of nonadiabatic effects. In fact, Maksimov and Shulga (1996) showed that, for metals with linear electron bands crossing the 8 In the works reviewed in this section they used Eq. (145) with the bare matrix elements gbmnν ðk; qÞ replaced by the screened matrix elements gmnν ðk; qÞ. All calculations were performed within DFT, using either the LDA or gradient-corrected DFT functionals. 015003-36 Feliciano Giustino: Electron-phonon interactions from first … Comparison between measured (ωexp ) and calculated (ωth ) vibrational frequencies of the E2g mode of graphite intercalation compounds. Open symbols are adiabatic DFPT calculations, and filled symbols are calculations including the nonadiabatic corrections. The line corresponds to ωth ¼ ωexp . From Saitta et al., 2008. FIG. 9. FIG. 8. Frequency of the Raman G band of graphene vs carrier concentration. The black filled disks are from Raman measurements of gated graphene on a silicon substrate at 295 K. The thick horizontal dashed line (red) shows the variation of the E2g mode frequency with doping, within the adiabatic approximation. The solid blue line shows the variation of the frequency calculated by including nonadiabatic frequency renormalization. From Pisana et al., 2007. Fermi level, ΠNA is significant only for wave vectors jqj ∼ ω=vF , where ω is the phonon energy and vF is the Fermi velocity. This result can be derived from Eq. (145). In the previous examples, the nonadiabatic renormalization of the vibrational frequencies is measurable but very small, typically of the order of 1% of the corresponding adiabatic frequencies. Saitta et al. (2008) considered the question as to whether one could find materials exhibiting large nonadiabatic renormalizations and considered several graphite intercalation compounds, namely, LiC6 , LiC12 , KC8 , KC24 , RbC8 , CaC6 , SrC6 , and BaC6 , as well as other metallic systems such as MgB2 , Mg, and Ti. In order to calculate the nonadiabatic renormalization at a reduced computational cost, the real part of the phonon self-energy was approximated as follows: 2 ℏReΠNA q¼0;νν ≃ N F hjgnnν ðk; q ¼ 0Þj iBZ , where h iBZ stands for the average taken over the wave vectors k in the Brillouin zone, and N F is the density of states at the Fermi level. This expression can be derived from Eq. (145) by replacing the bare matrix elements by their screened counterparts, and by neglecting the “interband” contributions m ≠ n in the sum. Figure 9 shows a comparison between vibrational frequencies from experiment and those calculated with or without including the nonadiabatic self-energy. It is clear that the nonadiabatic frequencies are in much better agreement with experiment than the corresponding adiabatic calculations. Furthermore, in these compounds the renormalization can reach values as large as ∼300 cm−1 . In contrast to this, the renormalization in Mg and Ti was found to be of only a few wave numbers in cm−1 . Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 The case of MgB2 proved more puzzling: here the calculated nonadiabatic frequency is 761 cm−1 , while experiments reported 600 cm−1 . In order to explain this discrepancy, Saitta et al. reasoned that a more accurate calculation would require taking into account the relaxation time of the electrons, as pointed out by Maksimov and Shulga (1996). This would act so as to partly wash out nonadiabatic effects. In the fieldtheoretic language of Sec. V, this observation corresponds to stating that when one approximates the dressed electron propagator G in Fig. 2(c) using the noninteracting KohnSham Green’s function, one should include at the very least the effects of finite electron lifetimes (due to electron-electron, electron-impurity, and electron-phonon scattering), for example, via the imaginary part of Eq. (157). The calculations discussed so far in this section addressed the nonadiabatic renormalization of zone-center phonons. The generalization to calculations of complete phonon dispersions was made by Calandra, Profeta, and Mauri (2010). In their work, Calandra et al. employed Wannier interpolation (see Sec. VI) in order to calculate the nonadiabatic phonon selfenergy of Eq. (145) throughout the Brillouin zone. Figure 10 shows a comparison between the standard DFPT phonon dispersion relations of CaC6 and the dispersions obtained after incorporating the nonadiabatic self-energy. It is seen that also in this case nonadiabatic effects are most pronounced at small q and can be as large as 7% of the adiabatic frequency. In their work Calandra et al. approximated the bare matrix element gbmnν ðk; qÞ appearing in Eq. (145) by the screened matrix element gmnν ðk; qÞ. This replacement was justified by reasoning that the error is of second order in the induced electron density, hence it should be negligible. The broadening of vibrational spectra arising from the electron-phonon interaction is almost invariably calculated from first principles using Eq. (146). Since the integration of the Dirac delta is computationally costly, it is common to rewrite that equation by neglecting the phonon energy in the delta function and by taking the low-temperature limit, as proposed by Allen (1972b): 015003-37 Feliciano Giustino: Electron-phonon interactions from first … FIG. 10. Phonon dispersion relations of CaC6 calculated using Wannier interpolation. The dashed lines (black) and the solid lines (red) represent the standard adiabatic calculation and the nonadiabatic phonon dispersions, respectively. From Calandra, Profeta, and Mauri, 2010. X Z dk γ qν ≃2 jg ðk; qÞj2 δðεnk − εF Þδðεmkþq − εF Þ; πωqν ΩBZ mnν mn ð185Þ where εF is the Fermi energy. Oddly enough, this is a sort of adiabatic approximation to the nonadiabatic theory. The main advantage is that Eq. (185) is positive definite, hence easier to converge numerically as compared to the complete expression in Eq. (146). The disadvantages are that the temperature dependence is lost, and that one cannot resolve fine features on the scale of a phonon energy. There exists a vast literature on first-principles calculations of phonon linewidths using Eq. (185), mostly in connection with electron-phonon superconductors.9 Equation (185) is now implemented in several large software projects (Giannozzi et al., 2009; Gonze et al., 2009), and it is used routinely. Phonon linewidths range from very small values such as ∼1 meV in Nb (Bauer et al., 1998) to large values such as ∼30 meV in MgB2 (Shukla et al., 2003). The agreement between calculations and neutron scattering or Raman measurements is usually reasonable. Calculations of phonon linewidths using the more accurate expression in Eq. (146) are computationally more demanding and have been reported less extensively in the literature.10 9 See, for example, early frozen-phonon calculations (Dacorogna, Cohen, and Lam, 1985; Chang and Cohen, 1986; Lam, Dacorogna, and Cohen, 1986) and more recent DFPT calculations (Savrasov, Savrasov, and Andersen, 1994; Bauer et al., 1998; Shukla et al., 2003; Heid et al., 2010). Earlier calculations not based on DFT were reviewed by Grimvall (1981). 10 See, for example, Lazzeri et al. (2006), Bonini et al. (2007), Giustino, Cohen, and Louie (2007), and Park, Giustino, Cohen, and Louie (2008). Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 So far we considered the effect of EPIs on the frequencies and lifetimes of vibrational excitations in solids. Another important phenomenon which modifies frequencies and lifetimes is anharmonicity. Anharmonic effects result from third- and higher-order terms in the Taylor expansion of the total potential energy U in the atomic displacements (Sec. III.A). These effects can be interpreted as additional interactions that couple the oscillators of the harmonic lattice; for example, thirdorder anharmonic effects reduce phonon lifetimes via energy upconversion or downconversion processes involving three phonons. Anharmonic effects can be described using a manybody field-theoretic formalism (Cowley, 1963), in complete analogy with the theory of EPIs discussed in Sec. IV. Calculation of anharmonic effects from first principles goes through the evaluation of third- and fourth-order derivatives of the total potential energy U in the adiabatic approximation. Third-order coefficients are routinely computed using DFPT (Debernardi, Baroni, and Molinari, 1995; Deinzer, Birner, and Strauch, 2003; Lazzeri, Calandra, and Mauri, 2003; Bonini et al., 2007; Broido et al., 2007). In those cases where the harmonic approximation fails completely, “self-consistent phonon” techniques can be employed (Hooton, 1955; Koehler, 1966). Recent implementations and calculations can be found in Errea, Rousseau, and Bergara (2011), Hellman, Abrikosov, and Simak (2011), Hellman et al. (2013), Monserrat, Drummond, and Needs (2013), and Errea, Calandra, and Mauri (2014). VIII. ELECTRON-PHONON INTERACTIONS IN PHOTOELECTRON SPECTROSCOPY In Sec. V.B.5 we have seen how the electron-phonon interaction in metals can lead to band structure “kinks” near the Fermi energy. This is illustrated by the model calculation in Fig. 4(a). The experimental investigation of these features started in the late 1990s, following the development of high-resolution ARPES. Since in ARPES only the component of the photoelectron momentum parallel to the sample surface is conserved (Damascelli, Hussain, and Shen, 2003), complete energy versus wave vector dispersion relations can be measured directly only for 2D or quasi-2D materials. Accordingly, the first observations of kinks were reported for the surface states of elemental metals11 and for the CuO2 planes of copper oxide superconductors.12 Ab initio calculations of ARPES kinks can be performed by using the diagonal part of the Fan-Migdal self-energy (the Debye-Waller self-energy will be discussed at the end of this section). To this aim, it is common to rewrite Eqs. (157) and (158) at finite temperature using a spectral representation: 11 See, for example, Hengsberger et al. (1999) and Valla, Fedorov, Johnson, and Hulbert (1999). 12 See, for example, Valla et al. (1999), Johnson et al. (2001), and Lanzara et al. (2001). 015003-38 Feliciano Giustino: Electron-phonon interactions from first … Z ΣFM nnk ðω; TÞ ¼ Z þ∞ dε −∞ 0 ∞ dε0 α2 Fnk ðε; ε0 Þ 1 − fðε=kB TÞ þ nðε0 =kB TÞ ℏω − ε − ε0 þ iℏη fðε=kB TÞ þ nðε0 =kB TÞ : þ ℏω − ε þ ε0 þ iℏη × ð186Þ Here the function α2 F is the so-called “Eliashberg function” and is defined as α2 Fnk ðε; ε0 Þ ¼ X Z dq jgnmν ðk; qÞj2 Ω BZ mν × δðε − εmkþq Þδðε0 − ℏωqν Þ: ð187Þ This quantity is positive, temperature independent, and contains all the materials-specific parameters. Physically it is proportional to the scattering rate of an electron in the state jnki into any electronic state at the energy ε, by emitting or absorbing any one phonon of energy ε0. One complication related to the Eliashberg function is that in the literature many variants of Eq. (187) can be found, each stemming from specific approximations; some of these expressions are summarized by Grimvall (1981). The first ab initio calculations of the phonon-induced electron self-energies and photoemission kinks were reported by Eiguren, de Gironcoli et al. (2003) for the surface state of the Be(0001) surface. Since the evaluation of Eqs. (186) and (187) is computationally demanding, Eiguren et al. employed simplified expressions which involve the following three approximations: (i) the Eliashberg function is average α2 Fn ðε; ε0 Þ ¼ R R replaced by 2 its isotropic 0 dkδðεnk − εÞ × α Fnk ðε; ε Þ= dkδðεnk − εÞ; (ii) phonon energies are neglected next to electron energies (as in the adiabatic approximation), and (iii) particle-hole symmetry is assumed. Using these approximations the imaginary part of the Fan-Migdal self-energy becomes Z jImΣFM n ðω; TÞj ¼ π ∞ 0 dε0 α2 Fn ðℏω; ε0 Þf1 þ 2nðε0 =kB TÞ þ f½ðℏω þ ε0 Þ=kB T − f½ðℏω − ε0 Þ=kB Tg; ð188Þ where the average of the self-energy is defined as for the Eliashberg function. The real part of the self-energy can be found starting from the same approximations and is given by Grimvall (1981). Figure 11 shows the self-energy of the surface state at the Be(0001) surface calculated by Eiguren, de Gironcoli et al. (2003) using Eq. (188). The imaginary part resembles a step function, with an onset around the energy threshold for phonon emission by a hole (40–80 meV in this case). At a qualitative level, this trend can be rationalized by replacing the Eliashberg function in Eq. (188) by a Dirac delta at a characteristic phonon energy ℏωph. In this case, the hole selfenergy becomes proportional to f½ðℏω þ ℏωph Þ=kB T. At T ¼ 0 this is precisely a step function with onset at −ℏωph . The real part of the self-energy vanishes for jωj ≫ ωmax, with Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 FIG. 11. Calculated Fan-Migdal self-energy of the surface state at the Be(0001) surface. (a) Imaginary part of the self-energy, obtained from Eq. (188). The dashed (black) line is the selfenergy evaluated using the DFT-LDA bands; the solid lines (color, gray scale) correspond to the self-energy calculated by taking into account the renormalization of the DFT band structure by the electron-phonon interaction. (b) Real part of the selfenergy, using the same color, gray scale code as in (a). The inset in (a) compares the renormalized band structure (color) with the “bare” DFT band (black dashed line). The inset of (b) shows the renormalization of the band velocity induced by the electronphonon interaction. From Eiguren, de Gironcoli et al., 2003. ωmax the largest phonon frequency. This can be seen in Fig. 11(b) and is a consequence of the approximation of particle-hole symmetry. Eiguren et al. also determined the renormalization of the surface state band structure arising from electron-phonon interactions, using Eq. (164); this is shown in the inset of Fig. 11(a). Overall the calculations of Eiguren, de Gironcoli et al. (2003) showed good agreement with photoelectron spectroscopy experiments, in both the shape and magnitude of the self-energy (LaShell, Jensen, and Balasubramanian, 2000). In addition to these calculations, several studies of the electron-phonon self-energy at metal surfaces were reported, namely, for the Cu(111) and Ag(111) surfaces (Eiguren et al., 2002), the Al(100), Ag(111), Cu(111), and Au(111) surfaces (Eiguren, Hellsing et al., 2003), and the W(110) surface (Eiguren and Ambrosch-Draxl, 2008a). Building on these studies, Eiguren, Ambrosch-Draxl, and Echenique (2009) performed a detailed analysis of the self-consistent solutions of the complex Dyson equation for the quasiparticle energies, Eqs. (164) and (165), and illustrated the key concepts in the cases of the W(110) surface and for the phonon-mediated superconductor MgB2. Equation (188) or closely related approximations were also employed in the study of electron and hole lifetimes in bulk Be (Sklyadneva et al., 2005), Pb (Sklyadneva et al., 2006), 015003-39 Feliciano Giustino: Electron-phonon interactions from first … and Mg (Leonardo et al., 2007); the photoemission kink in YBa2 Cu3 O7 (Heid et al., 2008); and the spectral function of Ca-intercalated graphite (Sanna et al., 2012). In the case of complex systems the validity of the approximations (i)–(iii) leading to Eq. (188) is not warranted, and a direct calculation of the Fan-Migdal self-energy using Eqs. (186) and (187) is necessary. Calculations of the complete self-energy were reported by Park et al. (2007) for graphene, by Giustino, Cohen, and Louie (2008) for the high-temperature superconductor La1−x Srx Cu2 O4, and by Margine, Lambert, and Giustino (2016) for Ca-intercalated bilayer graphene. Figure 12 shows the calculated self-energy and spectral function of graphene calculated by Park et al. (2007, 2009). The structure of the self-energy is similar to that shown in Fig. 11, with one important exception: ΣFM nnk ðωÞ does not vanish a few phonon energies away from the Fermi level, but tends instead toward a linear asymptote. Calandra and Mauri (2007) performed a combined ab initio and analytical study of the effects of the electron-phonon interaction on the electron bands of graphene and obtained very similar results. A linear asymptote in the real part of the self-energy is a general feature of systems which do not exhibit particle-hole symmetry. For another example see the work on copper oxides by Giustino, Cohen, and Louie (2008). Using the Fan-Migdal self-energy, it is possible to calculate the renormalization of the band velocity induced by the electron-phonon interaction. Let us denote by vnk ¼ ℏ−1 ∇k εnk the DFT band velocity and V nk ¼ ℏ−1 ∇k Enk the band velocity after including electron-phonon interactions. Using Eq. (164) with Γnk ¼ 0 we find that these two quantities are simply related by V nk ¼ Znk vnk ¼ vnk = ð1 þ λnk Þ, where Znk is the quasiparticle strength of Eq. (174), and λnk is the “mass enhancement parameter” or “electron-phonon coupling strength” (Grimvall, 1981): −1 λnk ¼ Z−1 nk − 1 ¼ −ℏ ∂ReΣnnk ðωÞ=∂ωjω¼Enk =ℏ : ð189Þ In the study of EPIs in metals, the coupling strength λnk is of significant interest since it is related to the superconducting transition temperature of phonon-mediated superconductors (see Secs. VIII.A and XI). The velocity renormalization in graphene calculated using Eq. (189) is shown in Figs. 12(c) and 12(d), while a calculation of the complete spectral function Aðk; ωÞ is shown in Fig. 12(e). Here the characteristic photoemission kink is visible between 150 and 200 meV but it is not very pronounced, since in this case λnk ∼ 0.1 (Park et al., 2009). These results are in good agreement with measured photoelectron spectra (Bostwick et al., 2007; Zhou et al., 2007). Incidentally, we remark that in the analysis of ARPES data it is common to extract the coupling strength λnk directly from the ratio of the band velocities above and below the electronphonon kink. However, this procedure is subject to a significant uncertainty, since the bare velocity is not known and must be approximated by fitting the fully interacting dispersions using ad hoc models. For example, in the vicinity of van Hove singularities this procedure leads to a significant overestimation of the electron-phonon coupling strength λnk (Park, Giustino, McChesney et al., 2008; Bianchi et al., 2010). Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 FIG. 12. (a), (b) Calculated real part of the Fan-Migdal self- energy in pristine and n-doped graphene, respectively (solid black lines). The doping level is 4 × 1013 cm−2 . The dashed lines correspond to a simplified analytical model where particle-hole symmetry is assumed. (c), (d) Electron band velocity renormalization resulting from the self-energies in (a) and (b). All calculations in (a)–(d) were performed using DFT-LDA. From Park et al., 2007. (e) Calculated spectral function of n-doped graphene for one of the branches of the Dirac cone. ωph indicates the characteristic phonon energy leading to the photoemission kink, and ED denotes the energy of the Dirac point. The calculations include GW quasiparticle corrections. From Park et al., 2009. In addition to photoemission kinks, recent ARPES measurements revealed the existence of polaron satellites in doped oxides, namely, TiO2 (Moser et al., 2013) and SrTiO3 (Chen et al., 2015; Cancellieri et al., 2016; Wang et al., 2016). The phenomenology is similar to what was discussed in relation to Fig. 4(b). The first theoretical studies along this direction were reported by Story et al. (2014), who applied the cumulant expansion approach to the case of the electron-phonon selfenergy; by Antonius et al. (2015), who identified satellites in the spectral functions of LiF and MgO; and by Verdi, Caruso, and Giustino (2017), who calculated the ARPES spectra of n-doped TiO2 . 015003-40 Feliciano Giustino: Electron-phonon interactions from first … At the end of this section, it is worth returning to the subject of the Debye-Waller self-energy. So far we only discussed the Fan-Migdal self-energy, starting from Eq. (186), and we ignored the Debye-Waller self-energy appearing in Eq. (152). This omission reflects the fact that, in the literature on electron-phonon interactions in metals, the DW term has always been disregarded. In order to rationalize this approximation, we rewrite the DW self-energy as follows, by combining Eqs. (160) and (40): ΣDW nnk ¼ hunk jV DW junk iuc ; ð190Þ P R KS with V DW ðrÞ ¼ Ω−1 ν dqðnqν þ 1=2ÞΔqν Δ−qν v ðrÞ. BZ The subscript “uc” indicates that the integral is over one unit cell. From Eq. (190) we see that V DW acts like a static local potential; indeed the first calculations including DW effects were performed by directly modifying the ionic pseudopotentials (Antončík, 1955; Walter et al., 1970). From Eq. (190) we also see that the only variation in the DW self-energy comes from the Bloch amplitudes unk . Let us consider the limiting situation of the homogeneous electron gas. In this case junk ðrÞj2 ¼ 1=Ω (Sec. III.B.5); therefore ΣDW nnk is a constant, independent of k. This behavior should be contrasted with the Fan-Migdal self-energy, which exhibits significant structure near the Fermi energy as can be seen in Fig. 4. In more realistic situations, such as doped semiconductors, k · p perturbation theory (Kittel, 1963) can be used to show that ΣDW nnk varies smoothly as a function of k within the same band. In contrast to this scenario, ΣDW nnk exhibits large variations across different bands. This carries important consequences for the calculation of temperature-dependent band gaps (Sec. IX.A.1). proportional to the band velocity, it follows that the heat capacity is directly proportional to the electron mass. This property can be used as a means to determine the strength of the electron-phonon coupling in simple metals from specific heat measurements (Grimvall, 1975). The general theory of the effects of electron-phonon interactions on the heat capacity and other thermodynamic functions was developed by Eliashberg (1963), Prange and Kadanoff (1964), and Grimvall (1969). A field-theoretic analysis of the effect of EPIs on thermodynamic functions was developed by Eliashberg (1963) starting from the identities of Luttinger and Ward (1960) in the zero-temperature limit. Eliashberg’s analysis was subsequently extended to all temperatures by Grimvall (1969). Here we quote only Grimvall’s result relating the electronic entropy to the FanMigdal self-energy of Sec. V.B.1: Se ¼ Z ∞ 0 Ce ¼ T We now come back to the mass enhancement parameter λnk introduced in Eq. (189), since this quantity played a central role in the development of the theory of EPIs in metals. The notion of mass enhancement becomes clear when we consider a parabolic band as in the model calculations of Fig. 4. Near the Fermi surface the noninteracting dispersions are given by εnk ¼ ℏkF · ℏðk − kF Þ=m, where kF is a wave vector on the Fermi surface, and the electron velocity is vnk ¼ ℏkF =m . After taking into account the EPI, the electron velocity is renormalized to V nk ¼ vnk =ð1 þ λnk Þ. Since the magnitude of the Fermi momentum is unchanged (see the caption of Fig. 4), this renormalization can be interpreted as an effective increase of the band mass from m to mep ¼ m ð1 þ λnk Þ. This reasoning holds for metals with parabolic bands and for doped semiconductors near band extrema and does not take into account the Debye-Waller selfenergy. The electron mass enhancement is reflected in the increase of the heat capacity of metals at low temperature. In fact, below the Debye temperature the electronic contribution to the heat capacity dominates over the lattice contribution (Kittel, 1976). Since the heat capacity is proportional to the density of states at the Fermi level, and the density of states is inversely ω½ω − ℏ−1 ReΣFM nnk ðω; TÞ dω: 2 cosh ðℏω=2kB TÞ ð191Þ In order to derive this relation, Grimvall started by expressing the thermodynamic potential of the coupled electron-phonon system in terms of the electron and phonon propagators and self-energies and identified the electronic contribution by neglecting terms of the order of ðme =M 0 Þ1=2 as well as electron-electron interactions (Grimvall, 1969, Appendix). Below the Debye temperature, an explicit expression for the entropy in Eq. (191) can be obtained by noting that the function cosh−2 ðℏω=2kB TÞ is nonvanishing only for ℏω ≲ 2kB T. In this range Eq. (189) yields ΣFM nnk ðω; TÞ ≃ −λnk ℏω, and therefore the integration in Eq. (191) can be carried out explicitly. As a result, the low-temperature heat capacity can be written as A. Electron mass enhancement in metals Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 N F k B ℏ3 ðkB TÞ2 ∂Se 2 2 2 ¼ π kB N F ð1 þ λnk ÞT: ∂T 3 ð192Þ If we ignore the EPI by setting λnk ¼ 0, this expression reduces to the standard textbook result for the free electron gas (Kittel, 1976). At high temperature Eq. (192) is no longer valid, and one has to evaluate the integral in Eq. (191) using the complete frequency-dependent FM self-energy. The main result of this procedure is that at high temperature the electronic heat capacity is no longer renormalized by EPIs. A detailed discussion of this aspect is provided by Grimvall (1969, 1981). Early examples of DFT calculations of mass enhancement parameters and comparisons with specific heat measurements in simple metals can be found in Dacorogna, Cohen, and Lam (1985), Savrasov, Savrasov, and Andersen (1994), and Liu and Quong (1996). IX. ELECTRON-PHONON EFFECTS IN THE OPTICAL PROPERTIES OF SEMICONDUCTORS A. Temperature dependence of band gaps and band structures 1. Perturbative calculations based on the Allen-Heine theory In Sec. V.B.3 we discussed how the electron-phonon interaction induces a “renormalization” of the electronic 015003-41 Feliciano Giustino: Electron-phonon interactions from first … energy levels and thereby gives rise to “temperaturedependent band structures.” These effects have been studied in detail using the Fan-Midgal and the Debye-Waller selfenergies, either via the Raleigh-Schrödinger approximation to Eq. (166) or via its adiabatic counterpart given by Eq. (167). Equation (167) was first employed in a number of calculations based on empirical pseudopotentials (see footnote 4), following the seminal work of Allen and Heine (1976). Allen and Cardona (1981) offered a clear introduction to the basic theory, a discussion of the computational methodology, as well as an historical perspective on earlier calculations. The evaluation of the Debye-Waller contribution to the selfenergy requires the calculation of the second-order variations of the Kohn-Sham potential with respect to the ionic displacements, Eq. (40). From a computational standpoint, this is challenging because one would have to use second-order DFPT, as discussed at the end of Sec. III.B.3. In order to avoid this complication, it is common practice to recast all secondorder derivatives as products of first-order derivatives. This strategy was introduced by Allen and Heine in the case of monatomic crystals and extended to polyatomic unit cells by Allen and Cardona. The key observation behind this approach is that one can impose translational invariance of the theory to second order in the nuclear displacements. Specifically, the variation of the Kohn-Sham eigenvalues ensuing an arbitrary displacement of the nuclei should not change if all nuclei are further displaced by the same amount. Using timeindependent perturbation theory, this condition yields the following two sum rules: X hψ nk j∂ καp V KS jψ nk isc ¼ 0; ð193Þ κp 0 XX X hψ nk j∂ 2καp;κ0 α0 p0 V KS jψ nk isc ¼ −2Re κ0 p0 × κ 0 p0 mq hψ nk j∂ καp V KS jψ mkþq isc hψ mkþq j∂ κ0 α0 p0 V KS jψ nk isc : εnk − εmkþq ð194Þ Here ∂ καp V KS is a short-hand notation for ∂V KS =∂τκαp and similarly for the second derivative; the primed summation indicates that eigenstates ψ mkþq such that εnk ¼ εmkþq are skipped. The first sum rule is equivalent to stating that the electron-phonon matrix elements gmnν ðk; qÞ associated with the three translational modes at jqj ¼ 0 must vanish; this is an alternative formulation of the “acoustic sum rule.” The second sum rule, Eq. (194), suggests to express the matrix elements of the second derivatives of the potential in terms of first-order derivatives. However, Eq. (194) cannot be used as it stands, since it involves a sum of matrix elements on the left-hand side. In order to proceed, Allen and Heine employed the rigid-ion approximation, whereby V KS is written as a sum of atom-centered contributions (see Sec. II.A.1). Under this approximation all the terms κp ≠ κ 0 p0 on the left-hand side of Eq. (194) are neglected, and an explicit expression for hψ nk j∂ 2καp;καp V KS jψ nk isc is obtained. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 In view of practical DFT implementations, Giustino, Louie, and Cohen (2010) used the sum rule in Eq. (194) in order to rewrite the Debye-Waller self-energy as follows: ΣDW nnk ¼ − 0 Z X dq g2;DW mnν ðk; qÞ ð2nqν þ 1Þ: ΩBZ εnk − εmk νm ð195Þ Here gDW mnν ðk; qÞ is an effective matrix element, and it is obtained from the standard DFPT matrix elements by means of inexpensive matrix multiplications: g2;DW mnν ðk; qÞ ¼ X tνκα;κ0 α0 ðqÞ κα κ 0 α0 tνκα;κ0 α0 ðqÞ ¼ 2ωqν hmn;κα ðkÞhmn;κ0 α0 ðkÞ; ð196Þ eκαν ðqÞeκα0 ν ðqÞ eκ0 αν ðqÞeκ0 α0 ν ðqÞ þ ; Mκ M κ0 ð197Þ X ðM κ ω0ν Þ1=2 eκαν ð0Þgmnν ðk; 0Þ: ð198Þ hmn;κα ðkÞ ¼ ν In the case of the three translational modes at jqj ¼ 0, these definitions are replaced by gDW mnν ðk; qÞ ¼ 0; see the discussion in Sec. XIII. The derivation of Eqs. (195)–(198) requires using Eqs. (20), (33)–(35), and (38), as well as taking the canonical average over the adiabatic nuclear quantum states. Equation (195) involves a summation over unoccupied Kohn-Sham states and so does the Fan-Migdal self-energy in Eq. (167). The numerical convergence of these sums is challenging, since one needs to evaluate a very large number of unoccupied electronic states. To address this issue, Gonze, Boulanger, and Côté (2011) developed a procedure whereby only a subset of unoccupied states is required, along the lines of the DFPT equations of Sec. III.B.3. The first ab initio calculations using the formalism of Allen and Heine were reported by Marini (2008), who investigated the temperature dependence of the optical absorption spectrum of silicon and boron nitride. In this work Marini included excitonic effects by combining the Bethe-Salpeter formalism (Onida, Reining, and Rubio, 2002) with the Allen-Heine theory and obtained good agreement with experiments by calculating the direct absorption peaks using DFT-LDA phonons and matrix elements (indirect optical absorption is discussed in Sec. IX.B). The second application of the Allen-Heine theory using DFT and LDA was reported by Giustino, Louie, and Cohen (2010) for the case of diamond. They investigated the temperature dependence of the direct band gap of diamond and found that the Fan-Migdal and the Debye-Waller self-energies are of comparable magnitude. The calculations captured the characteristic Varshni effect (Fig. 3) and were able to reproduce the measured redshift of the band gap in the temperature range 80–800 K. These calculations were based on the adiabatic version of the Allen-Heine theory and employed Eqs. (196)–(198) for the Debye-Waller self-energy. The calculations by Giustino et al. confirmed the large (> 0.5 eV) zero-point renormalization of the direct gap of diamond predicted by Zollner, Cardona, and Gopalan (1992) using the empirical pseudopotential method. 015003-42 Feliciano Giustino: Electron-phonon interactions from first … The unusually large zero-point correction to the electronic structure of diamond stimulated further work on this system: Cannuccia and Marini (2011, 2012) calculated the gap renormalization in diamond by employing both the adiabatic version of the Allen-Heine theory and the nonadiabatic Green’s function approach, as described in Sec. V.B.5. Their calculations confirmed the large zero-point renormalization and showed that the adiabatic theory underestimates the effect to some extent. Cannuccia and Marini (2012, 2013) also analyzed the quasiparticle renormalization and the spectral function. Antonius et al. (2014) revisited the electron-phonon interaction in diamond by assessing the reliability of the rigid-ion approximation and the importance of many-body GW quasiparticle corrections to the DFT-LDA band structure. The main findings were that the rigid-ion approximation introduces a very small error in diamond, of the order of ∼10 meV, while GW quasiparticle corrections can increase the electronphonon renormalization of the band gap by as much as ∼200 meV. The temperature dependence of the band gap of diamond calculated by Antonius et al. is shown in Fig. 13. Further work on diamond was reported by Poncé, Antonius, Gillet et al. (2014), who compared ab initio calculations based on the Allen-Heine theory with explicit frozen-phonon calculations (Sec. IX.A.2). The corrections to the rigid-ion approximation were found to be smaller than 4 meV in all cases considered. Poncé, Antonius, Boulanger et al. (2014) and Poncé, Antonius, Gillet et al. (2014) also reported a detailed assessment of the accuracy of the various levels of approximation in the calculation of the zero-point renormalization of energy levels, as well as a thorough comparison between the results of different first-principles implementations. The electron-phonon renormalization of band structures was also investigated in a number of other systems. For example, Kawai et al. (2014) studied zinc-blende GaN by combining the Allen-Heine theory with the Bethe-Salpeter approach. Poncé et al. (2015) investigated silicon, diamond, BN, α-AlN, and β-AlN using both the adiabatic version of the FIG. 13. Temperature dependence of the direct band gap of diamond calculated using the Allen-Heine theory. The upper curve shows the results obtained within DFPT at the LDA level. The lower curve was obtained via GW calculations in the frozenphonon approach. Triangles are experimental data. The zeropoint renormalization calculated by including GW quasiparticle corrections is 628 meV. From Antonius et al., 2014. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Allen-Heine theory and the nonadiabatic Green’s function method of Eqs. (157) and (158). Friedrich et al. (2015) investigated the zero-point renormalization in LiNbO3 using the adiabatic Allen-Heine theory. Villegas, Rocha, and Marini (2016) studied the anomalous temperature dependence of the band gap of black phosphorous. Antonius et al. (2015) investigated diamond, BN, LiF, and MgO, focusing on the dynamical aspects and the spectral function (see Sec. VIII). Antonius et al. (2015) and Poncé et al. (2015) were the first to report complete band structures at finite temperature. Poncé et al. (2015) paid special attention to the numerical convergence of the self-energy integrals with respect to the limit η → 0 of the broadening parameter. They noted that in the case of polar crystals the adiabatic correction to the electron energies of band extrema, as given by Eq. (167), diverges in the limit of dense Brillouin-zone sampling. This behavior stems from the polar singularity in the electronphonon matrix elements, Eq. (180). In fact, near band extrema the bands are approximately parabolic, and the integrand in the adiabatic Fan-Migdal self-energy goes as q−4 for q → 0, while the volume element goes only as dq ¼ 4πq2 dq. This problem can be avoided by first performing the integration over q in principal value, without neglecting phonon frequencies, and then taking the limit ωqν → 0 so as to recover the adiabatic approximation (Fan, 1951, Sec. IV). In this way the adiabatic approximation can still be employed without incurring into a singularity in the calculations. A practical strategy to correctly perform the principal value integration in firstprinciples calculations was recently proposed by Nery and Allen (2016); they treated the singularity via an explicitly analytic integration near q ¼ 0. The complications arising in polar materials can also be avoided at once by directly using the more accurate expression in Eq. (166) based on BrillouinWigner perturbation theory, or even better by calculating the spectral functions as in Kawai et al. (2014) and Antonius et al. (2015). In particular, Eq. (166) clearly shows that in more accurate approaches the infinitesimal η should be replaced by the finite physical linewidth Γnk . Although temperature-dependent band structures of polar materials were recently reported (Kawai et al., 2014; Antonius et al., 2015; Poncé et al., 2015), the specific role of the Fröhlich coupling discussed in Sec. VI.A.3 has received little attention so far. The only ab initio investigations which specifically addressed the role of polar couplings in this context are from Botti and Marques (2013) and Nery and Allen (2016). In order to understand the strategy of Botti and Marques, we consider the Hedin-Baym equations in Sec. IV.B.1. Botti and Marques proposed that, instead of splitting the screened Coulomb interaction W into electronic and nuclear contributions as in Eq. (104), one could try to directly calculate the screened Coulomb interaction W including the lattice screening, as in Eqs. (85) and (86). In order to make the calculations tractable, Botti and Marques evaluated the total dielectric matrices using a simplified model based on the Lyddane-Sachs-Teller relations. The resulting formalism combines GW calculations and experimentally measured LO-TO splittings. The zero-point renormalization of the band gaps calculated by Botti and Marques for LiF, LiCl, NaCl, and MgO were all > 1 eV. This is an interesting result and 015003-43 Feliciano Giustino: Electron-phonon interactions from first … deserves further investigation. We note incidentally that the Allen-Heine theory and that of Botti and Marques can both be derived from the Hedin-Baym equations. Therefore the approach of Botti and Marques should effectively correspond to calculating the Fan-Migdal self-energy by retaining only the long-range part of the polar electron-phonon matrix elements, i.e., Eq. (180). In the case of the work by Nery and Allen (2016), they reported a Fröhlich contribution to the zero-point renormalization of the band gap of GaN of 45 meV to be compared with the total renormalization arising from all modes of 150 meV. 2. Nonperturbative adiabatic calculations An alternative approach to the calculation of temperaturedependent band structures consists of avoiding perturbation theory and electron-phonon matrix elements altogether and replacing the entire methodology discussed in Sec. IX.A.1 by straightforward finite-difference calculations. To see how this alternative strategy works we perform a Taylor expansion of the Kohn-Sham eigenvalues εnk to second order in the atomic displacements Δτκαp and then average the result on a nuclear wave function identified by the quantum numbers fnqν g. After using Eq. (20) one obtains hεnk ifnqν g ¼ εnk þ X Z dq ∂ε ðnqν þ 1=2Þ nk ; ∂nqν ΩBZ ν ð199Þ where we used the formal definition ∂=∂nqν ¼ Δqν Δ−qν , and the variations Δqν are the same as in Eqs. (33)–(35). The nuclear wave functions are obtained from the ground state in Eq. (B10) by applying the ladder operators, as discussed in Appendix B. Equation (199) can be generalized to finite temperature by considering a canonical average over all possible nuclear states. The result maintains the same form as in Eq. (199), except that we now have the Bose-Einstein occupations nqν ðTÞ (see footnote 3). Equation (199) is precisely the conceptual starting point of the Allen-Heine theory of temperature-dependent band structures and appeared for the first time in Allen and Cardona (1981). If the variations Δqν Δ−qν εnk are calculated in second-order perturbation theory, one obtains precisely the formalism of Allen and Heine. It was proposed that the coefficients ∂εnk =∂nqν could alternatively be obtained from the derivatives of the vibrational frequencies with respect to the electronic occupations ℏ∂ωqν =∂fnk (Allen and Hui, 1980; King-Smith et al., 1989; Poncé, Antonius, Gillet et al., 2014). A formal derivation of the link between these alternative approaches can be found in Allen and Hui (1980), Appendix; they refer to this as Brooks’ theorem. Incidentally, the first ab initio calculation of temperature-dependent band gaps relied on this approach (King-Smith et al., 1989). Most commonly, the coefficients ∂εnk =∂nqν in Eq. (199) are evaluated using frozen-phonon supercell calculations, via the second derivative of the eigenvalue εnk with respect to collective atomic displacements along the vibrational eigenmodes eκαν ðqÞ. This approach was employed by Capaz et al. (2005) to study the temperature dependence of the band gaps in carbon nanotubes (within a tight-binding model), Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 and by Han and Bester (2013) to obtain the zero-point renormalization and temperature dependence of the gaps of silicon and diamond quantum dots. Recent examples include works on diamond, silicon, SiC (Monserrat and Needs, 2014), as well as CsSnI3 (Patrick, Jacobsen, and Thygesen, 2015). Frozen-phonon supercell calculations based on Eq. (199) carry the advantage that the rigid-ion approximation, which is necessary to obtain Eqs. (195)–(198), is no longer required. Therefore this approach is more accurate in principle. In practice, however, the calculations are challenging as they require large supercells, and the derivatives must be evaluated for every vibrational mode of the supercell. Several computational strategies were developed to tackle this challenge. Patrick and Giustino (2013) proposed to perform the averages leading to Eq. (199) via importance-sampling Monte Carlo integration. Monserrat (2016b) described a constrained Monte Carlo scheme which improves the variance of the Monte Carlo estimator. Recently Zacharias and Giustino (2016) showed that it is possible to perform these calculations more efficiently by replacing the stochastic sampling by a suitable choice of an “optimum” configuration; the result becomes exact in the thermodynamic limit of large supercells. In order to reduce the computational cost associated with the use of large supercells, Lloyd-Williams and Monserrat (2015) introduced nondiagonal supercells, which allow one to access phonon wave vectors belonging to a uniform grid of N p points using supercells containing only N p1=3 unit cells. The merit of these nonperturbative approaches is that they explicitly treat the nuclear wave functions and enable exploring effects which go beyond the Allen-Heine theory. For example, Monserrat, Drummond, and Needs (2013), Monserrat et al. (2014), Engel, Monserrat, and Needs (2015), and Monserrat, Engel, and Needs (2015) were able to investigate effects beyond the harmonic approximations in several systems, such as LiH, LiD, high-pressure He, molecular crystals of CH4 , NH3 , H2 O, HF, as well as ice. In all these cases they found large zero-point effects on the band gaps. Finally, we mention that the calculation of electronic properties at finite temperature via the Allen-Heine theory and its variants is closely related to what one would obtain using pathintegral molecular dynamics simulations (Della Sala et al., 2004; Ramírez, Herrero, and Hernández, 2006; Ramírez et al., 2008), or even classical molecular dynamics simulations at high enough temperatures (Franceschetti, 2007). B. Phonon-assisted optical absorption In addition to modifying the electron energy levels in solids, the electron-phonon interaction plays an important role in the optical properties of semiconductors and insulators, as it is responsible for phonon-assisted optical transitions. Phonon-assisted processes could be analyzed by considering the many-body electronic screening function ϵe ð12Þ in Eq. (95), by using the electron Green’s function G dressed by the electron-phonon self-energy Σep as in Eq. (151). Since this requires a lengthy detour, here we simply reproduce the standard result of second-order time-dependent perturbation theory (Bassani and Parravicini, 1975; Ridley, 1993): 015003-44 Feliciano Giustino: Electron-phonon interactions from first … Z πe2 1 dkdq X X ðfnk − fmkþq Þ ϵ0 cΩ ωnr ðωÞ Ω2BZ mnν s¼1 X vnp ðkÞgpmν ðk;qÞ gnpν ðk; qÞvpm ðk þ qÞ 2 þ ×e · εpk − εnk − ℏω εpkþq − εnk þ sℏωqν p αðωÞ ¼ × ðnqν þ 1=2 þ s=2Þδðεmkþq − εnk − ℏω þ sℏωqν Þ: ð200Þ In this expression αðωÞ is the absorption coefficient for visible light, e is the photon polarization, vmn are the matrix elements of the electron velocity operator, and nr ðωÞ is the real part of the refractive index. The two denominators in the second line correspond to indirect processes whereby a photon is absorbed and a phonon is absorbed or emitted (left), and processes whereby a phonon is absorbed or emitted, and subsequently a photon is absorbed (right). Equation (200) relies on the electric dipole approximation and is therefore valid for photon energies up to a few electron volts. The theory leading to Eq. (200) was originally developed by Hall, Bardeen, and Blatt (1954). The first ab initio calculation employing Eq. (200) was reported by Noffsinger et al. (2012) for the prototypical case of silicon. They employed DFT for computing phonons and electron-phonon matrix elements and the GW method for the quasiparticle band structures. The sampling of the Brillouin zone was achieved by means of the interpolation strategy described in Sec. VI. Figure 14 shows that the calculations by Noffsinger et al. are in very good agreement with experiment throughout the energy range of indirect absorption. Further work along similar lines was reported by Kioupakis et al. (2010), who calculated the indirect optical absorption by free carriers in GaN, and Peelaers, Kioupakis, and Van de Walle (2015), who studied the indirect absorption by free carriers in the transparent conducting oxide SnO2 . Recently, the ab initio theory of phonon-assisted absorption was also extended to the case of indirect Auger recombination by Kioupakis et al. (2015). One limitation of the theory by Hall et al. is that the indirect absorption onset is independent of temperature. This is seen by noting that the Dirac delta functions in Eq. (200) contain the band structure energies at clamped nuclei. The generalization to incorporate temperature-dependent band structures as discussed in Sec. IX.A.1 is nontrivial. Patrick and Giustino (2014) and Zacharias and Giustino (2016) showed that the electron-phonon renormalization of the band structure modifies the energies of real transitions but leaves unchanged the energies of virtual transitions. In other words the Allen-Heine renormalization should be incorporated only in the Dirac delta functions and in the first denominator in Eq. (200). In order to avoid these complications, Zacharias, Patrick, and Giustino (2015) developed an alternative approach which relies on the semiclassical approximation of Williams (1951) and Lax (1952). In this approximation, the initial states in the optical transitions are described quantum mechanically, and the final states are replaced by a quasiclassical continuum. In the formulation of Zacharias et al. the imaginary part of the temperature-dependent dielectric function takes the following form: ϵ2 ðω; TÞ ¼ 1 X −Efnqν g =kB T e hϵ2 ðωÞifnqν g ; Z fn g ð201Þ qν where ϵ2 ðωÞ denotes the imaginary part of the dielectric function at clamped nuclei, and the expectation values have the same meaning as in Eq. (199). Efnqν g is the energy of the quantum nuclear state specified by the quantum number fnqν g and Z is the canonical partition function. Zacharias et al. demonstrated that this approach provides an adiabatic approximation to Eq. (200) and seamlessly includes the temperature dependence of the electronic structure within the Allen-Heine theory. Using techniques similar to those of Sec. IX.A.2, they calculated the indirect optical absorption line shape of silicon at various temperatures and obtained very good agreement with experiment. These results were recently extended to the temperature-dependent optical spectra of diamond and gallium arsenide by Zacharias and Giustino (2016). X. CARRIER DYNAMICS AND TRANSPORT A. Electron linewidths and lifetimes FIG. 14. Phonon-assisted optical absorption in silicon: com- parison between first-principles calculations (solid lines, orange) and experiment (circles, blue). The calculations were performed using the theory of Hall, Bardeen, and Blatt (1954), as given by Eq. (200). Spectra calculated at different temperatures were shifted horizontally so as to match the experimental onsets. From Noffsinger et al., 2012. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 In Sec. V.B.4 we have seen how the Fan-Migdal self-energy can be used in order to evaluate the quasiparticle lifetimes (or equivalently linewidths) resulting from the electron-phonon interaction. The first ab initio calculations of this kind were reported by Eiguren et al. (2002) and Eiguren, de Gironcoli et al. (2003) in the study of the decay of metal surface states, and by Sklyadneva et al. (2005, 2006) and Leonardo et al. (2007) in the study of electron lifetimes of elemental metals. Some of these calculations and the underlying approximations were reviewed in Sec. VIII. Calculations of quasiparticle linewidths were also employed to study the temperature-dependent broadening of the optical spectra in 015003-45 Feliciano Giustino: Electron-phonon interactions from first … semiconductors. For example, Giustino, Louie, and Cohen (2010) and Poncé et al. (2015) investigated the broadening of the direct absorption edge of diamond and silicon, respectively. In both cases good agreement with experiment was obtained. More recently, the same approach was employed to study the broadening of photoluminescence peaks in leadiodide perovskites (Wright et al., 2016). In this case, it was found that the standard Fermi golden rule expression, Eq. (170), significantly overestimates the experimental data. The agreement with experiment is restored by taking into account the quasiparticle renormalization Znk ; see the discussion following Eq. (174). While these works were primarily concerned with the broadening of the spectral lines in photoemission or optical experiments, Eq. (170) can also be used to study carrier lifetimes in time-resolved experiments. The first ab initio study in this direction was reported by Sjakste, Vast, and Tyuterev (2007), who investigated the thermalization of hot electrons in GaAs and the exciton lifetimes in GaP. In the case of GaAs, Sjakste et al. found thermalization rates in quantitative agreement with time-resolved luminescence and transient optical absorption measurements. Work along similar lines was also reported for the intervalley scattering times in Ge (Tyuterev et al., 2011). Recently, the thermalization rates of hot electrons in GaAs were revisited by Bernardi et al. (2015). They employed Eq. (170) and the Wannier interpolation technique described in Sec. VI in order to finely sample the electron-phonon scattering processes near the bottom of the conduction band; see Fig. 15. Based on these calculations they were able to interpret transient absorption measurements in terms of the carrier lifetimes within each valley. Another interesting application of Eq. (170) was reported by Bernardi et al. (2014), who investigated the rate of hot carrier thermalization in silicon, within the context of photovoltaics applications. Recently Sangalli and Marini (2015a, 2015b) employed the lifetimes calculated using Eq. (170) in order to study carrier dynamics in silicon in real time. Strictly speaking, these developments lie outside of the scope of equilibrium Green’s functions discussed in Sec. IV and require concepts based on nonequilibrium Green’s functions (Kadanoff and Baym, 1962). However, the basic ingredients of the electron-phonon calculations remain unchanged. In all calculations discussed in this section, the electronphonon matrix elements were obtained within DFT. However, in order to accurately describe electron-phonon scattering near band extrema Bernardi et al. (2014, 2015) and Wright et al. (2016) employed GW quasiparticle band structures. This is important in order to obtain accurate band effective masses, which affect the carrier lifetimes via the density of states. B. Phonon-limited mobility The carrier lifetimes τnk of Eq. (170) are also useful in the calculation of electrical mobility, conductivity, and resistivity, within the context of the semiclassical model of electron dynamics in solids (Ashcroft and Mermin, 1976). In the semiclassical model, one describes the electronic response to an external perturbation by taking the fermionic occupations fnk to represent the probability density function in the phase space defined by the unperturbed band structure. The probabilities fnk are then determined using a standard Boltzmann equation. A comprehensive discussion of these methods can be found in the classic book of Ziman (1960). Here we touch only upon the key result which is needed in ab initio calculations of electrical conductivity. In the semiclassicalP model, the electrical current is calculated as R dkv J ¼ −2eΩ−1 nk f nk . In the absence of external fields n BZ and thermal gradients, the occupations f nk reduce to the standard Fermi-Dirac occupations at equilibrium f0nk , and the current vanishes identically. Upon introducing an electric field E, the electrons respond by adjusting their occupations. In this model it is assumed that the variation f nk − f 0nk is so small that the electronic density is essentially the same as in the unperturbed system. The modified occupations can be calculated using the linearized Boltzmann transport equation (Ziman, 1960) X ∂f0nk vnk · ð−eÞE ¼ − ∂εnk ν Z dq Γ ðk; qÞ ΩBZ mnν × ½ðfnk − f0nk Þ − ðf mkþq − f0mkþq Þ; ð202Þ where the kernel Γmnν ðk; qÞ is defined as Γmnν ðk; qÞ ¼ X 2π jg ðk; qÞj2 f0nk ð1 − f0mkþq Þ ℏ mnν s¼1 × ðnqν þ 1=2 − s=2Þδðεnk þ sℏωqν − εmkþq Þ: ð203Þ FIG. 15. Electron relaxation times in GaAs resulting from electron-phonon scattering. (a) Calculated relaxation times as a function of electron energy with respect to the conduction band bottom. The color code (gray shades) of the data points identifies the valley where each electronic state belongs. (b) Schematic representation of the conduction band valleys in GaAs. From Bernardi et al., 2015. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 The left-hand side of Eq. (202) represents the collisionless term of the Boltzmann equation, that is, the change in occupations due to the particle drift under the electric field. The right-hand side represents the change of occupations resulting from electrons scattered in or out of the state jnki by phonon emission or absorption. The rates in Eq. (203) are simply derived from Fermi’s golden rule (Grimvall, 1981). By solving Eq. (202) self-consistently for all f nk it is possible to calculate the current and from there the conductivity. The connection with the carrier lifetimes τnk of Eq. (170) is 015003-46 Feliciano Giustino: Electron-phonon interactions from first … obtained within the so-called “energy relaxation time approximation.” In this approximation the incoming electrons are neglected in Eq. (202); that is, the last term ðfmkþq − f0mkþq Þ in the second line is ignored. As a result the entire right-hand side of the equation simplifies to −ðf nk − f0nk Þ=τnk . The direct solution of Eq. (202) is computationally challenging, and fully ab initio calculations were reported only recently by Li (2015) for Si, MoS2 , and Al, and by Fiorentini and Bonini (2016) for n-doped Si. Figure 16 shows that the mobility of n-type silicon calculated by Li is in good agreement with experiment. The theory overestimates the measured values to some extent, and this might have to do with the limitations of the DFT matrix elements (see Sec. XII). In addition to the carrier mobility, Fiorentini and Bonini employed the ab initio Boltzmann formalism to calculate thermoelectric properties, such as the Lorenz number and the Seebeck coefficient. The first ab initio calculation of mobility was reported by Restrepo, Varga, and Pantelides (2009) for the case of silicon, within the energy relaxation time approximation. Other recent calculations using various approximations to Eq. (202) focused on silicon (Wang et al., 2011; Liao et al., 2015), graphene (Borysenko et al., 2010; Park et al., 2014; Restrepo et al., 2014; Sohier et al., 2014; Gunst et al., 2016; Kim, Park, and Marzari, 2016), MoS2 (Kaasbjerg, Thygesen, and Jacobsen, 2012; Li et al., 2013; Restrepo et al., 2014; Gunst et al., 2016), silicene (Li et al., 2013; Gunst et al., 2016), and SrTiO3 and KTiO3 (Himmetoglu et al., 2014; Himmetoglu and Janotti, 2016). Ab initio calculations of the resistivity of metals are less challenging than for semiconductors and started appearing already from the work of Bauer et al. (1998). Most calculations on metals are based on Ziman’s resistivity formula; see Grimvall (1981). An interesting recent example can be found in the work by Xu and Verstraete (2014) on the transport coefficients of lithium. We also highlight related work on phonon-limited transport in organic crystals (Hannewald and Bobbert, 2004a, 2004b; Ortmann, Bechstedt, and Hannewald, 2009; Vukmirović, Bruder, and Stojanović, 2012). XI. PHONON-MEDIATED SUPERCONDUCTORS The last application of ab initio calculations of EPIs that we consider here is the study of phonon-mediated superconductivity (Schrieffer, 1983). This research field is so vast that any attempt at covering it in a few pages would not do justice to the subject. For this reason, it was decided to limit the discussion to those novel theoretical and methodological developments which are aiming at fully predictive calculations, namely, the “anisotropic Migdal-Eliashberg theory” (Sec. XI.B) and the “density-functional theory for superconductors” (Sec. XI.C). For completeness, in Sec. XI.A we also summarized the most popular equations employed in the study of phonon-mediated superconductors. All calculations described in this section were performed at the DFT level. A. McMillan–Allen-Dynes formula Most ab initio calculations on phonon-mediated superconductors rely on a semiempirical expression for the critical temperature, first introduced by McMillan (1968) and then refined by Allen and Dynes (1975): ℏωlog 1.04ð1 þ λÞ exp − : kB T c ¼ 1.2 λ − μ ð1 þ 0.62λÞ Here T c is the superconducting critical temperature, ωlog is a logarithmic average of the phonon frequencies (Allen and Dynes, 1975), λ is the electron-phonon “coupling strength,” and μ is a parameter describing the Coulomb repulsion. The functional form of Eq. (204) was derived by McMillan by determining an approximate solution of the Eliashberg gap equations (see Sec. XI.B). λ and ωlog are calculated from the isotropic version of the Eliashberg function in Eq. (187) as follows (McMillan, 1968; Allen and Dynes, 1975; Grimvall, 1981; Allen and Mitrovic, 1982): 1 α FðωÞ ¼ NF 2 Z dkdq X jgmnν ðk; qÞj2 δðεnk − εF Þ Ω2BZ mnν × δðεmkþq − εF Þδðℏω − ℏωqν Þ; Z ωlog ¼ exp Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 ð205Þ α2 FðωÞ dω; ω ð206Þ Z 2 ∞ α2 FðωÞ log ω ; dω λ 0 ω ð207Þ λ¼2 FIG. 16. Temperature-dependent mobility of n-type silicon. The solid line (red) indicates the mobility calculated using the linearized Boltzmann transport equation, Eq. (202), and the dashed line (blue) corresponds to the energy relaxation time approximation. The triangles and diamonds are experimental data points. From Li, 2015. ð204Þ 0 ∞ where N F is the density of states at the Fermi level and the matrix elements gmnν ðk; qÞ are the same as in Eq. (38). The remaining parameter μ (Morel and Anderson, 1962) is obtained as 1=μ ¼ 1=μ þ logðωp =ωph Þ, where ℏωp is the characteristic plasma energy of the system, ℏωph the largest phonon energy, and μ is the average electron-electron Coulomb repulsion across the Fermi surface. More specifically, μ ¼ N F ⟪V nk;n0 k0 ⟫FS , where ⟪ ⟫FS denotes a double average over the Fermi surface, and V nk;n0 k0 ¼ hk0 n0 ; −k0 n0 jWjkn; −kni, with W the screened Coulomb interaction of Sec. IV.B.2 (Lee, Chang, and Cohen, 1995; Lee and Chang, 1996). 015003-47 Feliciano Giustino: Electron-phonon interactions from first … The coupling strength λ is related to the mass enhancement parameter λnk discussed in Sec. VIII.A. The main difference between λ and λnk is that the former represents an average over the Fermi surface, while the latter refers to the Fermi velocity renormalization of a specific electron band. While these quantities are related, they do not coincide and hence cannot be used interchangeably. Equations (204)–(207) involve a number of approximations. For example, it is assumed that the superconductor is isotropic and exhibits a single superconducting gap. Furthermore, almost invariably the effective Coulomb potential μ is treated as an adjustable parameter on the grounds that it should be in the range μ ¼ 0.1–0.2. This procedure introduces a large uncertainty in the determination of T c , especially at moderate coupling strengths. B. Anisotropic Migdal-Eliashberg theory A first-principles approach to the calculation of the superconducting critical temperature is provided by the anisotropic Migdal-Eliashberg theory (Migdal, 1958; Eliashberg, 1960). This is a field-theoretic approach to the superconducting pairing, formulated in the language of finite-temperature Green’s functions. At variance with the Hedin-Baym equations of Table I, the Migdal-Eliashberg theory is best developed within the Nambu-Gor’kov formalism (Gor’kov, 1958; Nambu, 1960), which enables describing the propagation of electron quasiparticles and of superconducting Cooper pairs on the same footing (Scalapino, 1969; Schrieffer, 1983). A comprehensive presentation of the Migdal-Eliashberg theory is provided by Allen and Mitrovic (1982). Their article served as the starting point of current first-principles implementations of the theory. In the Migdal-Eliashberg theory, one solves the following two coupled equations: Znk ðiωj Þ ¼ 1 þ λnk;n0 k0 ðiωÞ ¼ N F X 2ωqν jg 0 ðk; qÞj2 ; ℏ ν ω2qν þ ω2 nn ν ð210Þ with q ¼ k0 − k. Equations (208) and (209) are to be solved self-consistently for each temperature T. The superconducting critical temperature is then obtained as the highest temperature for which a nontrivial solution is obtained, that is, a solution with Δnk ðiωj Þ ≠ 0. From the superconducting gap along the imaginary axis it is then possible to obtain the gap at real frequencies by analytic continuation (Marsiglio, Schossmann, and Carbotte, 1988), and from there one can compute various thermodynamic functions. The first ab initio implementation of the anisotropic Migdal-Eliashberg theory was reported by Choi et al. (2002a, 2002b) and Choi, Cohen, and Louie (2003) in a study of the superconducting properties of MgB2 . They succeeded in explaining the anomalous heat capacity of MgB2 in terms of two distinct superconducting gaps and obtained a T c in good agreement with experiment. These calculations were later extended to MgB2 under pressure (Choi, Louie, and Cohen, 2009a) and other hypothetical borides (Choi, Louie, and Cohen, 2009b). Margine and Giustino (2013) demonstrated an implementation of the Migdal-Eliashberg theory based on the Wannier interpolation scheme of Sec. VI and reported applications to Pb and MgB2 . The superconducting gap and superconducting density of states of MgB2 calculated by Margine and Giustino are shown in Fig. 17. In all these calculations, the Coulomb repulsion ωj0 =ωj πkB T X qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ N F n0 k0 j0 ℏ2 ω20 þ Δ20 0 ðiω 0 Þ nk j j × λnk;n0 k0 ðiωj − iωj0 Þδðεn0 k0 − εF Þ; Znk ðiωj ÞΔnk ðiωj Þ ¼ ð208Þ Δn0 k0 ðiωj0 Þ πkB T X qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ N F n0 k0 j0 ℏ2 ω20 þ Δ20 0 ðiω 0 Þ j nk j × ½λnk;n0 k0 ðiωj − iωj0 Þ − N F V nk;n0 k0 × δðεn0 k0 − εF Þ; ð209Þ R 0 P −1 where k0 stands for ΩBZ dk . In these equations, T is the absolute temperature, and Znk ðiωj Þ is the quasiparticle renormalization function and is analogous to Znk in Eq. (189). Δnk ðiωj Þ is the superconducting gap function. The functions Znk ðiωj Þ and Δnk ðiωj Þ are determined along the imaginary frequency axis at the fermion Matsubara frequencies iωj ¼ ið2j þ 1ÞπkB T=ℏ with j an integer. The anisotropic and frequency-dependent generalization of Eq. (206) to be used in the Migdal-Eliashberg equations is Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 FIG. 17. (a) Energy distribution of the superconducting gap function of MgB2 as a function of temperature, calculated using the anisotropic Migdal-Eliashberg theory. The gap vanishes at the critical temperature (in this calculation T c ¼ 50 K). Two distinct superconducting gaps can be seen at each temperature. (b) Density of electronic states in the superconducting state of MgB2 at various temperatures calculated within the Migdal-Eliashberg theory. From Margine and Giustino, 2013. 015003-48 Feliciano Giustino: Electron-phonon interactions from first … was described empirically via μ , and this partly accounts for the slight discrepancy between the calculated T c of 50 K and the experimental T c of 39 K (Nagamatsu et al., 2001). Additional calculations based on the anisotropic MigdalEliashberg theory included a study of doped graphene (Margine and Giustino, 2014), as well as investigations of Li-decorated monolayer graphene (Zheng and Margine, 2016) and Ca-intercalated bilayer graphene (Margine, Lambert, and Giustino, 2016). In this latter work they incorporated Coulomb interactions from first principles, after calculating μ via the screened Coulomb interaction in the random-phase approximation. The calculated T c ¼ 7–8 K was in reasonable agreement with the experimental value of 4 K (Ichinokura et al., 2016). The Migdal-Eliashberg theory was also extended to describe the superconducting state as a function of applied magnetic field. A complete ab initio implementation was successfully demonstrated with an application to MgB2 (Aperis, Maldonado, and Oppeneer, 2015). Recently Sano et al. (2016) performed ab initio Migdal-Eliashberg calculations including retardation effects on high-pressure sulfur hydrides, obtaining good agreement with experiment. Interestingly in this work they also checked the effect of the zero-point renormalization of the electron bands within the Allen-Heine theory and found that it accounts for a change in T c of up to 20 K. C. Density-functional theory for superconductors Another promising ab initio approach to the calculation of the superconducting critical temperature is the densityfunctional theory for superconductors (Lüders et al., 2005; Marques et al., 2005). The starting point of this approach is a generalization of the Hohenberg-Kohn theorem (Hohenberg and Kohn, 1964) to a system described by three densities: the electron density in the normal state, the density of superconducting pairs, and the nuclear density. Based on this premise, Luders et al. mapped the fully interacting system into an equivalent Kohn-Sham system (Kohn and Sham, 1965) of noninteracting nuclei and noninteracting, yet superconducting, electrons. The resulting Kohn-Sham equations for the electrons take the form of Bogoliubov–de Gennes equations (Bogoliubov, 1958), whereby electrons are paired by an effective gap function Δðr; r0 Þ. In its simplest formulation, the density-functional theory for superconductors determines the expectation value of the pairing field over Kohn-Sham eigenstates Δnk ¼ hunk ðrÞjΔðr; r0 Þjunk ðr0 Þi, using the following gap equation: Δnk ¼ −Z nk Δnk − X Knk;n0 k0 Δn0 k0 n0 k 0 2En0 k0 E n0 k 0 ; tanh 2kB T ð211Þ where E2nk ¼ ε2nk þ jΔnk j2 . In this expression, the kernel K contains information about the phonon-mediated pairing interaction and the Coulomb repulsion between electrons K ¼ Kep þ Kee , and Z contains information about the electron-phonon interaction. More specifically, Kep and Z are evaluated starting from the electron-phonon matrix elements gmnν ðk; qÞ and the DFT electron band structure and phonon dispersions, as in the Migdal-Eliashberg theory. Kee is Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 approximated using the screened Coulomb interaction V nk;n0 k0 introduced below Eq. (207). Complete expressions for Z and K can be found in Marques et al. (2005). Equation (211) is reminiscent of the gap equation in the Bardeen-Cooper-Schrieffer (BCS) theory (Schrieffer, 1983), with the difference that the ab initio kernel K replaces the model interaction of the BCS theory, and the function Z introduces quasiparticle renormalization as in the MigdalEliashberg theory; see Eq. (208). At variance with the MigdalEliashberg theory, the gap function in the density-functional theory for superconductors does not carry an explicit frequency dependence. Nevertheless, retardation effects are fully included through the dependence of the kernels Z and K on the electron bands and the phonon dispersions. An important advantage of this theory is that the Coulomb potential μ is not required, since the electron-electron repulsion is seamlessly taken into account by means of the kernel Kee . The density-functional theory for superconductors was successfully employed to study the superconducting properties of MgB2 (Floris et al., 2005), Li, K, and Al under pressure (Profeta et al., 2006; Sanna et al., 2006), Pb (Floris et al., 2007), Ca-intercalated graphite (Sanna et al., 2007), highpressure hydrogen (Cudazzo et al., 2008, 2010), CaBeSi (Bersier et al., 2009), layered nitrides (Akashi et al., 2012), alkali-doped fullerides (Akashi and Arita, 2013b), compressed sulfur hydrides (Akashi et al., 2015), and intercalated layered carbides, silicides, and germanides (Flores-Livas and Sanna, 2015). An interesting recent development of the theory was the determination of the superconducting order parameter in real space χðr; r0 Þ ¼ hψ̂ ↑ ðrÞψ̂ ↓ ðr0 Þi (Linscheid, Sanna, Floris, and Gross, 2015). In the density-functional theory for superconductors, the order parameter is obtained from the superconducting gap using χ nk ¼ ðΔnk =2jEnk jÞtanh½Enk =ð2kB TÞ. Figure 18 shows the order parameter calculated by Linscheid et al. for both MgB2 and hole-doped graphane (Savini, Ferrari, and Giustino, 2010). The plots show Friedel-like oscillations of the superconducting density as a function of the relative coordinates between two paired electrons. FIG. 18. Superconducting order parameter χðr; r0 Þ in real space, calculated for (a) MgB2 and (b) hole-doped graphane. The plots show a top view (top) and a side view (bottom) of the hexagonal layers in each case. The variable s ¼ r − r0 is the relative coordinate in the order parameter, while the center-of-mass coordinate is placed in the middle of a B-B bond or a C-C bond. From Linscheid, Sanna, Floris, and Gross, 2015. 015003-49 Feliciano Giustino: Electron-phonon interactions from first … Further developments of the superconducting densityfunctional theory include the study of nonphononic pairing mechanisms, such as plasmon-assisted superconductivity (Akashi and Arita, 2013a), and the extension to magnetic systems (Linscheid, Sanna, Essenberger, and Gross, 2015; Linscheid, Sanna, and Gross, 2015). XII. ELECTRON-PHONON INTERACTIONS BEYOND THE LOCAL DENSITY APPROXIMATION TO DFT The calculations of electron-phonon interactions reviewed in Secs. VII–XI have in common the fact that most investigations used the local density approximation to DFT or a generalized gradient approximation (GGA) such as the PBE functional (Perdew, Burke, and Ernzerhof, 1996). Although the LDA and the GGA represent the workhorse of electronphonon calculations from first principles, there is growing evidence that these choices can lead to an underestimation of the electron-phonon coupling strength. At a conceptual level we understand this point by rewriting the electron-phonon matrix element after combining Eqs. (38), (142), and (143): Z gmnν ðk; qÞ ¼ humkþq j 0 en 0 dr0 ϵ−1 e ðr; r ; ωÞΔqν v ðr Þjunk iuc : ð212Þ In DFT the many-body dielectric matrix ϵe appearing in this expression is replaced by the RPA þ xc screening ϵHxc from Eq. (54). Given the DFT band gap problem, we expect ϵHxc to overestimate the screening, thereby leading to matrix elements gmnν ðk; qÞ which are underestimated to some extent. Several groups investigated this point on quantitative grounds. Zhang, Louie, and Cohen (2007) studied the electron-phonon coupling in a model copper oxide superconductor CaCuO2. By calculating the vibrational frequencies of the half-breathing Cu-O stretching mode, they established that the local spin-density approximation (LSDA) yields phonons which are too soft (65.3 meV) as compared to experiment (80.1 meV). In contrast, the introduction of Hubbard corrections in a LSDA þ U scheme restored agreement with experiment (80.9 meV). Since the electron-phonon matrix elements are connected to the phonon frequencies via the phonon selfenergy, Eq. (145), a corresponding underestimation of the matrix elements can be expected. These results were supported by the work of Floris et al. (2011), who developed DFPT within LSDA þ U and applied their formalism to the phonon dispersions of antiferromagnetic MnO and NiO. They found that the DFT underestimates measured LO energies by as much as 15 meV in MnO, while the use of LSDA þ U leads to good agreement with experiment. Related work was reported by Hong et al. (2012), who investigated the multiferroic perovskites CaMnO3 , SrMnO3 , BaMnO3 , LaCrO3 , LaFeO3 , and the double perovskite La2 CrFeO6 . They calculated the variation of the vibrational frequencies between the ferromagnetic and antiferromagnetic phases of these compounds as a function of the Hubbard U parameter and compared DFT þ U calculations with hybrid-functional calculations. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Lazzeri et al. (2008) investigated the effect of quasiparticle GW corrections on the electron-phonon coupling of graphene and graphite, for the A1 0 phonon at K and the E2g phonon at Γ. They evaluated the intraband electron-phonon matrix elements using a frozen-phonon approach, noting that gnnν ðk; q ¼ 0Þ precisely represents the shift of the KohnSham energy εnk upon displacing the atoms according to the νth phonon eigenmode at q ¼ 0. Lazzeri et al. found that the matrix elements increase by almost 40% from DFT to GW. The GW values led to slopes in the phonon dispersions near K in very good agreement with inelastic x-ray scattering data (Grüneis et al., 2009b). Similar results, albeit less dramatic, were obtained by Grüneis et al. (2009a) for the potassiumintercalated graphite KC8 . Laflamme Janssen et al. (2010) studied the electron-phonon coupling in the C60 molecule as a model for superconducting alkali-doped fullerides. They employed the PBE0 hybrid functional (Perdew, Ernzerhof, and Burke, 1996) with a fraction of exact exchange α ¼ 30% and obtained an enhancement of the total coupling strength λ of 42% as compared to PBE. This work was followed up by Faber et al. (2011), who used the GW approximation and obtained a similar enhancement of 48%. We also point out an earlier work by Saito (2002) based on the B3LYP functional, reporting similar results. Yin, Kutepov, and Kotliar (2013) investigated the effects of using the GW approximation and the HSE hybrid functional (Heyd, Scuseria, and Ernzerhof, 2003) on the electronphonon coupling in the superconducting bismuthates Ba1−x Kx BiO3 and chloronitrides β-ZrNCl, as well as MgB2 . In the case of Ba1−x Kx BiO3 they obtained a threefold increase in the coupling strength λ from PBE to HSE. This enhancement brought the critical temperature calculated using Eq. (204) to 31 K, very close to the experimental value of 32 K. Similarly, in the case of β-ZrNCl, Yin et al. obtained a 50% increase of λ, bringing the calculated critical temperature of 18 K close to the experimental value of 16 K. Instead, in the case of MgB2 , they noticed only a slight increase of the electron-phonon coupling as compared to the standard LDA. Another application of hybrid functionals to the study of EPIs was reported by Komelj and Krakauer (2015). They investigated the sensitivity of the superconducting critical temperature of the H3 S phase of sulfur hydride to the exchange and correlation functionals. They found that the PBE0 functional enhances the critical temperature by up to 25% as compared to PBE, bringing T c from 201–217 K to 253–270 K (the spread in values is related to the choice of the parameter μ ). Mandal, Cohen, and Haule (2014) reported work on the superconductor FeSe based on dynamical mean-field theory (DMFT). In this case DMFT yielded a threefold enhancement of the coupling strength for selected modes. As mentioned in Sec. IX.A.1, Antonius et al. (2014) performed GW calculations of the electron-phonon coupling in diamond using a frozen-phonon approach. They found that quasiparticle corrections lead to a uniform enhancement of the electron-phonon matrix elements. The net effect is an increase of the zero-point renormalization of the band gap by 40% as compared to standard LDA calculations. Monserrat (2016a) 015003-50 Feliciano Giustino: Electron-phonon interactions from first … confirmed this result and found a GW correction of comparable magnitude in the case of silicon. However, Monserrat also found that the GW corrections to the zero-point band gap renormalization of LiF, MgO, and TiO2 are very small (∼5% of the PBE value); therefore at present it is not possible to draw general conclusions. Finally, we mention that Faber et al. (2015) examined possible strategies for systematically incorporating GW corrections in electron-phonon calculations. By using diamond, graphene, and C60 as test cases, they showed that a “constant screening” approximation is able to reproduce complete GW results with an error below 10% at reduced computational cost. This approximation amounts to evaluating the variation of the Green’s function G in a frozen-phonon calculation, while retaining the screened Coulomb interaction W of the unperturbed ground state. All these recent developments point to the need of moving beyond local exchange and correlation functionals in the study of electron-phonon interactions from first principles. In the future, it will be important to devise accurate computational methods for calculating not only the intraband electronphonon matrix elements (as in the frozen-phonon method) but also matrix elements between all states and for scattering across the entire Brillouin zone. For completeness we emphasize that the underestimation of the EPI matrix elements by semilocal DFT functionals does not propagate in the same way into different materials properties. This is readily understood by examining two fundamental quantities, the Allen-Heine renormalization of electron bands, Eq. (167), and the adiabatic phonon frequencies, as obtained from Eqs. (126) and (127). In the former case the electronic screening enters as ϵ−2 ∞ ; in the latter case the −1=2 . screening contributes through a term which scales with ϵ∞ As a result, in the hypothetical case of a semiconductor for which DFT underestimated the electronic permittivity by 20%, we would have an error of ∼40% in the energy renormalization, and of ∼10% in the phonon frequencies. This example is an oversimplification of the problem, but it shows that different properties relating to the EPI could be affected to a very different degree by the inherent limitations of DFT functionals. XIII. CONCLUSIONS The study of electron-phonon interactions has a long and distinguished history, but it is only during the past two decades that quantitative and predictive calculations have become possible. First-principles calculations of electronphonon couplings are finding an unprecedented variety of applications in many areas of condensed matter and materials physics, from spectroscopy to transport, from metals to semiconductors and superconductors. In this article we discussed the standard DFT formalism for performing calculations of electron-phonon interactions, showed how most equations can be derived from a field-theoretic framework using a few well-defined approximations, and reviewed recent applications of the theory to many materials of current interest. As calculation methods improve relentlessly and quantitative comparisons between theory and experiment become Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 increasingly refined, new and more complex questions arise. Much is still left to do, both in the fundamental theory of electron-phonon interactions and in the development of more accurate and more efficient computational methods. For one, we are still using theories where the coupling matrix elements are calculated using the adiabatic local density approximation to DFT. The need for moving beyond standard DFT and beyond the adiabatic approximation can hardly be overemphasized. Progress is being made on the incorporation of nonlocal corrections into electron-phonon matrix elements, for example, using hybrid functionals or GW techniques, but very little is known about retardation effects. It is expected that such effects may be important in the study of heavily doped oxides and semiconductors, in both their normal and superconducting states (Mahan, 1993, Sec. 6.3.A), but ab initio investigations are currently missing. This is truly uncharted territory and a systematic effort in this direction is warranted. In this article we emphasized that it is possible to formulate a compact, unified theory of electron-phonon interactions starting from a fully ab initio field-theoretic approach. The only assumption which is absolutely crucial to the theory is the harmonic approximation. Abandoning the harmonic approximation leads to the appearance of several new terms in the equations, and the resulting formalism becomes considerably more complex than in Table I. Despite these difficulties, given the importance of anharmonic effects in many systems of current interest, extending the theory to the case of anharmonic phonons and multiphonon interactions constitutes a pressing challenge. Ab initio investigations of anharmonic effects on the temperature dependence of band gaps have recently been reported (Monserrat, Drummond, and Needs, 2013; Antonius et al., 2015). Since these studies rely on nonperturbative adiabatic calculations in supercells, it is highly desirable to establish a clear formal connection of these methods with the rigorous field-theoretic approach of Sec. IV. Along the same line, it is important to clarify the relation between many-body approaches, adiabatic supercells calculations, and more traditional classical or path-integral molecular dynamics simulations. The study of electron-phonon interactions has long been dominated by Fröhlich-like Hamiltonians, whereby the electron-phonon coupling is retained only to linear order in the atomic displacements. This is the case for all the model Hamiltonians mentioned in Sec. V.B.6. It is now clear that quadratic couplings, leading to the Debye-Waller contributions in the optical spectra of semiconductors, are by no means negligible and should be investigated more systematically. For example, in the current literature it is invariably assumed that Debye-Waller contributions are negligible in metals near the Fermi surface; while this is probably the case for the simplest elemental metals, what happens in the case of multiple Fermisurface sheets is far from clear and should be tested by direct calculations. The identification of the correct matrix elements to be calculated is not always a trivial task as discussed for the case of the nonadiabatic phonon self-energy. In the future it will be important to pay attention to these aspects, especially in view of detailed comparison with experiment. For now, the issue of whether the phonon self-energy arising from EPIs should be 015003-51 Feliciano Giustino: Electron-phonon interactions from first … calculated using bare or screened EPI matrix elements (Sec. VII) is to be considered an open question and calls for further investigation. The theory and applications reviewed in this article focused on nonmagnetic systems. The rationale for this choice is that a complete many-body theory of electron-phonon interactions for magnetic systems is not available yet. Recent investigations of spin-phonon couplings were conducted by assuming that the spin and the vibrational degrees of freedom can be decoupled, as in the Born-Oppenheimer approximation. Under this assumption it is possible to investigate how the spin configuration responds to a frozen phonon or, alternatively, how the vibrational frequencies depend on the spin configuration [see, for example, Chan et al. (2007), Łażewski et al. (2010), Lee and Rabe (2011), and Cao, Giustino, and Radaelli (2015)]. In all these cases it is desirable to employ a more rigorous many-body theory of spin-phonon interactions. The Hedin-Baym equations discussed in Sec. IV maintain their validity in the case of spin-polarized systems, provided collinear spins are assumed. In more general situations, where it is important to consider noncollinear spins, external magnetic perturbations, or spin-dependent interactions such as spin-orbit and Rashba-Dresselhaus couplings, it becomes necessary to generalize the equations in Table I. Although such a generalization has not been reported yet, the work of Aryasetiawan and Biermann (2008) constitutes a promising starting point. In that work the Schwinger functional derivative technique (see Sec. IV.B.1) was used to extend Hedin’s equations at clamped nuclei to systems containing spindependent interactions. Generalizing Aryasetiawan and Biermann’s work to incorporate nuclear vibrations will be important for the study of electron-phonon interactions in many systems of current interest, from multifunctional materials to topological quantum matter. At this time it is not possible to predict how this fastmoving field will evolve over the years to come. However, the impressive progress made during the past decade gives us confidence that this interesting research area will continue to thrive and will keep surprising us with fascinating challenges and exciting new opportunities. ACKNOWLEDGMENTS I am indebted to Samuel Poncé, Carla Verdi, and Marios Zacharias for a critical reading of the manuscript, and to many colleagues who have kindly provided feedback on the arXiv preprint version of this article. This article is the result of many stimulating discussions with friends and colleagues over the last few years. I thank, in particular, Philip Allen, Stefano Baroni, Lilia Boeri, Nicola Bonini, Fabio Caruso, Hyoung Joon Choi, Marvin Cohen, Michel Côté, Andrea Dal Corso, Claudia Draxl, Asier Eiguren, Paolo Giannozzi, Stefano de Gironcoli, Giulia Galli, Xavier Gonze, Göran Grimvall, Eberhard Gross, Branko Gumhalter, Sohrab Ismail-Beigi, Emmanuil Kioupakis, Georg Kresse, Steven Louie, Roxana Margine, Andrea Marini, Miguel Marques, Nicola Marzari, Takashi Miyake, Bartomeu Monserrat, Jeffrey Neaton, Richard Needs, Jesse Noffsinger, Cheol-Hwan Park, Christopher Patrick, Warren Pickett, Samuel Poncé, Paolo Radaelli, Lucia Reining, John Rehr, Patrick Rinke, Angel Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Rubio, Matthias Scheffler, Young-Woo Son, Alexander Tkatchenko, Chris Van de Walle, Carla Verdi, Matthieu Verstraete, and Marios Zacharias. I also thank Marco Bernardi, Asier Eiguren, Xavier Gonze, Eberhard Gross, Wu Li, Steven Louie, and Francesco Mauri for kindly allowing me to reproduce their figures. This work was supported by the Leverhulme Trust (Grant No. RL-2012001), the Graphene Flagship (Horizon 2020 Grant No. 696656-GrapheneCorel), and the UK Engineering and Physical Sciences Research Council (Grants No. EP/J009857/ 1 and No. EP/M020517/1). APPENDIX A: BORN–VON KÁRMÁN BOUNDARY CONDITIONS In this Appendix we provide more details on the notation related to the Born–von Kármán boundary conditions used throughout this article. The crystalline unit cell is defined by the primitive lattice vectors ai with i ¼P1, 2, 3, and the pth unit cell is identified by the vector Rp ¼ i ni ai, with ni integers between 0 and N i − 1. The BvK supercell contains N p ¼ N 1 × N 2 × N 3 unit cells. The primitive vectors of the reciprocal lattice are denoted by bj and fulfill the duality condition ai · bj ¼ 2πδij . We consider Bloch wave vectors q belonging to a P uniform grid in one unit cell of the reciprocal lattice q ¼ j ðmj =N j Þbj , with mj being integers between 0 and N j − 1. This grid contains the same number of q vectors as the number of unit cells in the BvK supercell. From these definitions the standard sum rules follow: X expðiq · Rp Þ ¼ N p δp0 ; q X expðiq · Rp Þ ¼ N p δq0 : ðA1Þ p If G is a reciprocal lattice vector, the replacement of any of the q vectors by q þ G in these expressions and in all expressions presented in this article is inconsequential, since expðiG · Rp Þ ¼ 1. Similarly, any replacement of Rp by Rp þ T, where T is a lattice vector of the BvK supercell is inconsequential. Owing to these properties we are at liberty to replace the q grid with a Wigner-Seitz grid, i.e., the first Brillouin zone, and the supercell with a Wigner-Seitz supercell. These choices are useful for practical calculations in order to exploit the symmetry operations of the crystal and to truncate the interatomic force constants, given by Eq. (13), outside a Wigner-Seitz supercell. APPENDIX B: LADDER OPERATORS IN EXTENDED SYSTEMS In this Appendix we describe the construction of the phonon ladder operators âqν =â†qν and derive the phonon Hamiltonian given by Eq. (22). We show how the definition of the ladder operators depends on the behavior of the wave vector q under inversion. The normal modes introduced in Eq. (15) can be used to define a linear coordinate transformation of the ionic displacements as follows: 015003-52 Feliciano Giustino: Electron-phonon interactions from first … zqν ¼ N p−1=2 X e−iq·Rp ðMκ =M 0 Þ1=2 eκα;ν ðqÞΔτκαp : ðB1Þ Here zqν is referred to as a “complex normal coordinate” (Brüesch, 1982). The exponential and the masses in Eq. (B1) are chosen so as to obtain Eq. (22) starting from Eq. (12). Since there are 3MN p degrees of freedom, and since the complex normal coordinates correspond to 2 × 3MN p real variables, this coordinate transformation carries some redundancy. Indeed by combining Eqs. (18) and (B1) it is seen that z−qν ¼ zqν : Δτκαp ¼ N p−1=2 ðM 0 =M κ Þ1=2 X qν eiq·Rp eκα;ν ðqÞzqν : X q∈B;ν X eκα;ν ðqÞxqν eiq·Rp eκα;ν ðqÞðxqν þ iyqν Þ : ðB4Þ 1X Ĥp ¼ ℏω ð−∂ 2 =∂ x~ 2qν − ∂ 2 =∂ y~ 2qν þ x~ 2qν þ y~ 2qν Þ 2 q∈B;ν qν 1 X ℏω ð−∂ 2 =∂ x~ 2qν þ x~ 2qν Þ; 2 q∈A;ν qν ðB5Þ where for ease of notation we performed the scaling x~ qν ¼ xqν =2lqν Ĥp ¼ X q∈B;ν The q vectors of the set C have been grouped together with those in B by taking the real part in the second line. It can be verified that in this expression there are exactly 3MN p real coordinates; therefore we can choose the xqν for q in A and the pairs xqν , yqν for q in B as the independent variables. These variables are referred to as “real normal coordinates” (Brüesch, 1982). Using Eqs. (12)–(18), (A1), and (B4) the nuclear Hamiltonian can be written in terms of 3MN p independent harmonic oscillators in the real normal coordinates: þ pﬃﬃﬃ âqν;x ¼ ð~xqν þ ∂=∂ x~ qν Þ= 2; ðB3Þ q∈A;ν þ2Re for q in B; ðB7Þ ðB8Þ and similarly for âqν;y. With these definitions Eq. (B5) becomes The right-hand side is real valued after Eqs. (18) and (B2). In preparation for the transition to a quantum description of lattice vibrations, it is useful to identify 3MN p independent normal coordinates. This can be done by partitioning the grid of q vectors into three sets. We call A the set of vectors which are invariant under inversion, that is, −q þ G ¼ q for some reciprocal lattice vector G (including jGj ¼ 0). The center of the Brillouin zone and the centers of its faces belong to this set. The remaining vectors can be separated further into B and C, in such a way that all the vectors in C are obtained from those in B by inversion (modulo a reciprocal lattice vector). After defining zqν ¼ xqν þ iyqν , Eq. (B3) can be rewritten as N p−1=2 ðM0 =M κ Þ1=2 y~ qν ¼ yqν =lqν with lqν the zero-point displacement amplitude of Eq. (21). In the case of jqj ¼ 0 there are three normal modes for which ωqν ¼ 0, and the corresponding potential terms x~ 2qν must be removed from Eq. (B5). The eigenstates of Eq. (B5) are found by introducing the real ladder operators for each normal coordinate (CohenTannoudji, Diu, and Laloe, 1977): ðB2Þ The inverse relation of Eq. (B1) is Δτκαp ¼ x~ qν ¼ xqν =lqν ; καp for q in A; Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 ðB6Þ þ ℏωqν ðâ†qν;x âqν;x þ â†qν;y âqν;y þ 1Þ X ℏωqν ðâ†qν;x âqν;x þ 1=2Þ: ðB9Þ q∈A;ν The eigenstates of this Hamiltonian are products of simple harmonic oscillators (Merzbacher, 1998), and the ground state is −1=2ð χ 0 ðfτ κp gÞ ¼ Ae P q∈A;ν P x~ 2qν þ q∈B;ν x~ 2qν þ~y2qν Þ ; ðB10Þ with A a normalization constant. The relations between the positions τ κp and the normal coordinates x~ qν , y~ qν are given by Eqs. (B1), (B6), (B7), and (21). The eigenstates of Ĥ p can be generated by applying â†qν;x and â†qν;y to the ground state χ 0 . However this approach is not entirely satisfactory, since we cannot assign separate quantum numbers to modes with wave vectors q or −q. In order to avoid this inconvenience we observe that, for each normal mode, the first line of Eq. (B5) defines an effective isotropic two-dimensional harmonic oscillator. The degenerate eigenstates of this oscillator can be combined to form eigenstates of the angular momentum. This leads to right and left circular quanta with the same energy and definite angular momentum (Cohen-Tannoudji, Diu, and Laloe, 1977). This analogy motivates the consideration of the following linear combinations, for q in B: pﬃﬃﬃ âþ qν ¼ ðâqν;x þ iâqν;y Þ= 2; ðB11Þ pﬃﬃﬃ â−qν ¼ ðâqν;x − iâqν;y Þ= 2: ðB12Þ Since both âqν;x and âqν;y lower the energy of an eigenstate by the same quantum of energy ℏωqν, the resulting states are degenerate and their linear combinations are also eigenstates for the same eigenvalue. As a consequence we can generate all the eigenstates of the Hamiltonian Ĥp by acting on the ground −;† state χ 0 with the creation operators âþ;† qν and âqν . In this reasoning the wave vectors q belong to B; if we now consider Eqs. (B2), (B11), and (B12), we see that formally we also have − â−qν ¼ âþ −qν . Therefore it is natural to associate âqν to phonons propagating along the direction −q. 015003-53 Feliciano Giustino: Electron-phonon interactions from first … These observations suggest replacing the real ladder oper− ators of Eq. (B8) by the complex ladder operators âþ qν and â−qν for q in B and C, respectively. In the case of q in A we keep the real operators âqν;x . These definitions can be turned into the following compact expressions: âqν ¼ âqν;x for q in A; pﬃﬃﬃ âqν ¼ ðâqν;x þ iâqν;y Þ= 2 for q in B; C: ðB13Þ ðB14Þ Using these operators the nuclear Hamiltonian of Eq. (B5) takes the well-known form given by Eq. (22). Any eigenstate Q of Ĥp can now be generated as qν ðnqν !Þ−1=2 ðâ†qν Þnqν χ 0 . In this form we see that it is possible to independently assign a number of phonons nqν to each wave vector q and each mode ν. Using Eqs. (B6)–(B8), (B13), and (B14) we also have the basic identity zqν ¼ lqν ðâqν þ â†−qν Þ: ðB15Þ By combining this last expression with Eq. (B3) we obtain Eq. (20). REFERENCES Abrikosov, A. A., L. P. Gor’kov, and I. E. Dzyaloshinski, 1975, Methods of Quantum Field Theory in Statistical Physics (Dover, New York). Adler, S. L., 1962, “Quantum theory of the dielectric constant in real solids,” Phys. Rev. 126, 413–420. Agapito, L. A., A. Ferretti, A. Calzolari, S. Curtarolo, and M. Buongiorno Nardelli, 2013, “Effective and accurate representation of extended Bloch states on finite Hilbert spaces,” Phys. Rev. B 88, 165127. Akashi, R., and R. Arita, 2013a, “Development of density-functional theory for a plasmon-assisted superconducting state: Application to lithium under high pressures,” Phys. Rev. Lett. 111, 057006. Akashi, R., and R. Arita, 2013b, “Nonempirical study of superconductivity in alkali-doped fullerides based on density functional theory for superconductors,” Phys. Rev. B 88, 054510. Akashi, R., M. Kawamura, S. Tsuneyuki, Y. Nomura, and R. Arita, 2015, “First-principles study of the pressure and crystal-structure dependences of the superconducting transition temperature in compressed sulfur hydrides,” Phys. Rev. B 91, 224513. Akashi, R., K. Nakamura, R. Arita, and M. Imada, 2012, “Hightemperature superconductivity in layered nitrides β − Lix MNCl (M ¼ Ti, Zr, Hf): Insights from density functional theory for superconductors,” Phys. Rev. B 86, 054513. Albers, R. C., L. Bohlin, M. Roy, and J. W. Wilkins, 1976, “Normal and umklapp phonon decay rates due to phonon-phonon and electron-phonon scattering in potassium at low temperatures,” Phys. Rev. B 13, 768–786. Alexandrov, A. S., 2008, Polarons in advanced materials (Springer, New York). Alexandrov, A. S., and J. T. Devreese, 2010, Advances in polaron physics (Springer, New York). Allen, P. B., 1972a, “Electron-phonon coupling and pseudopotentials: The mass enhancements of the noble metals,” Phys. Rev. B 5, 3857–3862. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Allen, P. B., 1972b, “Neutron spectroscopy of superconductors,” Phys. Rev. B 6, 2577–2579. Allen, P. B., 1976, “Fermi-surface harmonics: A general method for nonspherical problems. application to Boltzmann and Eliashberg equations,” Phys. Rev. B 13, 1416–1427. Allen, P. B., 1978, “Solids with thermal or static disorder. I. oneelectron properties,” Phys. Rev. B 18, 5217–5224. Allen, P. B., and M. Cardona, 1981, “Theory of the temperature dependence of the direct gap of germanium,” Phys. Rev. B 23, 1495–1505. Allen, P. B., and M. Cardona, 1983, “Temperature dependence of the direct gap of Si and Ge,” Phys. Rev. B 27, 4760–4769. Allen, P. B., and M. L. Cohen, 1969, “Pseudopotential calculation of the mass enhancement and superconducting transition temperature of simple metals,” Phys. Rev. 187, 525–538. Allen, P. B., and M. L. Cohen, 1970, “Calculation of the temperature dependence of the electron-phonon mass enhancement,” Phys. Rev. B 1, 1329–1336. Allen, P. B., M. L. Cohen, L. M. Falicov, and R. V. Kasowski, 1968, “Superconductivity and band structure from a single pseudopotential: Zinc and cadmium,” Phys. Rev. Lett. 21, 1794–1796. Allen, P. B., and R. C. Dynes, 1975, “Transition temperature of strongcoupled superconductors reanalyzed,” Phys. Rev. B 12, 905–922. Allen, P. B., and V. Heine, 1976, “Theory of the temperature dependence of electronic band structures,” J. Phys. C 9, 2305. Allen, P. B., and J. C. K. Hui, 1980, “Thermodynamics of solids: Corrections from electron-phonon interactions,” Z. Phys. B 37, 33–38. Allen, P. B., and M. J. G. Lee, 1972, “Phase-shift pseudopotentials and the electron-phonon interaction: Theory and results for alkali metals,” Phys. Rev. B 5, 3848–3857. Allen, P. B., and B. Mitrovic, 1982, Theory of Superconducting Tc, edited by F. Seitz, D. Turnbull, and H. Ehrenreich, Solid State Physics, Vol. 37 (Academic, New York). Allen, P. B., and J. P. Nery, 2017, “Low temperature semiconductor band-gap thermal shifts: T 4 shifts from ordinary acoustic and T 2 from piezoacoustic coupling,” Phys. Rev. B 95, 035211. Animalu, A. O. E., and V. Heine, 1965, “The screened model potential for 25 elements,” Philos. Mag. 12, 1249–1270. Antončík, E., 1955, “On the theory of temperature shift of the absorption curve in non-polar crystals,” Czech. J. Phys. 5, 449–461. Antonius, G., S. Poncé, P. Boulanger, M. Côté, and X. Gonze, 2014, “Many-body effects on the zero-point renormalization of the band structure,” Phys. Rev. Lett. 112, 215501. Antonius, G., S. Poncé, E. Lantagne-Hurtubise, G. Auclair, X. Gonze, and M. Côté, 2015, “Dynamical and anharmonic effects on the electron-phonon coupling and the zero-point renormalization of the electronic structure,” Phys. Rev. B 92, 085137. Aperis, A., P. Maldonado, and P. M. Oppeneer, 2015, “Ab initio theory of magnetic-field-induced odd-frequency two-band superconductivity in mgb2 ,” Phys. Rev. B 92, 054516. Aryasetiawan, F., and S. Biermann, 2008, “Generalized hedin’s equations for quantum many-body systems with spin-dependent interactions,” Phys. Rev. Lett. 100, 116402. Aryasetiawan, F., and O. Gunnarsson, 1998, “The GW method,” Rep. Prog. Phys. 61, 237. Aryasetiawan, F., L. Hedin, and K. Karlsson, 1996, “Multiple plasmon satellites in Na and Al spectral functions from ab initio cumulant expansion,” Phys. Rev. Lett. 77, 2268–2271. Ashcroft, N. W., and N. D. Mermin, 1976, Solid State Physics (Harcourt, New York). Ashcroft, N. W., and J. W. Wilkins, 1965, “Low temperature electronic specific heat of simple metals,” Phys. Lett. 14, 285–287. 015003-54 Feliciano Giustino: Electron-phonon interactions from first … Audouze, C., F. Jollet, M. Torrent, and X. Gonze, 2006, “Projector augmented-wave approach to density-functional perturbation theory,” Phys. Rev. B 73, 235101. Bachelet, G. B., D. R. Hamann, and M. Schlüter, 1982, “Pseudopotentials that work: From H to Pu,” Phys. Rev. B 26, 4199–4228. Bardeen, J., 1937, “Conductivity of monovalent metals,” Phys. Rev. 52, 688–697. Bardeen, J., and D. Pines, 1955, “Electron-phonon interaction in metals,” Phys. Rev. 99, 1140–1150. Bardeen, J., and W. Shockley, 1950, “Deformation potentials and mobilities in non-polar crystals,” Phys. Rev. 80, 72–80. Baroni, S., S. de Gironcoli, A. Dal Corso, and P. Giannozzi, 2001, “Phonons and related crystal properties from density-functional perturbation theory,” Rev. Mod. Phys. 73, 515–562. Baroni, S., P. Giannozzi, and A. Testa, 1987, “Green’s-function approach to linear response in solids,” Phys. Rev. Lett. 58, 1861–1864. Bassani, G. F., and G. P. Parravicini, 1975, Electronic states and optical transitions in solids (Pergamon, New York). Bauer, R., A. Schmid, P. Pavone, and D. Strauch, 1998, “Electronphonon coupling in the metallic elements Al, Au, Na, and Nb: A first-principles study,” Phys. Rev. B 57, 11276–11282. Baym, G., 1961, “Field-theoretic approach to the properties of the solid state,” Ann. Phys. (N.Y.) 14, 1–42. Becker, M., and H. Y. Fan, 1949, “Optical properties of semiconductors. III. Infra-red transmission of silicon,” Phys. Rev. 76, 1531–1532. Berciu, M., 2006, “Green’s function of a dressed particle,” Phys. Rev. Lett. 97, 036402. Berger, E., P. Valášek, and W. von der Linden, 1995, “Two-dimensional Hubbard-Holstein model,” Phys. Rev. B 52, 4806–4814. Bernardi, M., D. Vigil-Fowler, J. Lischner, J. B. Neaton, and S. G. Louie, 2014, “Ab initio study of hot carriers in the first picosecond after sunlight absorption in silicon,” Phys. Rev. Lett. 112, 257402. Bernardi, M., D. Vigil-Fowler, C. S. Ong, J. B. Neaton, and S. G. Louie, 2015, “Ab initio study of hot electrons in GaAs,” Proc. Natl. Acad. Sci. U.S.A. 112, 5291–5296. Bersier, C., A. Floris, A. Sanna, G. Profeta, A. Continenza, E. K. U. Gross, and S. Massidda, 2009, “Electronic, vibrational, and superconducting properties of CaBeSi: First-principles calculations,” Phys. Rev. B 79, 104503. Bhosale, J., A. K. Ramdas, A. Burger, A. Muñoz, A. H. Romero, M. Cardona, R. Lauck, and R. K. Kremer, 2012, “Temperature dependence of band gaps in semiconductors: Electron-phonon interaction,” Phys. Rev. B 86, 195208. Bianchi, M., E. D. L. Rienks, S. Lizzit, A. Baraldi, R. Balog, L. Hornekær, and Ph. Hofmann, 2010, “Electron-phonon coupling in potassium-doped graphene: Angle-resolved photoemission spectroscopy,” Phys. Rev. B 81, 041403. Bloch, F., 1929, “Über die Quantenmechanik der Elektronen in Kristallgittern,” Z. Phys. 52, 555–600. Blöchl, P. E., 1994, “Projector augmented-wave method,” Phys. Rev. B 50, 17953–17979. Bogoliubov, N. N., 1958, “A new method in the theory of superconductivity. I,” Sov. Phys. JETP 7, 41–46 [http://www.jetp.ac.ru/ cgi‑bin/e/index/e/7/1/p41?a=list]. Bonini, N., M. Lazzeri, N. Marzari, and F. Mauri, 2007, “Phonon anharmonicities in graphite and graphene,” Phys. Rev. Lett. 99, 176802. Born, M., and K. Huang, 1954, Dynamical Theory of Crystal Lattices (Clarendon, Oxford). Born, M., and R. Oppenheimer, 1927, “Zur Quantentheorie der Molekeln,” Ann. Phys. (Berlin) 389, 457–484. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Borysenko, K. M., J. T. Mullen, E. A. Barry, S. Paul, Y. G. Semenov, J. M. Zavada, M. Buongiorno Nardelli, and K. W. Kim, 2010, “First-principles analysis of electron-phonon interactions in graphene,” Phys. Rev. B 81, 121412. Bostwick, A., T. Ohta, T. Seyller, K. Horn, and E. Rotenberg, 2007, “Quasiparticle dynamics in graphene,” Nat. Phys. 3, 36–40. Botti, S., and M. A. L. Marques, 2013, “Strong renormalization of the electronic band gap due to lattice polarization in the GW formalism,” Phys. Rev. Lett. 110, 226404. Broido, D. A., M. Malorny, G. Birner, N. Mingo, and D. A. Stewart, 2007, “Intrinsic lattice thermal conductivity of semiconductors from first principles,” Appl. Phys. Lett. 91, 231922. Brouder, C., G. Panati, M. Calandra, C. Mourougane, and N. Marzari, 2007, “Exponential localization of Wannier functions in insulators,” Phys. Rev. Lett. 98, 046402. Brüesch, P., 1982, Phonons, Theory and Experiments, Vol. 1 (Springer-Verlag, Berlin). Bungaro, C., K. Rapcewicz, and J. Bernholc, 2000, “Ab initio phonon dispersions of wurtzite AlN, GaN, and InN,” Phys. Rev. B 61, 6720–6725. Butler, W. H., F. J. Pinski, and P. B. Allen, 1979, “Phonon linewidths and electron-phonon interaction in Nb,” Phys. Rev. B 19, 3708–3721. Calandra, M., and F. Mauri, 2007, “Electron-phonon coupling and electron self-energy in electron-doped graphene: Calculation of angular-resolved photoemission spectra,” Phys. Rev. B 76, 205411. Calandra, M., G. Profeta, and F. Mauri, 2010, “Adiabatic and nonadiabatic phonon dispersion in a Wannier function approach,” Phys. Rev. B 82, 165111. Campbell, D. K., T. A. DeGrand, and S. Mazumdar, 1984, “Soliton energetics in Peierls-Hubbard models,” Phys. Rev. Lett. 52, 1717–1720. Cancellieri, C., A. S. Mishchenko, U. Aschauer, A. Filippetti, C. Faber, O. S. Barišić, V. A. Rogalev, T. Schmitt, N. Nagaosa, and V. N. Strocov, 2016, “Polaronic metal state at the LaAlO3 =SrTiO3 interface,” Nat. Commun. 7, 10386. Cannuccia, E., and A. Marini, 2011, “Effect of the quantum zeropoint atomic motion on the optical and electronic properties of diamond and trans-polyacetylene,” Phys. Rev. Lett. 107, 255501. Cannuccia, E., and A. Marini, 2012, “Zero point motion effect on the electronic properties of diamond, trans-polyacetylene and polyethylene,” Eur. Phys. J. B 85, 320. Cannuccia, E., and A. Marini, 2013, “Ab initio study of the effects induced by the electron-phonon scattering in carbon based nanostructures,” arXiv:1304.0072. Cao, K., F. Giustino, and P. G. Radaelli, 2015, “Theory of electromagnons in CuO,” Phys. Rev. Lett. 114, 197201. Capaz, R. B., C. D. Spataru, P. Tangney, M. L. Cohen, and S. G. Louie, 2005, “Temperature dependence of the band gap of semiconducting carbon nanotubes,” Phys. Rev. Lett. 94, 036801. Carbotte, J. P., and R. C. Dynes, 1967, “Resistivity of solid aluminum,” Phys. Lett. A 25, 532–533. Cardona, M., 2001, “Renormalization of the optical response of semiconductors by electron-phonon interaction,” Phys. Status Solidi A 188, 1209–1232. Cardona, M., 2005, “Electron-phonon interaction in tetrahedral semiconductors,” Solid State Commun. 133, 3–18. Cardona, M., and M. L. W. Thewalt, 2005, “Isotope effects on the optical spectra of semiconductors,” Rev. Mod. Phys. 77, 1173–1224. Caruso, F., and F. Giustino, 2015, “Spectral fingerprints of electronplasmon coupling,” Phys. Rev. B 92, 045123. Caruso, F., H. Lambert, and F. Giustino, 2015, “Band structures of plasmonic polarons,” Phys. Rev. Lett. 114, 146404. 015003-55 Feliciano Giustino: Electron-phonon interactions from first … Caudal, N., A. M. Saitta, M. Lazzeri, and F. Mauri, 2007, “Kohn anomalies and nonadiabaticity in doped carbon nanotubes,” Phys. Rev. B 75, 115423. Ceperley, D. M., and B. J. Alder, 1980, “Ground state of the electron gas by a stochastic method,” Phys. Rev. Lett. 45, 566–569. Chakraborty, B., and P. B. Allen, 1978, “Theory of temperature dependence of optical properties of solids,” J. Phys. C 11, L9. Chan, K. T., J. D. Sau, P. Zhang, and M. L. Cohen, 2007, “Ab initio calculations of phonon splitting in antiferromagnetic ZnCr2 O4 ,” Phys. Rev. B 75, 054304. Chang, K. J., and M. L. Cohen, 1986, “Electron-phonon interactions and superconductivity in Si, Ge, and Sn,” Phys. Rev. B 34, 4552–4557. Chang, K. J., M. M. Dacorogna, M. L. Cohen, J. M. Mignot, G. Chouteau, and G. Martinez, 1985, “Superconductivity in highpressure metallic phases of Si,” Phys. Rev. Lett. 54, 2375–2378. Chen, C., J. Avila, E. Frantzeskakis, A. Levy, and M. C. Asensio, 2015, “Observation of a two-dimensional liquid of Fröhlich polarons at the bare SrTiO3 surface,” Nat. Commun. 6, 8585. Choi, H. J., M. L. Cohen, and S. G. Louie, 2003, “Anisotropic Eliashberg theory of MgB2: T c , isotope effects, superconducting energy gaps, quasiparticles, and specific heat,” Physica C (Amsterdam) 385, 66–74. Choi, H. J., S. G. Louie, and M. L. Cohen, 2009a, “Anisotropic Eliashberg theory for superconductivity in compressed and doped MgB2 ,” Phys. Rev. B 79, 094518. Choi, H. J., S. G. Louie, and M. L. Cohen, 2009b, “Prediction of superconducting properties of CaB2 using anisotropic Eliashberg theory,” Phys. Rev. B 80, 064503. Choi, H. J., D. Roundy, H. Sun, M. L. Cohen, and S. G. Louie, 2002a, “First-principles calculation of the superconducting transition in MgB2 within the anisotropic Eliashberg formalism,” Phys. Rev. B 66, 020513. Choi, H. J., D. Roundy, H. Sun, M. L. Cohen, and S. G. Louie, 2002b, “The origin of the anomalous superconducting properties of MgB2 ,” Nature (London) 418, 758–760. Cohen, M. H., and V. Heine, 1961, “Cancellation of kinetic and potential energy in atoms, molecules, and solids,” Phys. Rev. 122, 1821–1826. Cohen, M. L., and T. K. Bergstresser, 1966, “Band structures and pseudopotential form factors for fourteen semiconductors of the diamond and zinc-blende structures,” Phys. Rev. 141, 789–796. Cohen-Tannoudji, C., B. Diu, and F. Laloe, 1977, Quantum Mechanics, Vol. 1 (Wiley, New York). Cowley, R. A., 1963, “The lattice dynamics of an anharmonic crystal,” Adv. Phys. 12, 421–480. Cudazzo, P., G. Profeta, A. Sanna, A. Floris, A. Continenza, S. Massidda, and E. K. U. Gross, 2008, “Ab initio description of high-temperature superconductivity in dense molecular hydrogen,” Phys. Rev. Lett. 100, 257001. Cudazzo, P., G. Profeta, A. Sanna, A. Floris, A. Continenza, S. Massidda, and E. K. U. Gross, 2010, “Electron-phonon interaction and superconductivity in metallic molecular hydrogen. II. superconductivity under pressure,” Phys. Rev. B 81, 134506. Dacorogna, M. M., K. J. Chang, and M. L. Cohen, 1985, “Pressure increase of the electron-phonon interaction in superconducting hexagonal silicon,” Phys. Rev. B 32, 1853–1855. Dacorogna, M. M., M. L. Cohen, and P. K. Lam, 1985, “Selfconsistent calculation of the q dependence of the electron-phonon coupling in aluminum,” Phys. Rev. Lett. 55, 837–840. Dal Corso, A., 2007, “Density functional perturbation theory for lattice dynamics with fully relativistic ultrasoft pseudopotentials: Application to fcc-Pt and fcc-Au,” Phys. Rev. B 76, 054308. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Dal Corso, A., 2008, “Ab initio phonon dispersions of face centered cubic Pb: effects of spin-orbit coupling,” J. Phys. Condens. Matter 20, 445202. Dal Corso, A., 2013, “Ab initio phonon dispersions of transition and noble metals: effects of the exchange and correlation functional,” J. Phys. Condens. Matter 25, 145401. Dal Corso, A., S. Baroni, R. Resta, and S. de Gironcoli, 1993, “Ab initio calculation of phonon dispersions in II-VI semiconductors,” Phys. Rev. B 47, 3588–3592. Dal Corso, A., and S. de Gironcoli, 2000, “Ab initio phonon dispersions of Fe and Ni,” Phys. Rev. B 62, 273–277. Dal Corso, A., A. Pasquarello, and A. Baldereschi, 1997, “Densityfunctional perturbation theory for lattice dynamics with ultrasoft pseudopotentials,” Phys. Rev. B 56, R11369–R11372. Damascelli, A., Z. Hussain, and Z.-X. Shen, 2003, “Angle-resolved photoemission studies of the cuprate superconductors,” Rev. Mod. Phys. 75, 473–541. Debernardi, A., S. Baroni, and E. Molinari, 1995, “Anharmonic phonon lifetimes in semiconductors from density-functional perturbation theory,” Phys. Rev. Lett. 75, 1819–1822. de Gironcoli, S., 1995, “Lattice dynamics of metals from densityfunctional perturbation theory,” Phys. Rev. B 51, 6773–6776. Deinzer, G., G. Birner, and D. Strauch, 2003, “Ab initio calculation of the linewidth of various phonon modes in germanium and silicon,” Phys. Rev. B 67, 144304. Della Sala, F., R. Rousseau, A. Görling, and D. Marx, 2004, “Quantum and thermal fluctuation effects on the photoabsorption spectra of clusters,” Phys. Rev. Lett. 92, 183401. Díaz-Sánchez, L. E., A. H. Romero, and X. Gonze, 2007, “Phonon band structure and interatomic force constants for bismuth: Crucial role of spin-orbit interaction,” Phys. Rev. B 76, 104302. D’Innocenzo, V., G. Grancini, M. J. P. Alcocer, A. R. S. Kandada, S. D. Stranks, M. M. Lee, G. Lanzani, H. J. Snaith, and A. Petrozza, 2014, “Excitons versus free charges in organo-lead tri-halide perovskites,” Nat. Commun. 5, 3586. Dumke, W. P., 1956, “Deformation potential theory for n-type Ge,” Phys. Rev. 101, 531–536. Dynes, R. C., and J. P. Carbotte, 1968, “Phonon-limited resistivity of some simple metals,” Phys. Rev. 175, 913–919. Eiguren, A., and C. Ambrosch-Draxl, 2008a, “Complex quasiparticle band structure induced by electron-phonon interaction: Band splitting in the 1 × 1H=Wð110Þ surface,” Phys. Rev. Lett. 101, 036402. Eiguren, A., and C. Ambrosch-Draxl, 2008b, “Wannier interpolation scheme for phonon-induced potentials: Application to bulk MgB2 , W, and the 1 × 1 H-covered W(110) surface,” Phys. Rev. B 78, 045124. Eiguren, A., C. Ambrosch-Draxl, and P. M. Echenique, 2009, “Selfconsistently renormalized quasiparticles under the electron-phonon interaction,” Phys. Rev. B 79, 245103. Eiguren, A., S. de Gironcoli, E. V. Chulkov, P. M. Echenique, and E. Tosatti, 2003, “Electron-phonon interaction at the Be(0001) surface,” Phys. Rev. Lett. 91, 166803. Eiguren, A., and I. G. Gurtubay, 2014, “Helmholtz Fermi surface harmonics: an efficient approach for treating anisotropic problems involving Fermi surface integrals,” New J. Phys. 16, 063014. Eiguren, A., B. Hellsing, E. V. Chulkov, and P. M. Echenique, 2003, “Phonon-mediated decay of metal surface states,” Phys. Rev. B 67, 235423. Eiguren, A., B. Hellsing, F. Reinert, G. Nicolay, E. V. Chulkov, V. M. Silkin, S. Hüfner, and P. M. Echenique, 2002, “Role of bulk and surface phonons in the decay of metal surface states,” Phys. Rev. Lett. 88, 066805. 015003-56 Feliciano Giustino: Electron-phonon interactions from first … Eliashberg, G. M., 1960, “Interactions between electrons and lattice vibrations in a superconductor,” Sov. Phys. JETP 11, 696–702 [http://www.jetp.ac.ru/cgi‑bin/e/index/e/11/3/p696?a=list]. Eliashberg, G. M., 1963, “The low temperature specific heat of metals,” Sov. Phys. JETP 16, 780–781. Emin, D., 2013, Polarons (Cambridge University Press, Cambridge, England). Engel, E. A., B. Monserrat, and R. J. Needs, 2015, “Vibrational renormalisation of the electronic band gap in hexagonal and cubic ice,” J. Chem. Phys. 143, 244708. Engelsberg, S., and J. R. Schrieffer, 1963, “Coupled electron-phonon system,” Phys. Rev. 131, 993–1008. Errea, I., M. Calandra, and F. Mauri, 2014, “Anharmonic free energies and phonon dispersions from the stochastic self-consistent harmonic approximation: Application to platinum and palladium hydrides,” Phys. Rev. B 89, 064302. Errea, I., B. Rousseau, and A. Bergara, 2011, “Anharmonic stabilization of the high-pressure simple cubic phase of calcium,” Phys. Rev. Lett. 106, 165501. Faber, C., P. Boulanger, C. Attaccalite, E. Cannuccia, I. Duchemin, T. Deutsch, and X. Blase, 2015, “Exploring approximations to the GW self-energy ionic gradients,” Phys. Rev. B 91, 155109. Faber, C., J. Laflamme Janssen, M. Côté, E. Runge, and X. Blase, 2011, “Electron-phonon coupling in the C60 fullerene within the many-body GW approach,” Phys. Rev. B 84, 155104. Fan, H. Y., 1951, “Temperature dependence of the energy gap in semiconductors,” Phys. Rev. 82, 900–905. Fetter, A. L., and J. D. Walecka, 2003, Quantum theory of manyparticle systems (Dover Publications, New York). Fiorentini, M., and N. Bonini, 2016, “Thermoelectric coefficients of n-doped silicon from first principles via the solution of the Boltzmann transport equation,” Phys. Rev. B 94, 085204. Flores-Livas, J. A., and A. Sanna, 2015, “Superconductivity in intercalated group-IV honeycomb structures,” Phys. Rev. B 91, 054508. Floris, A., S. de Gironcoli, E. K. U. Gross, and M. Cococcioni, 2011, “Vibrational properties of MnO and NiO from DFTþ U-based density functional perturbation theory,” Phys. Rev. B 84, 161102. Floris, A., G. Profeta, N. N. Lathiotakis, M. Lüders, M. A. L. Marques, C. Franchini, E. K. U. Gross, A. Continenza, and S. Massidda, 2005, “Superconducting properties of MgB2 from first principles,” Phys. Rev. Lett. 94, 037004. Floris, A., A. Sanna, S. Massidda, and E. K. U. Gross, 2007, “Two-band superconductivity in Pb from ab initio calculations,” Phys. Rev. B 75, 054508. Franceschetti, A., 2007, “First-principles calculations of the temperature dependence of the band gap of Si nanocrystals,” Phys. Rev. B 76, 161301. Frenkel, J., 1932, Wave Mechanics: Elementary Theory (Oxford University Press, New York). Friedrich, M., A. Riefer, S. Sanna, W. G. Schmidt, and A. Schindlmayr, 2015, “Phonon dispersion and zero-point renormalization of LiNbO3 from density-functional perturbation theory,” J. Phys. Condens. Matter 27, 385402. Fröhlich, H., 1937, “Theory of electrical breakdown in ionic crystals,” Proc. R. Soc. A 160, 230–241. Fröhlich, H., 1954, “Electrons in lattice fields,” Adv. Phys. 3, 325–361. Fröhlich, H., and N. F. Mott, 1939, “The mean free path of electrons in polar crystals,” Proc. R. Soc. A 171, 496–504. Fröhlich, H., H. Pelzer, and S. Zienau, 1950, “Properties of slow electrons in polar materials,” Philos. Mag. Ser. 7 41, 221–242. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Giannozzi, P., S. de Gironcoli, P. Pavone, and S. Baroni, 1991, “Ab initio calculation of phonon dispersions in semiconductors,” Phys. Rev. B 43, 7231–7242. Giannozzi, P., et al., 2009, “QUANTUM ESPRESSO: a modular and open-source software project for quantum simulations of materials,” J. Phys. Condens. Matter 21, 395502. Gillis, N. S., 1970, “Self-consistent phonons and the coupled electron-phonon system,” Phys. Rev. B 1, 1872–1876. Giuliani, G., and G. Vignale, 2005, Quantum Theory of the Electron Liquid (Cambridge University Press, Cambridge, England). Giustino, F., 2014, Materials Modelling using Density Functional Theory (Oxford University Press, New York). Giustino, F., M. L. Cohen, and S. G. Louie, 2007, “Electron-phonon interaction using Wannier functions,” Phys. Rev. B 76, 165108. Giustino, F., M. L. Cohen, and S. G. Louie, 2008, “Small phonon contribution to the photoemission kink in the copper oxide superconductors,” Nature (London) 452, 975–978. Giustino, F., S. G. Louie, and M. L. Cohen, 2010, “Electron-phonon renormalization of the direct band gap of diamond,” Phys. Rev. Lett. 105, 265501. Giustino, F., J. R. Yates, I. Souza, M. L. Cohen, and S. G. Louie, 2007, “Electron-phonon interaction via electronic and lattice wannier functions: Superconductivity in boron-doped diamond reexamined,” Phys. Rev. Lett. 98, 047005. Göbel, A., T. Ruf, M. Cardona, C. T. Lin, J. Wrzesinski, M. Steube, K. Reimann, J.-C. Merle, and M. Joucla, 1998, “Effects of the isotopic composition on the fundamental gap of CuCl,” Phys. Rev. B 57, 15183–15190. Gonze, X., 1995a, “Perturbation expansion of variational principles at arbitrary order,” Phys. Rev. A 52, 1086–1095. Gonze, X., 1995b, “Adiabatic density-functional perturbation theory,” Phys. Rev. A 52, 1096–1114. Gonze, X., 1997, “First-principles responses of solids to atomic displacements and homogeneous electric fields: Implementation of a conjugate-gradient algorithm,” Phys. Rev. B 55, 10337–10354. Gonze, X., D. C. Allan, and M. P. Teter, 1992, “Dielectric tensor, effective charges, and phonons in α-quartz by variational densityfunctional perturbation theory,” Phys. Rev. Lett. 68, 3603–3606. Gonze, X., P. Boulanger, and M. Côté, 2011, “Theoretical approaches to the temperature and zero-point motion effects on the electronic band structure,” Ann. Phys. (Berlin) 523, 168–178. Gonze, X., and C. Lee, 1997, “Dynamical matrices, Born effective charges, dielectric permittivity tensors, and interatomic force constants from density-functional perturbation theory,” Phys. Rev. B 55, 10355–10368. Gonze, X., et al., 2009, “ABINIT: First-principles approach to material and nanosystem properties,” Comput. Phys. Commun. 180, 2582–2615. Gopalan, S., P. Lautenschlager, and M. Cardona, 1987, “Temperature dependence of the shifts and broadenings of the critical points in GaAs,” Phys. Rev. B 35, 5577–5584. Gor’kov, L. P., 1958, “On the energy spectrum of superconductors,” Sov. Phys. JETP 7, 505–508 [http://www.jetp.ac.ru/cgi‑bin/e/ index/e/7/3/p505?a=list]. Grimvall, G., 1969, “New aspects on the electron-phonon system at finite temperatures with an application on lead and mercury,” Phys. Kondens. Mater. 9, 283–299. Grimvall, G., 1975, “Electron-electron renormalization of the electronic heat capacity in simple metals,” Phys. Scr. 12, 337. Grimvall, G., 1981, The electron-phonon interaction in metals (North-Holland, Amsterdam). Grüneis, A., C. Attaccalite, A. Rubio, D. V. Vyalikh, S. L. Molodtsov, J. Fink, R. Follath, W. Eberhardt, B. Büchner, and T. Pichler, 2009a, 015003-57 Feliciano Giustino: Electron-phonon interactions from first … “Electronic structure and electron-phonon coupling of doped graphene layers in KC8 ,” Phys. Rev. B 79, 205106. Grüneis, A., et al., 2009b, “Phonon surface mapping of graphite: Disentangling quasi-degenerate phonon dispersions,” Phys. Rev. B 80, 085423. Gumhalter, B., V. Kovač, F. Caruso, H. Lambert, and F. Giustino, 2016, “On the combined use of GW approximation and cumulant expansion in the calculations of quasiparticle spectra: The paradigm of Si valence bands,” Phys. Rev. B 94, 035103. Gunnarsson, O., B. I. Lundqvist, and J. W. Wilkins, 1974, “Contribution to the cohesive energy of simple metals: Spin-dependent effect,” Phys. Rev. B 10, 1319–1327. Gunst, T., T. Markussen, K. Stokbro, and M. Brandbyge, 2016, “First-principles method for electron-phonon coupling and electron mobility: Applications to two-dimensional materials,” Phys. Rev. B 93, 035414. Guzzo, M., J. J. Kas, F. Sottile, M. G. Silly, F. Sirotti, J. J. Rehr, and L. Reining, 2012, “Plasmon satellites in valence-band photoemission spectroscopy,” Eur. Phys. J. B 85, 324. Guzzo, M., J. J. Kas, L. Sponza, C. Giorgetti, F. Sottile, D. Pierucci, M. G. Silly, F. Sirotti, J. J. Rehr, and L. Reining, 2014, “Multiple satellites in materials with complex plasmon spectra: From graphite to graphene,” Phys. Rev. B 89, 085425. Guzzo, M., G. Lani, F. Sottile, P. Romaniello, M. Gatti, J. J. Kas, J. J. Rehr, M. G. Silly, F. Sirotti, and L. Reining, 2011, “Valence electron photoemission spectrum of semiconductors: Ab initio description of multiple satellites,” Phys. Rev. Lett. 107, 166401. Hall, L. H., J. Bardeen, and F. J. Blatt, 1954, “Infrared absorption spectrum of germanium,” Phys. Rev. 95, 559–560. Hamann, D. R., M. Schlüter, and C. Chiang, 1979, “Norm-conserving pseudopotentials,” Phys. Rev. Lett. 43, 1494–1497. Han, P., and G. Bester, 2013, “Large nuclear zero-point motion effect in semiconductor nanoclusters,” Phys. Rev. B 88, 165311. Hannewald, K., and P. A. Bobbert, 2004a, “Ab initio theory of charge-carrier conduction in ultrapure organic crystals,” Appl. Phys. Lett. 85, 1535–1537. Hannewald, K., and P. A. Bobbert, 2004b, “Anisotropy effects in phonon-assisted charge-carrier transport in organic molecular crystals,” Phys. Rev. B 69, 075212. Hayman, B., and J. P. Carbotte, 1971, “Resistivity and electronphonon interaction in Li,” J. Phys. F 1, 828. He, L., F. Liu, G. Hautier, M. J. T. Oliveira, M. A. L. Marques, F. D. Vila, J. J. Rehr, G.-M. Rignanese, and A. Zhou, 2014, “Accuracy of generalized gradient approximation functionals for densityfunctional perturbation theory calculations,” Phys. Rev. B 89, 064305. He, L., and D. Vanderbilt, 2001, “Exponential decay properties of Wannier functions and related quantities,” Phys. Rev. Lett. 86, 5341–5344. Hedin, L., 1965, “New method for calculating the one-particle Green’s function with application to the electron-gas problem,” Phys. Rev. 139, A796–A823. Hedin, L., and B. I. Lundqvist, 1971, “Explicit local exchangecorrelation potentials,” J. Phys. C 4, 2064. Hedin, L., and S. Lundqvist, 1969, Effects of electron-electron and electron-phonon interactions on the one-electron states of solids, edited by F. Seitz, D. Turnbull, and H. Ehrenreich, Solid State Physics, Vol. 23 (Academic, New York). Heid, R., K.-P. Bohnen, I. Yu. Sklyadneva, and E. V. Chulkov, 2010, “Effect of spin-orbit coupling on the electron-phonon interaction of the superconductors Pb and Tl,” Phys. Rev. B 81, 174527. Heid, R., K.-P. Bohnen, R. Zeyher, and D. Manske, 2008, “Momentum dependence of the electron-phonon coupling and Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 self-energy effects in superconducting YBa2 Cu3 O7 within the local density approximation,” Phys. Rev. Lett. 100, 137001. Heine, V., and I. Abarenkov, 1964, “A new method for the electronic structure of metals,” Philos. Mag. 9, 451–465. Hellman, O., I. A. Abrikosov, and S. I. Simak, 2011, “Lattice dynamics of anharmonic solids from first principles,” Phys. Rev. B 84, 180301. Hellman, O., P. Steneteg, I. A. Abrikosov, and S. I. Simak, 2013, “Temperature dependent effective potential method for accurate free energy calculations of solids,” Phys. Rev. B 87, 104111. Hengsberger, M., D. Purdie, P. Segovia, M. Garnier, and Y. Baer, 1999, “Photoemission study of a strongly coupled electron-phonon system,” Phys. Rev. Lett. 83, 592–595. Herring, C., 1940, “A new method for calculating wave functions in crystals,” Phys. Rev. 57, 1169–1177. Heyd, J., G. E. Scuseria, and M. Ernzerhof, 2003, “Hybrid functionals based on a screened Coulomb potential,” J. Chem. Phys. 118, 8207. Himmetoglu, B., and A. Janotti, 2016, “Transport properties of KTaO3 from first principles,” J. Phys. Condens. Matter 28, 065502. Himmetoglu, B., A. Janotti, H. Peelaers, A. Alkauskas, and C. G. Van de Walle, 2014, “First-principles study of the mobility of SrTiO3 ,” Phys. Rev. B 90, 241204. Hoddeson, L. H., and G. Baym, 1980, “The development of the quantum mechanical electron theory of metals: 1900-28,” Proc. R. Soc. A 371, 8–23. Hohenberg, P., and W. Kohn, 1964, “Inhomogeneous electron gas,” Phys. Rev. 136, B864–B871. Holstein, T., 1959, “Studies of polaron motion: Part I. The molecularcrystal model,” Ann. Phys. (N.Y.) 8, 325–342. Hone, D., 1960, “Exchange and correlation corrections to the electron-phonon interaction,” Phys. Rev. 120, 1600–1606. Hong, J., A. Stroppa, J. Íñiguez, S. Picozzi, and D. Vanderbilt, 2012, “Spin-phonon coupling effects in transition-metal perovskites: A DFT þ U and hybrid-functional study,” Phys. Rev. B 85, 054417. Hooton, D. J., 1955, “LI. a new treatment of anharmonicity in lattice thermodynamics: I,” Philos. Mag. 46, 422–432. Hybertsen, M. S., and S. G. Louie, 1986, “Electron correlation in semiconductors and insulators: Band gaps and quasiparticle energies,” Phys. Rev. B 34, 5390–5413. Ichinokura, S., K. Sugawara, A. Takayama, T. Takahashi, and S. Hasegawa, 2016, “Superconducting calcium-intercalated bilayer graphene,” ACS Nano 10, 2761–2765. Johnson, P. D., et al., 2001, “Doping and temperature dependence of the mass enhancement observed in the cuprate Bi2 Sr2 CaCu2 O8þδ ,” Phys. Rev. Lett. 87, 177007. Kaasbjerg, K., K. S. Thygesen, and K. W. Jacobsen, 2012, “Phononlimited mobility in n-type single-layer MoS2 from first principles,” Phys. Rev. B 85, 115317. Kadanoff, L. P., and G. Baym, 1962, Quantum statistical mechanics: Green’s function methods in equilibrium and nonequilibrium problems, Frontiers in Physics (Benjamin, New York). Karki, B. B., R. M. Wentzcovitch, S. de Gironcoli, and S. Baroni, 2000, “Ab initio lattice dynamics of MgSiO3 perovskite at high pressure,” Phys. Rev. B 62, 14750–14756. Kas, J. J., J. J. Rehr, and L. Reining, 2014, “Cumulant expansion of the retarded one-electron Green function,” Phys. Rev. B 90, 085112. Kato, T., T. Kobayashi, and M. Namiki, 1960, “Formal theory of Green functions,” Prog. Theor. Phys. 15, 3–60. Kaveh, M., and N. Wiser, 1972, “Temperature and volume dependence of the electrical resistivity of sodium and potassium,” Phys. Rev. B 6, 3648–3658. Kawai, H., K. Yamashita, E. Cannuccia, and A. Marini, 2014, “Electron-electron and electron-phonon correlation effects on the 015003-58 Feliciano Giustino: Electron-phonon interactions from first … finite-temperature electronic and optical properties of zinc-blende GaN,” Phys. Rev. B 89, 085202. Keating, P. N., 1968, “Dielectric screening and the phonon spectra of metallic and nonmetallic crystals,” Phys. Rev. 175, 1171–1180. Kheifets, A. S., V. A. Sashin, M. Vos, E. Weigold, and F. Aryasetiawan, 2003, “Spectral properties of quasiparticles in silicon: A test of many-body theory,” Phys. Rev. B 68, 233205. Kim, T. Y., C.-H. Park, and N. Marzari, 2016, “The electronic thermal conductivity of graphene,” Nano Lett. 16, 2439–2443. King-Smith, R. D., R. J. Needs, V. Heine, and M. J. Hodgson, 1989, “A first-principle calculation of the temperature dependence of the indirect band gap of silicon,” Europhys. Lett. 10, 569. King-Smith, R. D., and D. Vanderbilt, 1993, “Theory of polarization of crystalline solids,” Phys. Rev. B 47, 1651–1654. Kioupakis, E., P. Rinke, A. Schleife, F. Bechstedt, and C. G. Van de Walle, 2010, “Free-carrier absorption in nitrides from first principles,” Phys. Rev. B 81, 241201. Kioupakis, E., D. Steiauf, P. Rinke, K. T. Delaney, and C. G. Van de Walle, 2015, “First-principles calculations of indirect auger recombination in nitride semiconductors,” Phys. Rev. B 92, 035207. Kittel, C., 1963, Quantum Theory of Solids (Wiley, New York). Kittel, C., 1976, Introduction to Solid State Physics (Wiley, New York), 5th ed. Koehler, T. R., 1966, “Theory of the self-consistent harmonic approximation with application to solid neon,” Phys. Rev. Lett. 17, 89–91. Kohn, W., 1959a, “Analytic properties of Bloch waves and Wannier functions,” Phys. Rev. 115, 809–821. Kohn, W., 1959b, “Image of the fermi surface in the vibration spectrum of a metal,” Phys. Rev. Lett. 2, 393–394. Kohn, W., and L. J. Sham, 1965, “Self-consistent equations including exchange and correlation effects,” Phys. Rev. 140, A1133–A1138. Komelj, M., and H. Krakauer, 2015, “Electron-phonon coupling and exchange-correlation effects in superconducting H3 S under high pressure,” Phys. Rev. B 92, 205125. Kreibich, T., and E. K. U. Gross, 2001, “Multicomponent densityfunctional theory for electrons and nuclei,” Phys. Rev. Lett. 86, 2984–2987. Kreibich, T., R. van Leeuwen, and E. K. U. Gross, 2008, “Multicomponent density-functional theory for electrons and nuclei,” Phys. Rev. A 78, 022501. Kresse, G., J. Furthmüller, and J. Hafner, 1995, “Ab initio force constant approach to phonon dispersion relations of diamond and graphite,” Europhys. Lett. 32, 729. Laflamme Janssen, J., M. Côté, S. G. Louie, and M. L. Cohen, 2010, “Electron-phonon coupling in C60 using hybrid functionals,” Phys. Rev. B 81, 073106. Lam, P. K., M. M. Dacorogna, and M. L. Cohen, 1986, “Selfconsistent calculation of electron-phonon couplings,” Phys. Rev. B 34, 5065–5069. Langreth, D. C., 1970, “Singularities in the X-ray spectra of metals,” Phys. Rev. B 1, 471–477. Lanzara, A., et al., 2001, “Evidence for ubiquitous strong electronphonon coupling in high-temperature superconductors,” Nature (London) 412, 510–514. LaShell, S., E. Jensen, and T. Balasubramanian, 2000, “Nonquasiparticle structure in the photoemission spectra from the Be(0001) surface and determination of the electron self energy,” Phys. Rev. B 61, 2371–2374. Lautenschlager, P., P. B. Allen, and M. Cardona, 1985, “Temperature dependence of band gaps in Si and Ge,” Phys. Rev. B 31, 2163–2171. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Lautenschlager, P., P. B. Allen, and M. Cardona, 1986, “Phononinduced lifetime broadenings of electronic states and critical points in Si and Ge,” Phys. Rev. B 33, 5501–5511. Lautenschlager, P., M. Garriga, S. Logothetidis, and M. Cardona, 1987, “Interband critical points of GaAs and their temperature dependence,” Phys. Rev. B 35, 9174–9189. Lautenschlager, P., M. Garriga, L. Vina, and M. Cardona, 1987, “Temperature dependence of the dielectric function and interband critical points in silicon,” Phys. Rev. B 36, 4821–4830. Lax, M., 1952, “The Franck-Condon principle and its application to crystals,” J. Chem. Phys. 20, 1752–1760. Łażewski, J., P. Piekarz, J. Toboła, B. Wiendlocha, P. T. Jochym, M. Sternik, and K. Parlinski, 2010, “Phonon mechanism of the magnetostructural phase transition in MnAs,” Phys. Rev. Lett. 104, 147205. Lazzeri, M., C. Attaccalite, L. Wirtz, and F. Mauri, 2008, “Impact of the electron-electron correlation on phonon dispersion: Failure of LDA and GGA DFT functionals in graphene and graphite,” Phys. Rev. B 78, 081406. Lazzeri, M., M. Calandra, and F. Mauri, 2003, “Anharmonic phonon frequency shift in MgB2 ,” Phys. Rev. B 68, 220509. Lazzeri, M., and F. Mauri, 2006, “Nonadiabatic Kohn anomaly in a doped graphene monolayer,” Phys. Rev. Lett. 97, 266407. Lazzeri, M., S. Piscanec, F. Mauri, A. C. Ferrari, and J. Robertson, 2006, “Phonon linewidths and electron-phonon coupling in graphite and nanotubes,” Phys. Rev. B 73, 155426. Lee, C., P. Ghosez, and X. Gonze, 1994, “Lattice dynamics and dielectric properties of incipient ferroelectric TiO2 rutile,” Phys. Rev. B 50, 13379–13387. Lee, J. H., and K. M. Rabe, 2011, “Large spin-phonon coupling and magnetically induced phonon anisotropy in SrMO3 perovskites (M ¼ V, Cr, Mn, Fe, Co),” Phys. Rev. B 84, 104440. Lee, K.-H., and K. J. Chang, 1996, “Linear-response calculation of the Coulomb pseudopotential μ for Nb,” Phys. Rev. B 54, 1419–1422. Lee, K.-H., K. J. Chang, and M. L. Cohen, 1995, “First-principles calculations of the Coulomb pseudopotential μ : Application to Al,” Phys. Rev. B 52, 1425–1428. Lee, T. D., F. E. Low, and D. Pines, 1953, “The motion of slow electrons in a polar crystal,” Phys. Rev. 90, 297–302. Leonardo, A., I. Yu. Sklyadneva, V. M. Silkin, P. M. Echenique, and E. V. Chulkov, 2007, “Ab initio calculation of the phonon-induced contribution to the electron-state linewidth on the Mg(0001) surface versus bulk Mg,” Phys. Rev. B 76, 035404. Li, W., 2015, “Electrical transport limited by electron-phonon coupling from boltzmann transport equation: An ab initio study of Si, Al, and MoS2 ,” Phys. Rev. B 92, 075405. Li, X., J. T. Mullen, Z. Jin, K. M. Borysenko, M. Buongiorno Nardelli, and K. W. Kim, 2013, “Intrinsic electrical transport properties of monolayer silicene and MoS2 from first principles,” Phys. Rev. B 87, 115418. Liao, B., B. Qiu, J. Zhou, S. Huberman, K. Esfarjani, and G. Chen, 2015, “Significant reduction of lattice thermal conductivity by the electron-phonon interaction in silicon with high carrier concentrations: A first-principles study,” Phys. Rev. Lett. 114, 115901. Linscheid, A., A. Sanna, F. Essenberger, and E. K. U. Gross, 2015, “Ab initio theory of superconductivity in a magnetic field. I. spin density functional theory for superconductors and eliashberg equations,” Phys. Rev. B 92, 024505. Linscheid, A., A. Sanna, A. Floris, and E. K. U. Gross, 2015, “Firstprinciples calculation of the real-space order parameter and 015003-59 Feliciano Giustino: Electron-phonon interactions from first … condensation energy density in phonon-mediated superconductors,” Phys. Rev. Lett. 115, 097002. Linscheid, A., A. Sanna, and E. K. U. Gross, 2015, “Ab initio theory of superconductivity in a magnetic field. II. numerical solution,” Phys. Rev. B 92, 024506. Lischner, J., D. Vigil-Fowler, and S. G. Louie, 2013, “Physical origin of satellites in photoemission of doped graphene: An ab initio GW plus cumulant study,” Phys. Rev. Lett. 110, 146801. Liu, A. Y., and A. A. Quong, 1996, “Linear-response calculation of electron-phonon coupling parameters,” Phys. Rev. B 53, R7575–R7579. Lloyd-Williams, J. H., and B. Monserrat, 2015, “Lattice dynamics and electron-phonon coupling calculations using nondiagonal supercells,” Phys. Rev. B 92, 184301. Lüders, M., M. A. L. Marques, N. N. Lathiotakis, A. Floris, G. Profeta, L. Fast, A. Continenza, S. Massidda, and E. K. U. Gross, 2005, “Ab initio theory of superconductivity. I. Density functional formalism and approximate functionals,” Phys. Rev. B 72, 024545. Luttinger, J. M., 1960, “Fermi surface and some simple equilibrium properties of a system of interacting fermions,” Phys. Rev. 119, 1153–1163. Luttinger, J. M., and J. C. Ward, 1960, “Ground-state energy of a many-fermion system. II,” Phys. Rev. 118, 1417–1427. Mahan, G. D., 1993, Many-Particle Physics (Plenum, New York), 2nd ed. Maksimov, E. G., 1976, “A self-consistent description of the electron-phonon system in metals and the problem of lattice stability,” Sov. Phys. JETP 42, 1138–1143 [http://www.jetp.ac.ru/cgi‑bin/e/ index/e/42/6/p1138?a=list]. Maksimov, E. G., and S. V. Shulga, 1996, “Nonadiabatic effects in optical phonon self-energy,” Solid State Commun. 97, 553–560. Mandal, S., R. E. Cohen, and K. Haule, 2014, “Strong pressuredependent electron-phonon coupling in FeSe,” Phys. Rev. B 89, 220502. Maradudin, A. A., and S. H. Vosko, 1968, “Symmetry properties of the normal vibrations of a crystal,” Rev. Mod. Phys. 40, 1–37. Margine, E. R., and F. Giustino, 2013, “Anisotropic MigdalEliashberg theory using Wannier functions,” Phys. Rev. B 87, 024505. Margine, E. R., and F. Giustino, 2014, “Two-gap superconductivity in heavily n-doped graphene: Ab initio Migdal-Eliashberg theory,” Phys. Rev. B 90, 014518. Margine, E. R., H. Lambert, and F. Giustino, 2016, “Electronphonon interaction and pairing mechanism in superconducting Ca-intercalated bilayer graphene,” Sci. Rep. 6, 21414. Marini, A., 2008, “Ab initio finite-temperature excitons,” Phys. Rev. Lett. 101, 106405. Marini, A., S. Poncé, and X. Gonze, 2015, “Many-body perturbation theory approach to the electron-phonon interaction with density-functional theory as a starting point,” Phys. Rev. B 91, 224310. Marques, M. A. L., M. Lüders, N. N. Lathiotakis, G. Profeta, A. Floris, L. Fast, A. Continenza, E. K. U. Gross, and S. Massidda, 2005, “Ab initio theory of superconductivity. II. Application to elemental metals,” Phys. Rev. B 72, 024546. Marsiglio, F., M. Schossmann, and J. P. Carbotte, 1988, “Iterative analytic continuation of the electron self-energy to the real axis,” Phys. Rev. B 37, 4965–4969. Martin, R. M., 2004, Electronic structure: Basic theory and practical methods (Cambridge University Press, Cambridge, England). Marzari, N., A. A. Mostofi, J. R. Yates, I. Souza, and D. Vanderbilt, 2012, “Maximally localized Wannier functions: Theory and applications,” Rev. Mod. Phys. 84, 1419–1475. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Marzari, N., and D. Vanderbilt, 1997, “Maximally localized generalized Wannier functions for composite energy bands,” Phys. Rev. B 56, 12847–12865. Mauri, F., O. Zakharov, S. de Gironcoli, S. G. Louie, and M. L. Cohen, 1996, “Phonon softening and superconductivity in tellurium under pressure,” Phys. Rev. Lett. 77, 1151–1154. McMillan, W. L., 1968, “Transition temperature of strong-coupled superconductors,” Phys. Rev. 167, 331–344. Mermin, N. D., 1966, “A short simple evaluation of expressions of the Debye-Waller form,” J. Math. Phys. (N.Y.) 7, 1038–1038. Merzbacher, E., 1998, Quantum Mechanics (Wiley, New York), 3rd ed. Migdal, A. B., 1958, “Interaction between electrons and lattice vibrations in a normal metal,” Sov. Phys. JETP 7, 996–1001 [http://www.jetp.ac.ru/cgi‑bin/e/index/e/7/6/p996?a=list]. Monserrat, B., 2016a, “Correlation effects on electron-phonon coupling in semiconductors: Many-body theory along thermal lines,” Phys. Rev. B 93, 100301. Monserrat, B., 2016b, “Vibrational averages along thermal lines,” Phys. Rev. B 93, 014302. Monserrat, B., N. D. Drummond, and R. J. Needs, 2013, “Anharmonic vibrational properties in periodic systems: energy, electronphonon coupling, and stress,” Phys. Rev. B 87, 144302. Monserrat, B., N. D. Drummond, C. J. Pickard, and R. J. Needs, 2014, “Electron-phonon coupling and the metallization of solid helium at terapascal pressures,” Phys. Rev. Lett. 112, 055504. Monserrat, B., E. A. Engel, and R. J. Needs, 2015, “Giant electronphonon interactions in molecular crystals and the importance of nonquadratic coupling,” Phys. Rev. B 92, 140302. Monserrat, B., and R. J. Needs, 2014, “Comparing electron-phonon coupling strength in diamond, silicon, and silicon carbide: Firstprinciples study,” Phys. Rev. B 89, 214304. Mooradian, A., and G. B. Wright, 1966, “Observation of the interaction of plasmons with longitudinal optical phonons in GaAs,” Phys. Rev. Lett. 16, 999–1001. Morel, P., and P. W. Anderson, 1962, “Calculation of the superconducting state parameters with retarded electron-phonon interaction,” Phys. Rev. 125, 1263–1271. Moser, S., et al., 2013, “Tunable polaronic conduction in anatase TiO2 ,” Phys. Rev. Lett. 110, 196403. Mostofi, A. A., J. R. Yates, Y.-S. Lee, I. Souza, D. Vanderbilt, and N. Marzari, 2008, “Wannier90: A tool for obtaining maximallylocalised Wannier functions,” Comput. Phys. Commun. 178, 685–699. Mott, N. F., and H. Jones, 1936, The Theory of the Properties of Metals and Alloys (Oxford University Press, New York). Nagamatsu, J., N. Nakagawa, T. Muranaka, Y. Zenitani, and J. Akimitsu, 2001, “Superconductivity at 39 K in magnesium diboride,” Nature (London) 410, 63–64. Nakajima, S., 1954, Proceedings of the International Conference on Theoretical Physics at Kyoto-Tokyo (Science Council of Japan). Nambu, Y., 1960, “Quasi-particles and gauge invariance in the theory of superconductivity,” Phys. Rev. 117, 648–663. Nery, J. P., and P. B. Allen, 2016, “Influence of Fröhlich polaron coupling on renormalized electron bands in polar semiconductors: Results for zinc-blende GaN,” Phys. Rev. B 94, 115135. Noffsinger, J., F. Giustino, S. G. Louie, and M. L. Cohen, 2009, “Origin of superconductivity in boron-doped silicon carbide from first principles,” Phys. Rev. B 79, 104511. Noffsinger, J., F. Giustino, B. D. Malone, C.-H. Park, S. G. Louie, and M. L. Cohen, 2010, “EPW: A program for calculating the electron-phonon coupling using maximally localized wannier functions,” Comput. Phys. Commun. 181, 2140–2148. 015003-60 Feliciano Giustino: Electron-phonon interactions from first … Noffsinger, J., E. Kioupakis, C. G. Van de Walle, S. G. Louie, and M. L. Cohen, 2012, “Phonon-assisted optical absorption in silicon from first principles,” Phys. Rev. Lett. 108, 167402. Nordheim, L., 1931, “Zur Elektronentheorie der Metalle. I,” Ann. Phys. (Berlin) 401, 607–640. Olguín, D., M. Cardona, and A. Cantarero, 2002, “Electron-phonon effects on the direct band gap in semiconductors: LCAO calculations,” Solid State Commun. 122, 575–589. Onida, G., L. Reining, and A. Rubio, 2002, “Electronic excitations: density-functional versus many-body Green’s-function approaches,” Rev. Mod. Phys. 74, 601–659. Ortmann, F., F. Bechstedt, and K. Hannewald, 2009, “Theory of charge transport in organic crystals: Beyond Holstein’s smallpolaron model,” Phys. Rev. B 79, 235206. Park, C.-H., N. Bonini, T. Sohier, G. Samsonidze, B. Kozinsky, M. Calandra, F. Mauri, and N. Marzari, 2014, “Electron-phonon interactions and the intrinsic electrical resistivity of graphene,” Nano Lett. 14, 1113–1119. Park, C.-H., F. Giustino, M. L. Cohen, and S. G. Louie, 2007, “Velocity renormalization and carrier lifetime in graphene from the electron-phonon interaction,” Phys. Rev. Lett. 99, 086804. Park, C.-H., F. Giustino, M. L. Cohen, and S. G. Louie, 2008, “Electron-phonon interactions in graphene, bilayer graphene, and graphite,” Nano Lett. 8, 4229–4233. Park, C.-H., F. Giustino, J. L. McChesney, A. Bostwick, T. Ohta, E. Rotenberg, M. L. Cohen, and S. G. Louie, 2008, “Van Hove singularity and apparent anisotropy in the electron-phonon interaction in graphene,” Phys. Rev. B 77, 113410. Park, C.-H., F. Giustino, C. D. Spataru, M. L. Cohen, and S. G. Louie, 2009, “Angle-resolved photoemission spectra of graphene from first-principles calculations,” Nano Lett. 9, 4234–4239. Parr, R. G., and W. Yang, 1994, Density-functional theory of atoms and molecules (Oxford University Press, New York). Patrick, C. E., and F. Giustino, 2013, “Quantum nuclear dynamics in the photophysics of diamondoids,” Nat. Commun. 4, 2006. Patrick, C. E., and F. Giustino, 2014, “Unified theory of electronphonon renormalization and phonon-assisted optical absorption,” J. Phys. Condens. Matter 26, 365503. Patrick, C. E., K. W. Jacobsen, and K. S. Thygesen, 2015, “Anharmonic stabilization and band gap renormalization in the perovskite CsSnI3 ,” Phys. Rev. B 92, 201205. Peelaers, H., E. Kioupakis, and C. G. Van de Walle, 2015, “Freecarrier absorption in transparent conducting oxides: Phonon and impurity scattering in SnO2 ,” Phys. Rev. B 92, 235201. Pekar, S. I., 1946, “Autolocalization of an electron in a dielectric inertially polarizing medium,” Zh. Eksp. Teor. Fiz. 16, 335–340. Perdew, J. P., K. Burke, and M. Ernzerhof, 1996, “Generalized gradient approximation made simple,” Phys. Rev. Lett. 77, 3865–3868. Perdew, J. P., M. Ernzerhof, and K. Burke, 1996, “Rationale for mixing exact exchange with density functional approximations,” J. Chem. Phys. 105, 9982–9985. Perdew, J. P., and Alex Zunger, 1981, “Self-interaction correction to density-functional approximations for many-electron systems,” Phys. Rev. B 23, 5048–5079. Perroni, C. A., E. Piegari, M. Capone, and V. Cataudella, 2004, “Polaron formation for nonlocal electron-phonon coupling: A variational wave-function study,” Phys. Rev. B 69, 174301. Phillips, J. C., 1958, “Energy-band interpolation scheme based on a pseudopotential,” Phys. Rev. 112, 685–695. Phillips, J. C., and L. Kleinman, 1959, “New method for calculating wave functions in crystals and molecules,” Phys. Rev. 116, 287–294. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Pick, R. M., M. H. Cohen, and R. M. Martin, 1970, “Microscopic theory of force constants in the adiabatic approximation,” Phys. Rev. B 1, 910–920. Pines, D., and D. Bohm, 1952, “A collective description of electron interactions: II. collective vs individual particle aspects of the interactions,” Phys. Rev. 85, 338–353. Pisana, S., M. Lazzeri, C. Casiraghi, K. S. Novoselov, A. K. Geim, A. C. Ferrari, and F. Mauri, 2007, “Breakdown of the adiabatic Born-Oppenheimer approximation in graphene,” Nat. Mater. 6, 198–201. Piscanec, S., M. Lazzeri, J. Robertson, A. C. Ferrari, and F. Mauri, 2007, “Optical phonons in carbon nanotubes: Kohn anomalies, peierls distortions, and dynamic effects,” Phys. Rev. B 75, 035427. Pizzi, G., D. Volja, B. Kozinsky, M. Fornari, and N. Marzari, 2014, “BoltzWann: A code for the evaluation of thermoelectric and electronic transport properties with a maximally-localized Wannier functions basis,” Comput. Phys. Commun. 185, 422–429. Poncé, S., G. Antonius, P. Boulanger, E. Cannuccia, A. Marini, M. Côté, and X. Gonze, 2014, “Verification of first-principles codes: Comparison of total energies, phonon frequencies, electronphonon coupling and zero-point motion correction to the gap between ABINIT and QE/Yambo,” Comput. Mater. Sci. 83, 341–348. Poncé, S., G. Antonius, Y. Gillet, P. Boulanger, J. Laflamme Janssen, A. Marini, M. Côté, and X. Gonze, 2014, “Temperature dependence of electronic eigenenergies in the adiabatic harmonic approximation,” Phys. Rev. B 90, 214304. Poncé, S., Y. Gillet, J. Laflamme Janssen, A. Marini, M. Verstraete, and X. Gonze, 2015, “Temperature dependence of the electronic structure of semiconductors and insulators,” J. Chem. Phys. 143, 102813. Poncé, S., E. R. Margine, C. Verdi, and F. Giustino, 2016, “EPW: Electron-phonon coupling, superconducting and transport properties using maximally localized wannier functions,” Comput. Phys. Commun. 209, 116–133. Prange, R. E., and L. P. Kadanoff, 1964, “Transport theory for electron-phonon interactions in metals,” Phys. Rev. 134, A566–A580. Prendergast, D., and S. G. Louie, 2009, “Bloch-state-based interpolation: An efficient generalization of the Shirley approach to interpolating electronic structure,” Phys. Rev. B 80, 235126. Profeta, G., C. Franchini, N. N. Lathiotakis, A. Floris, A. Sanna, M. A. L. Marques, M. Lüders, S. Massidda, E. K. U. Gross, and A. Continenza, 2006, “Superconductivity in lithium, potassium, and aluminum under extreme pressure: A first-principles study,” Phys. Rev. Lett. 96, 047003. Quong, A. A., and B. M. Klein, 1992, “Self-consistent-screening calculation of interatomic force constants and phonon dispersion curves from first principles,” Phys. Rev. B 46, 10734–10737. Ralph, H. I., 1970, “Theoretical phonon limited electron mobility in silicon,” Solid State Commun. 8, 1095–1098. Ramírez, R., C. P. Herrero, and E. R. Hernández, 2006, “Path-integral molecular dynamics simulation of diamond,” Phys. Rev. B 73, 245202. Ramírez, R., C. P. Herrero, E. R. Hernández, and M. Cardona, 2008, “Path-integral molecular dynamics simulation of 3C − SiC,” Phys. Rev. B 77, 045210. Resta, R., 1994, “Macroscopic polarization in crystalline dielectrics: the geometric phase approach,” Rev. Mod. Phys. 66, 899–915. Restrepo, O. D., K. E. Krymowski, J. Goldberger, and W. Windl, 2014, “A first principles method to simulate electron mobilities in 2D materials,” New J. Phys. 16, 105009. 015003-61 Feliciano Giustino: Electron-phonon interactions from first … Restrepo, O. D., K. Varga, and S. T. Pantelides, 2009, “Firstprinciples calculations of electron mobilities in silicon: Phonon and coulomb scattering,” Appl. Phys. Lett. 94, 212103. Richter, W., 1984, “Coupled plasmon-polar phonon modes in semiconductors: Spatial dispersion and other properties,” in Polarons and Excitons in Polar Semiconductors and Ionic Crystals, Vol. 127, edited by J. T. Devreese and F. Peeters (Springer, New York), pp. 209–243. Rickayzen, G., 1980, Green’s Functions and Condensed Matter, Techniques of Physics (Academic, New York). Ridley, B. K., 1993, Quantum Processes in Semiconductors (Clarendon, Oxford). Rösch, O., and O. Gunnarsson, 2004, “Electron-phonon interaction in the t-J model,” Phys. Rev. Lett. 92, 146403. Saito, M., 2002, “Electron-phonon coupling of electron- or holeinjected C60 ,” Phys. Rev. B 65, 220508. Saitta, A. M., M. Lazzeri, M. Calandra, and F. Mauri, 2008, “Giant nonadiabatic effects in layer metals: Raman spectra of intercalated graphite explained,” Phys. Rev. Lett. 100, 226401. Sangalli, D., and A. Marini, 2015a, “Complete collisions approximation to the Kadanoff-Baym equation: a first-principles implementation,” J. Phys. Conf. Ser. 609, 012006. Sangalli, D., and A. Marini, 2015b, “Ultra-fast carriers relaxation in bulk silicon following photo-excitation with a short and polarized laser pulse,” Europhys. Lett. 110, 47004. Sanna, A., C. Franchini, A. Floris, G. Profeta, N. N. Lathiotakis, M. Lüders, M. A. L. Marques, E. K. U. Gross, A. Continenza, and S. Massidda, 2006, “Ab initio prediction of pressure-induced superconductivity in potassium,” Phys. Rev. B 73, 144512. Sanna, A., S. Pittalis, J. K. Dewhurst, M. Monni, S. Sharma, G. Ummarino, S. Massidda, and E. K. U. Gross, 2012, “Phononic self-energy effects and superconductivity in CaC6 ,” Phys. Rev. B 85, 184514. Sanna, A., G. Profeta, A. Floris, A. Marini, E. K. U. Gross, and S. Massidda, 2007, “Anisotropic gap of superconducting CaC6 : A first-principles density functional calculation,” Phys. Rev. B 75, 020511. Sano, W., T. Koretsune, T. Tadano, R. Akashi, and R. Arita, 2016, “Effect of Van Hove singularities on high-T c superconductivity in H3 S,” Phys. Rev. B 93, 094525. Savini, G., A. C. Ferrari, and F. Giustino, 2010, “First-principles prediction of doped graphane as a high-temperature electronphonon superconductor,” Phys. Rev. Lett. 105, 037002. Savrasov, S. Y., 1992, “Linear response calculations of lattice dynamics using muffin-tin basis sets,” Phys. Rev. Lett. 69, 2819–2822. Savrasov, S. Y., and G. Kotliar, 2003, “Linear response calculations of lattice dynamics in strongly correlated systems,” Phys. Rev. Lett. 90, 056401. Savrasov, S. Y., D. Y. Savrasov, and O. K. Andersen, 1994, “Linearresponse calculations of electron-phonon interactions,” Phys. Rev. Lett. 72, 372–375. Scalapino, D. J., 1969, The Electron-Phonon Interaction and StrongCoupling Superconductors, edited by R. D. Parks, Superconductivity, Vol. 1 (Dekker). Schäfer, W., and M. Wegener, 2002, Semiconductor Optics and Transport Phenomena, Advanced Texts in Physics (Springer, New York). Schrieffer, J. R., 1983, Theory of Superconductivity, Advanced Book Program Series (Perseus). Schwinger, J., 1951, “On the Green’s functions of quantized fields. I,” Proc. Natl. Acad. Sci. U.S.A. 37, 452–455. Sham, L. J., 1961, “Electron-phonon interaction by the method of pseudo-potentials,” Proc. Phys. Soc. London 78, 895. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Sham, L. J., and J. M. Ziman, 1963, Effects of electron-electron and electron-phonon interactions on the one-electron states of solids, edited by F. Seitz and D. Turnbull, Solid State Physics, Vol. 15 (Academic, New York). Shockley, W., and J. Bardeen, 1950, “Energy bands and mobilities in monatomic semiconductors,” Phys. Rev. 77, 407–408. Shuey, R. T., 1965, “Electron-phonon interaction for indirect interband transitions in germanium,” Phys. Rev. 139, A1675–A1684. Shukla, A., et al., 2003, “Phonon dispersion and lifetimes in MgB2 ,” Phys. Rev. Lett. 90, 095506. Sjakste, J., N. Vast, M. Calandra, and F. Mauri, 2015, “Wannier interpolation of the electron-phonon matrix elements in polar semiconductors: Polar-optical coupling in GaAs,” Phys. Rev. B 92, 054307. Sjakste, J., N. Vast, and V. Tyuterev, 2007, “Ab initio method for calculating electron-phonon scattering times in semiconductors: Application to GaAs and GaP,” Phys. Rev. Lett. 99, 236405. Sjölander, A., and R. Johnson, 1965, Proceedings of the International Conference on Inelastic Scattering of Neutrons, Bombay, 1964 (IAEA Proceedings Series) Vol. 1, pp. 61–76. Sklyadneva, I. Yu., E. V. Chulkov, W.-D. Schöne, V. M. Silkin, R. Keyling, and P. M. Echenique, 2005, “Role of electron-phonon interactions versus electron-electron interactions in the broadening mechanism of the electron and hole linewidths in bulk Be,” Phys. Rev. B 71, 174302. Sklyadneva, I. Yu., A. Leonardo, P. M. Echenique, S. V. Eremeev, and E. V. Chulkov, 2006, “Electron-phonon contribution to the phonon and excited electron (hole) linewidths in bulk Pd,” J. Phys. Condens. Matter 18, 7923. Sohier, T., M. Calandra, C.-H. Park, N. Bonini, N. Marzari, and F. Mauri, 2014, “Phonon-limited resistivity of graphene by firstprinciples calculations: Electron-phonon interactions, straininduced gauge field, and boltzmann equation,” Phys. Rev. B 90, 125414. Souza, I., N. Marzari, and D. Vanderbilt, 2001, “Maximally localized Wannier functions for entangled energy bands,” Phys. Rev. B 65, 035109. Sternheimer, R. M., 1954, “Electronic polarizabilities of ions from the Hartree-Fock wave functions,” Phys. Rev. 96, 951–968. Story, S. M., J. J. Kas, F. D. Vila, M. J. Verstraete, and J. J. Rehr, 2014, “Cumulant expansion for phonon contributions to the electron spectral function,” Phys. Rev. B 90, 195135. Su, W. P., J. R. Schrieffer, and A. J. Heeger, 1979, “Solitons in polyacetylene,” Phys. Rev. Lett. 42, 1698–1701. Troullier, N., and J. L. Martins, 1991, “Efficient pseudopotentials for plane-wave calculations,” Phys. Rev. B 43, 1993–2006. Tyuterev, V. G., S. V. Obukhov, N. Vast, and J. Sjakste, 2011, “Ab initio calculation of electron-phonon scattering time in germanium,” Phys. Rev. B 84, 035201. Valla, T., A. V. Fedorov, P. D. Johnson, and S. L. Hulbert, 1999, “Many-body effects in angle-resolved photoemission: Quasiparticle energy and lifetime of a Mo(110) surface state,” Phys. Rev. Lett. 83, 2085–2088. Valla, T., A. V. Fedorov, P. D. Johnson, B. O. Wells, S. L. Hulbert, Q. Li, G. D. Gu, and N. Koshizuka, 1999, “Evidence for quantum critical behavior in the optimally doped cuprate Bi2 Sr2 CaCu2 O8þδ ,” Science 285, 2110–2113. Vanderbilt, D., 1990, “Soft self-consistent pseudopotentials in a generalized eigenvalue formalism,” Phys. Rev. B 41, 7892–7895. van Leeuwen, R., 2004, “First-principles approach to the electronphonon interaction,” Phys. Rev. B 69, 115110. Varga, B. B., 1965, “Coupling of plasmons to polar phonons in degenerate semiconductors,” Phys. Rev. 137, A1896–A1902. 015003-62 Feliciano Giustino: Electron-phonon interactions from first … Varshni, Y. P., 1967, “Temperature dependence of the energy gap in semiconductors,” Physica (Utrecht) 34, 149–154. Verdi, C., F. Caruso, and F. Giustino, 2017, “Origin of the crossover from polarons to Fermi liquids in transition metal oxides” (unpublished). Verdi, C., and F. Giustino, 2015, “Fröhlich electron-phonon vertex from first principles,” Phys. Rev. Lett. 115, 176401. Verstraete, M. J., M. Torrent, F. Jollet, Z. Gilles, and X. Gonze, 2008, “Density functional perturbation theory with spin-orbit coupling: Phonon band structure of lead,” Phys. Rev. B 78, 045119. Villegas, C. E. P., A. R. Rocha, and A. Marini, 2016, “Anomalous temperature dependence of the band gap in black phosphorus,” Nano Lett. 16, 5095–5101. Vogl, P., 1976, “Microscopic theory of electron-phonon interaction in insulators or semiconductors,” Phys. Rev. B 13, 694–704. von Barth, U., and L. Hedin, 1972, “A local exchange-correlation potential for the spin polarized case. I,” J. Phys. C 5, 1629. Vukmirović, N., C. Bruder, and V. M. Stojanović, 2012, “Electronphonon coupling in crystalline organic semiconductors: Microscopic evidence for nonpolaronic charge carriers,” Phys. Rev. Lett. 109, 126407. Walker, C. T., and G. A. Slack, 1970, “Who named the ON’s?,” Am. J. Phys. 38, 1380–1389. Walter, J. P., R. R. L. Zucca, M. L. Cohen, and Y. R. Shen, 1970, “Temperature dependence of the wavelength-modulation spectra of GaAs,” Phys. Rev. Lett. 24, 102–104. Wang, X., D. Vanderbilt, J. R. Yates, and I. Souza, 2007, “Fermisurface calculation of the anomalous hall conductivity,” Phys. Rev. B 76, 195109. Wang, X., J. R. Yates, I. Souza, and D. Vanderbilt, 2006, “Ab initio calculation of the anomalous Hall conductivity by Wannier interpolation,” Phys. Rev. B 74, 195118. Wang, Z., S. Wang, S. Obukhov, N. Vast, J. Sjakste, V. Tyuterev, and N. Mingo, 2011, “Thermoelectric transport properties of silicon: Toward an ab initio approach,” Phys. Rev. B 83, 205208. Wang, Z., et al., 2016, “Tailoring the nature and strength of electronphonon interactions in the SrTiO3 ð001Þ 2D electron liquid,” Nat. Mater. 15, 835–839. Wannier, G. H., 1937, “The structure of electronic excitation levels in insulating crystals,” Phys. Rev. 52, 191–197. Williams, F. E., 1951, “Theoretical low temperature spectra of the thallium activated potassium chloride phosphor,” Phys. Rev. 82, 281–282. Wiser, N., 1963, “Dielectric constant with local field effects included,” Phys. Rev. 129, 62–69. Rev. Mod. Phys., Vol. 89, No. 1, January–March 2017 Wright, A. D., C. Verdi, R. L. Milot, G. E. Eperon, M. A. PérezOsorio, H. J. Snaith, F. Giustino, M. B. Johnston, and L. M. Herz, 2016, “Electron-phonon coupling in hybrid lead halide perovskites,” Nat. Commun. 7, 11755. Xu, B., and M. J. Verstraete, 2014, “First principles explanation of the positive Seebeck coefficient of lithium,” Phys. Rev. Lett. 112, 196603. Yates, J. R., X. Wang, D. Vanderbilt, and I. Souza, 2007, “Spectral and Fermi surface properties from Wannier interpolation,” Phys. Rev. B 75, 195121. Yin, M. T., and M. L. Cohen, 1982, “Ab initio calculation of the phonon dispersion relation: Application to Si,” Phys. Rev. B 25, 4317–4320. Yin, Z. P., A. Kutepov, and G. Kotliar, 2013, “Correlation-enhanced electron-phonon coupling: Applications of GW and screened hybrid functional to bismuthates, chloronitrides, and other highT c superconductors,” Phys. Rev. X 3, 021011. Yu, P. Y., and M. Cardona, 2010, Fundamentals of Semiconductors (Springer, New York), 4th ed. Zacharias, M., and F. Giustino, 2016, “One-shot calculation of temperature-dependent optical spectra and phonon-induced bandgap renormalization,” Phys. Rev. B 94, 075125. Zacharias, M., C. E. Patrick, and F. Giustino, 2015, “Stochastic approach to phonon-assisted optical absorption,” Phys. Rev. Lett. 115, 177401. Zhang, P., S. G. Louie, and M. L. Cohen, 2007, “Electron-phonon renormalization in cuprate superconductors,” Phys. Rev. Lett. 98, 067005. Zheng, J.-J., and E. R. Margine, 2016, “First-principles calculations of the superconducting properties in Li-decorated monolayer graphene within the anisotropic Migdal-Eliashberg formalism,” Phys. Rev. B 94, 064509. Zhou, J. S., J. J. Kas, L. Sponza, I. Reshetnyak, M. Guzzo, C. Giorgetti, M. Gatti, F. Sottile, J. J. Rehr, and L. Reining, 2015, “Dynamical effects in electron spectroscopy,” J. Chem. Phys. 143, 184109. Zhou, S. Y., G.-H. Gweon, A. V. Fedorov, P. N. First, W. A. De Heer, D.-H. Lee, F. Guinea, A. H. Castro Neto, and A. Lanzara, 2007, “Substrate-induced bandgap opening in epitaxial graphene,” Nat. Mater. 6, 770–775. Ziman, J. M., 1960, Electrons and phonons: the theory of transport phenomena in solids (Clarendon, Oxford). Zollner, S., M. Cardona, and S. Gopalan, 1992, “Isotope and temperature shifts of direct and indirect band gaps in diamondtype semiconductors,” Phys. Rev. B 45, 3376–3385. 015003-63